2.
98 V. I. Kushch
Maxwell [57] who deﬁned them as the complex point charges and studied the
relationship between the potential ﬁelds of multipoles and spherical harmonics.
To avoid confusing, the notions “multipole” (point source), “multipole ﬁeld” (poten-
tial) and “multipole moment” (strength) should be clearly distinguished. Among sev-
eral available in literature deﬁnitions, the most general one, probably,
is [25]:
“...A multipole expansion is a series expansion of the effect produced by a
given system in terms of an expansion parameter which becomes small as the
distance away from the system increases”.
The basis functions and the expansion coefﬁcients are referred as the potential
ﬁelds and moments (strengths) of multipoles, respectively. What is important, this
deﬁnition imposes no restrictions on the basis functions and, in what follows, we
accept it.
By tradition, we call the method exposed in this Chapter the Multipole Expan-
sion Method (MEM) despite the fact that multipole expansion is only a part of
solution procedure. The basic idea of the method consists in reducing the boundary
value problem stated on the piece-homogeneous domain to the ordinary system of
linear algebraic equations. In so doing, a considerable analytical effort involving
the mathematical physics and theory of special functions is required. This effort is
quite rewarding, in view of the obtained this way remarkably simple and efﬁcient
computational algorithms.
MEM is essentially the series method, where the partial solutions of differential
equation obtained by separation of variables in an appropriate coordinate system
constitute a countable set of basis functions. The speciﬁc curvilinear coordinate
system is dictated by the inclusion shape and introduced in a way that the matrix-
inclusion interface coincides with the coordinate surface. An important for our study
feature of the basis functions is that at this coordinate surface they form a full and
orthogonal set of surface harmonics and thus provide an efﬁcient way of fulﬁlling
the interface boundary conditions.
In this Chapter, we review the work done for the scalar (conductivity) and vec-
torial (linear elasticity) problems. Two matrix type composites under study are (a)
particulate composites with spherical and spheroidal inclusions and (b) unidirec-
tional ﬁbrous composite materials with circular and elliptic (in cross-section) ﬁbers.
The isotropic as well as anisotropic properties of constituents are considered. The
review is structured as follows.
The homogenization problem, in particular, the rational way of introducing the
macro parameters and effective properties of composite is brieﬂy discussed in Sect.1.
The general formulas for the macroscopic ﬂux vector and stress tensor are derived
in terms of corresponding average gradient ﬁelds and dipole moments (stresslets) of
the disturbance ﬁelds, i.e., in the form most appropriate for the multipole expansion
approach.
3.
Multipole Expansion Method in Micromechanics of Composites 99
In Sect.2, we consider the Multipole Expansion Method in application to con-
ductivity of composite with spherical inclusions as the most widely used and
traditionally associated with multipoles geometry. This problem is well explored
and we revisit it with aim to demonstrate the basic technique of the method
and discuss the principal moments. In the subsequent Sections, the Multipole
Expansion Method is applied to the elasticity problem as well as expanded on
the composites with more complicated geometry of inclusions and properties of
constituents.
All the Sections are structured uniformly, in accordance with the MEM solution
ﬂow. We begin with the problem for a single inclusion, immersed in non-uniform
far ﬁeld. These results, on the one hand, provide a necessary background for the
subsequent study. On the other hand, they can be viewed as the generalized Eshelby’s
model expanded on the case of non-uniform far load—but still readily implanted in
that or another self-consistent scheme.
Next, the Finite Cluster Model (FCM) is considered. To obtain an accurate solu-
tion of the multiple inclusion problem, the above solution for a single inclusion
is combined with the superposition principle and the re-expansion formulas for a
given geometry of inclusion. These results constitute the intermediate, second step
of the method and will be further developed in order to obtain the full-featured
model of composite. At the same time, this model can be viewed as the gen-
eralized Maxwell’s model, where the particle-particle interactions are taken into
account.
Then, the Representative Unit Cell (RUC) model of composite is studied. Here,
the periodic solutions and corresponding lattice sums are introduced. A complete
solution of the model provides a detailed analysis of the local ﬁelds, their ana-
lytical integration gives the exact, only dipole moments containing expressions
of the effective conductivity and elasticity tensors.This model can be viewed as
the generalized Rayleigh’s model expanded on the general type geometry (both
regular and random) of composite, with an adequate account for the interaction
effects.
1 Homogenization Problem
The homogenization problem is in the focus of the composite mechanics for the
last 50years. The various aspects of this problem including (a) structure levels, (c)
representative volume element (RVE) size and shape, (b) way of introducing the
macro parameters and effective properties of composite, etc., were widely discussed
in several books and thousands of papers. Our aim is more limited and speciﬁc: here,
we will discuss how the multipole expansion solutions apply to the homogenization
problem.
4.
100 V. I. Kushch
1.1 Conductivity
1.1.1 Deﬁnition of Macroscopic Quantities: Volume Versus
Surface Averaging
The macroscopic, or effective, conductivity tensor ∗
= λ∗
i j is deﬁned by the
Fourier law:
q = − ∗
· ∇T . (1.1)
In (1.1), ∇T and q are the macroscopic temperature gradient and heat ﬂux vector,
respectively. Their introduction is not as self-obvious and the researchers are not
unanimous in this matter. In most publications, ∇T and q are taken as the volume-
averaged values of corresponding local ﬁelds:
∇T =
1
V V
∇T dV ; q =
1
V V
qdV ; (1.2)
where V is a volume of the representative volume element (RVE) of composite solid.
For the matrix type composite we consider, V = N
q=0 Vq, Vq being the volume
of qth inclusion and V0 being the matrix volume inside RVE. An alternate, surface
averaging-based deﬁnition of the macroscopic conductivity parameters is [90]:
∇T =
1
V S0
T ndS, q =
1
V S0
(q · n) rdS. (1.3)
It is instructive to compare these two deﬁnitions. We employ the gradient theorem
[64] to write
1
V V
∇T dV =
1
V S0
T (0)
ndS +
1
V
N
q=1 Sq
T (q)
− T (0)
ndS, (1.4)
where Sq is the surface of Vq, S0 is the outer surface of RVE and n is the unit normal
vector. As seen from (1.4), the compared formulas coincide only if temperature is
continuous T (0) = T (q) at the interface. Noteworthy, (1.3) holds true for com-
posites with imperfect interfaces whereas (1.2) obviously not. On order to compare
two deﬁnitions of q , we employ the identity q = ∇ · q ⊗ r and the divergence
theorem [64] to get
1
V V
qdV =
1
V S0
q(0)
· n rdS
+
1
V
N
q=1 Sq
q(q)
· n − q(0)
· n rdS.
5.
Multipole Expansion Method in Micromechanics of Composites 101
Again, two deﬁnitions coincide only if the normal ﬂux qn = q · n is continuous
across the interface—and again Eq.(1.3) holds true for composites with imperfect
interfaces.
Thus, (1.2) is valid only for the composites with perfect thermal contact between
the constituents. The deﬁnition (1.3) is advantageous at least in the following aspects:
• It involves only the observable quantities—temperature and ﬂux—at the surface of
composite specimen. In essence, we consider RVE as a “black box” whose interior
structure may affect numerical values of the macro parameters—but not the way
they were introduced.
• This deﬁnition is valid for composites with arbitrary interior microstructure and
arbitrary (not necessarily perfect) interface bonding degree as well as for porous
and cracked solids.
• Numerical simulation becomes quite similar to (and reproducible in) the exper-
imental tests where we apply the temperature drop (voltage, etc.) to the surface
of specimen and measure the heat ﬂux (current, etc.) passing the surface. Macro-
scopic conductivity of composite is then found as the output-to-input ratio. In
so doing, we have no need to study interior microstructure of composite and/or
perform volume averaging of the local ﬁelds.
1.1.2 Formula for Macroscopic Flux
Now, we derive the formula, particularly useful for the effective conductivity study
by the Multipole Expansion Method. We start with the generalized Green’s theorem
V
(uLv − vLu)dV =
S
u
∂v
∂M
− v
∂u
∂M
dS, (1.5)
where
Lu =
m
i, j=1
λi j
∂2u
∂xi ∂xj
,
∂u
∂M
=
m
i, j=1
λi j n j
∂u
∂xi
. (1.6)
In our context, m = 2 or 3. Physical meaning of the differential operators (1.6) is
clear from the formulas
Lu = ∇ · ( · ∇u) = −∇ · q(u);
∂u
∂M
= ( · ∇u) · n = −qn(u). (1.7)
WeapplyEqs.(1.5) and(1.7) tothematrixpart (V0) of RVE: withnoloss ingenerality,
we assume the outer boundary of RVE S0 entirely belonging to the matrix. In new
notations,
6.
102 V. I. Kushch
V0
T (0)
∇ · q T − T ∇ · q T (0)
dV
=
N
q=0 Sq
T (0)
qn T − T qn T (0)
dS, (1.8)
where T (0) is an actual temperature ﬁeld in matrix phase of composite and T is a trail
temperature ﬁeld obeying, as well as T (0), the energy conservation law ∇ ·q (T ) = 0
in every point of V0. Therefore, the volume integral in the left hand side of (1.8) is
identically zero.
In the right hand side of (1.8), we take T = xk and multiply by the Cartesian
unit vector ik to get
N
q=0 Sq
T (0)
0 · n + qn T (0)
r ds = 0,
where r = xkik is the radius-vector and n = nkik is the unit normal vector to the
surface Sq. In view of qn T (0) = q T (0) · n and (1.3), we come to the formula
q = − 0 · ∇T +
1
V
N
q=1 Sq
T (0)
qn r − qn(T (0)
)r ds, (1.9)
where we denote qn(r) = qn(xk)ik.
This formula is remarkable in several aspects.
• First, and most important, this equation together with (1.1) provide evaluation of
the effective conductivity tensor of composite solid. Using RUC as the represen-
tative volume enables further simpliﬁcation of Eq.(1.9).
• In derivation, no constraints were imposed on the shape of inclusions and inter-
face conditions. Therefore, (1.9) is valid for the composite with anisotropic con-
stituents and arbitrary matrix-to-inclusion interface shape, structure and bonding
type.
• Integrals in (1.9) involve only the matrix phase temperature ﬁeld, T (0). Moreover,
these integrals are identically zero for all but dipole term in the T (0) multipole
expansion in a vicinity of each inclusion and, in fact, represent contribution of
these inclusions to the overall conductivity tensor.
• In the Multipole Expansion Method, where temperature in the matrix is initially
taken in the form of multipole expansion, an analytical integration in (1.9) is
straightforward and yields the exact, ﬁnite form expressions for the effective
properties.
7.
Multipole Expansion Method in Micromechanics of Composites 103
1.2 Elasticity
The fourth rank effective elastic stiffness tensor C∗ = C∗
i jkl is deﬁned by
σ = C∗
: ε , (1.10)
where the macroscopic strain ε and stress σ tensors are conventionally deﬁned
as volume-averaged quantities:
ε =
1
V V
εdV ; σ =
1
V V
σdV. (1.11)
This deﬁnition is valid for the composites with perfect mechanical bonding—and
fails completely for the composites with imperfect interfaces. Also, this deﬁnition is
“conditionally” correct for the porous and cracked solids.
Analogous to (1.3) surface averaging-based deﬁnition of the macroscopic strain
and stress tensors [4]
ε =
1
2V S0
(n ⊗ u + u ⊗ n) dS; σ =
1
V S0
r ⊗ (σ · n) dS; (1.12)
resolves the problem. In the case of perfect interfaces, this deﬁnition agrees with the
conventional one, (1.11). This result is known in elastostatics as the mean strain the-
orem (e.g., [20]). Also, it follows from the mean stress theorem [20] that the volume
averaged σ in (1.11) is consistent with (1.12) in the case of perfect mechanical
contact between the matrix and inclusions. What is important for us, (1.12) holds
true for the composites with imperfect interfaces (e.g., [11]).
1.2.1 Formula for Macroscopic Stress
The Betti’s reciprocal theorem [20] written for the matrix domain V0 of RVE states
that the equality
N
q=0 Sq
Tn(u(0)
) · u − Tn(u ) · u(0)
dS = 0
is valid for any displacement vector u obeying the equilibrium equation
∇ · (C : ∇u) = 0. Following [44], we take it in the form ui j = ii xj . The dot
product Tn(u(0)) · ui j = σ
(0)
il nlxj and, by deﬁnition (1.12),
S0
Tn(u(0)
) · ui j dS = V σi j .
8.
104 V. I. Kushch
On the other hand,
Tn(ui j ) · u(0)
= σkl(ui j )nlu−
k = C
(0)
i jklnlu−
k ;
comparison with (1.12) gives us
1
V S0
Tn(ui j ) · u(0)
dS = C
(0)
i jkl εkl .
Thus, we come out with the formula
σi j = C
(0)
i jkl εkl +
1
V
N
q=1 Sq
Tn(u(0)
) · ui j − Tn(ui j ) · u(0)
dS (1.13)
consistent with [74].
The Eq.(1.13) is the counterpart of (1.9) in the elasticity theory and everything
said above with regard to (1.9) holds true for (1.13).
• This formula is valid for the composite with arbitrary (a) shape of disperse phase,
(b) anisotropy of elastic properties of constituents and (c) interface bonding type.
• Together with (1.10), (1.13) enables evaluation of the effective stiffness tensor of
composite provided the local displacement ﬁeld u(0) is known/found in some way.
• An yet another remarkable property of this formula consists in that the integral it
involves (stresslet, in [74] terminology) is non-zero only for the dipole term in the
vector multipole expansion of u(0).
2 Composite with Spherical Inclusions: Conductivity
Problem
The multipoles are usually associated with the spherical geometry, and the most work
in the multipoles theory have been done for this case. In particular, the conductiv-
ity problem for a composite with spherical inclusions has received much attention
starting from the pioneering works of Maxwell [57] and Rayleigh [73]. Now, this
problem has been thoroughly studied and we revisit it to illustrate the basic technique
of the method. To be speciﬁc, we consider thermal conductivity of composite. These
results apply also to the mathematically equivalent physical phenomena (electric
conductivity, diffusion, magnetic permeability, etc.).
9.
Multipole Expansion Method in Micromechanics of Composites 105
2.1 Background Theory
2.1.1 Spherical Harmonics
The spherical coordinates (r, θ, ϕ) relate the Cartesian coordinates (x1, x2, x3) by
x1 + ix2 = r sin θ exp(iϕ), x3 = r cos θ (r ≥ 0, 0 ≤ θ ≤ π, 0 ≤ ϕ < 2π).
(2.1)
Separation of variables in Laplace equation
ΔT (r) = 0 (2.2)
in spherical coordinates gives us a set of partial (“normal”, in Hobson’s [23] termi-
nology) solutions of the form
rt
Ps
t (cos θ) exp(isϕ) (−∞ < t < ∞, −t ≤ s ≤ t) (2.3)
referred [57] as scalar solid spherical harmonics of degree t and order s. Here, Ps
t are
the associate Legendre’s functions of ﬁrst kind [23]. With regard to the asymptotic
behavior, the whole set (2.3) is divided into two subsets: regular (inﬁnitely growing
with r → ∞) and singular (tending to zero with r → ∞) functions. We denote them
separately as
ys
t (r) =
rt
(t + s)!
χs
t (θ, ϕ); Ys
t (r) =
(t − s)!
rt+1
χs
t (θ, ϕ) (t ≥ 0, |s| ≤ t), (2.4)
respectively. In (2.4), χs
t are the scalar surface spherical harmonics
χs
t (θ, ϕ) = Ps
t (cos θ) exp(isϕ). (2.5)
They possess the orthogonality property
1
S S
χs
t χl
k dS = αtsδtkδsl, αts =
1
2t + 1
(t + s)!
(t − s)!
, (2.6)
where integral is taken over the spherical surface S; over bar means complex con-
jugate and δi j is the Kronecker’s delta. Adopted in (2.4) normalization is aimed to
simplify the algebra [29, 71]: so, we have
y−s
t (r) = (−1)sys
t (r), Y−s
t (r) = (−1)sYs
t (r). (2.7)
We mention also the differentiation rule [23]:
10.
106 V. I. Kushch
D1ys
t = ys−1
t−1 , D2ys
t = −ys+1
t−1 , D3ys
t = ys
t−1;
D1Ys
t = Ys−1
t+1 , D2Ys
t = −Ys+1
t+1 , D3Ys
t = −Ys
t+1;
(2.8)
or, in the compact form,
(D2)s
(D3)t−s 1
r
= (−1)t
Ys
t (r) (2.9)
where Di are the differential operators
D1 =
∂
∂x1
− i
∂
∂x2
, D2 = D1 =
∂
∂x1
+ i
∂
∂x2
, D3 =
∂
∂x3
. (2.10)
These operators can be viewed as the directional derivatives along the complex
Cartesian unit vectors ei deﬁned as
e1 = (i1 + ii1)/2, e2 = e1, e3 = i3. (2.11)
2.1.2 Spherical Harmonics Versus Multipole Potentials
Maxwell [57] has discovered the relationship between the solid spherical harmonics
(2.7) and the potential ﬁelds of multipoles. So, the potential surrounding a point
charge (being a singular point of zeroth order, or monopole) is 1/r = Y0
0 (r). The
ﬁrst order singular point, or dipole, is obtained by pushing two monopoles of equal
strength—but with opposite signs—toward each other. The potential of the dipole
to be given (up to rescaling) by the directional derivative ∇u1 (1/r), where u1 is the
direction along which the two monopoles approach one another. Similarly, pushing
together two dipoles with opposite signs gives (up to rescaling) a quadrupole with
potential ∇u1 ∇u2 (1/r), where u2 s the direction along which the dipoles approach,
and so on. In general, the multipole of order t is constructed with aid of 2t point
charges and has the potential proportional to ∇u1 ∇u2 . . . ∇ut (1/r). The latter can
be expanded into a weighted sum of 2t + 1 spherical harmonics of order t, i.e.,
Ys
t (r), −t ≤ s ≤ t. And, vise versa, Ys
t (r) can be written as ∇u1 ∇u2 . . . ∇ut (1/r)
provided the directions ui are taken in accordance with the formula (2.9). This is
why the series expansion in terms of solid spherical harmonics (2.7) is often referred
as the multipole expansion.
2.2 General Solution for a Single Inclusion
Let consider the regular, non-uniform temperature far ﬁeld Tf ar in unbounded
solid (matrix) of conductivity λ0. We insert a spherical inclusion of radius R and
11.
Multipole Expansion Method in Micromechanics of Composites 107
conductivity λ1 inclusion assuming that its presence does not alter the incident ﬁeld.
The inclusion causes local disturbance Tdis of temperature ﬁeld vanishing at inﬁnity
and depending, besides Tf ar , on the shape and size of inclusion, conductivities of
the matrix and inclusion materials and the matrix-inclusion bonding type. The tem-
perature ﬁeld T (T = T (0) in the matrix, T = T (1) in the inclusion) satisﬁes (2.2).
At the interface S (r = R), the perfect thermal contact is supposed:
[[T ]] = 0; [[qr ]] = 0; (2.12)
where [[ f ]] = ( f (0) − f (1))|r=R is a jump of quantity f through the interface S and
qn = −λ∇T · n is the normal heat ﬂux. Our aim is to determine the temperature in
and outside the inclusion.
2.2.1 Multipole Expansion Solution
The temperature ﬁeld in the inclusion T (1) is ﬁnite and hence its series expansion
contains the regular solutions ys
t (r) (2.4) only:
T (1)
(r) =
∞
t=0
t
s=−t
dtsys
t (r) (2.13)
where dts are the unknown coefﬁcients (complex, in general). Temperature is a real
quantity, so (2.7) leads to analogous relation between the series expansion coefﬁ-
cients: dt,−s = (−1)sdts. In accordance with physics of the problem, temperature
T (0) in the matrix domain is written as T (0) = Tf ar + Tdis, where Tdis(r) → 0 with
r → ∞. It means that Tdis series expansion contains the singular solutions Ys
t
only. So, we have
T (0)
(r) = Tf ar (r) +
∞
t=1
t
s=−t
AtsYs
t (r), (2.14)
where Ats are the unknown coefﬁcients. Again, At,−s = (−1)s Ats. The second,
series term in (2.14) is the multipole expansion of the disturbance ﬁeld Tdis.
2.2.2 Far Field Expansion
We consider Tf ar as the governing parameter. It can be prescribed either analytically
or in tabular form (e.g., obtained from numerical analysis). In fact, it sufﬁces to
know Tf ar values in the integration points at the interface S deﬁned by r = R. Due
to regularity of Tf ar in a vicinity of inclusion, its series expansion is analogous to
(2.13), with the another set of coefﬁcients cts. In view of (2.6), they are equal to
12.
108 V. I. Kushch
cts =
(t + s)!
4πR2αts S
Tf ar χs
t dS. (2.15)
For a given Tf ar , we can consider cts as the known values. Integration in (2.15) can
be done either analytically or numerically: in the latter case, the appropriate scheme
[42] comprises uniform distribution of integration points in azimuthal direction ϕ
with Gauss-Legendre formula [1] for integration with respect to θ.
2.2.3 Resolving Equations
The last step consists is substituting T (0) (2.14) and T (1) (2.13) into the bonding
conditions (2.12). From the ﬁrst, temperature continuity condition we get for r = R
∞
t=0
t
s=−t
cts
Rt
(t + s)!
χs
t (θ, ϕ) +
∞
t=1
t
s=−t
Ats
(t − s)!
Rt+1
χs
t (θ, ϕ) (2.16)
=
∞
t=0
t
s=−t
dts
Rt
(t + s)!
χs
t (θ, ϕ).
From here, for t = 0 (χ0
0 ≡ 1) we get immediately d00 = c00. For t = 0, in view of
χs
t orthogonality property (2.6), we come to a set of linear algebraic equations
(t − s)! (t + s)!
R2t+1
Ats + cts = dts. (2.17)
The second, normal ﬂux continuity condition gives us also
−
(t + 1)
t
(t − s)! (t + s)!
R2t+1
Ats + cts = ωdts, (2.18)
where ω = λ1/λ0. By eliminating dts from (2.17) to (2.18), we get the coefﬁ-
cients Ats:
(ω + 1 + 1/t)
(ω − 1)
(t − s)! (t + s)!
R2t+1
Ats = −cts; (2.19)
then, the dts coefﬁcients can be found from (2.17). The obtained general solution
is exact and, in the case of polynomial far ﬁeld, ﬁnite one.
2.3 Finite Cluster Model (FCM)
Now, we consider an unbounded solid containing a ﬁnite array of N spherical inclu-
sions of radius Rq and conductivity λq centered in the points Oq. In the (arbitrarily
13.
Multipole Expansion Method in Micromechanics of Composites 109
introduced) global Cartesian coordinate system Ox1x2x3, position of qth inclusion
is deﬁned by the vector Rq = X1qex1 + X2qex2 + X3qex3, q = 1, 2, . . . , N. Their
non-overlapping condition is Rpq > Rp + Rq, where the vector Rpq = Rq − Rp
gives relative position of pth and qth inclusions. We introduce the local, inclusion-
associated coordinate systems Ox1qx2qx3q with origins in Oq. The local variables
rp = r − Rp of different coordinate systems relate each other by rq = rp − Rpq.
2.3.1 Superposition Principle
A new feature of this problem consists in the following. Now, a given inclusion
undergoes a joint action of incident far ﬁeld and the disturbance ﬁelds caused by all
other inclusions. In turn, this inclusion affects the ﬁeld around other inclusions. This
means that the problem must be solved for all the inclusions simultaneously. For this
purpose, we apply the superposition principle widely used for tailoring the solution
of linear problem in the multiple-connected domain. This principle [81] states that
a general solution for the multiple-connected domain can be written as a
superposition sum of general solutions for the single-connected domains whose
intersection gives the considered multiple-connected domain.
The derived above general solution for a single-connected domain allows to write
a formal solution of the multiple inclusion problem. Moreover, the above exposed
integration based expansion procedure (2.15) provides a complete solution of the
problem. An alternate way consists in using the re-expansion formulas (referred
also as the addition theorems) for the partial solutions. This way does not involve
integration and appears more computationally efﬁcient. The re-expansion formulas
is the second component added to the solution procedure at this stage.
2.3.2 Re-Expansion Formulas
In notations (2.4), the re-expansion formulas for the scalar solid harmonics take the
simplest possible form. Three kinds of re-expansion formulas are: singular-to-regular
(S2R)
Ys
t (r + R) =
∞
k=0
k
l=−k
(−1)k+l
Ys−l
t+k (R)yl
k(r), r < R ; (2.20)
regular-to-regular (R2R)
ys
t (r + R) =
t
k=0
k
l=−k
ys−l
t−k(R)yl
k(r); (2.21)
14.
110 V. I. Kushch
and singular-to-singular (S2S)
Ys
t (r + R) =
∞
k=t
k
l=−k
(−1)t+k+s+l
ys−l
k−t (R)Yl
k(r), r > R . (2.22)
The formula (2.21) is ﬁnite and hence exact and valid for any r and R. In [77],
(2.21) and (2.22) are regarded as translation of regular and singular solid harmonics,
respectively. In [19], they are called translation of local and multipole expansions
whereas (2.20) is referred as conversion of a multipole expansion into a local one. The
formulas (2.20)–(2.22) can be derived in several ways, one of them based on using
the formula (2.15). Noteworthy, these formulas constitute a theoretical background
of the Fast Multipole Method [19].
2.3.3 Multipole Expansion Theorem
To illustrate the introduced concepts and formulas, we consider a standard problem
of the multipoles theory. Let N monopoles of strength qp are located at the points
Rp. We need to ﬁnd the multipole expansion of the total potential ﬁeld in the point
r where r > Rs and Rs = maxp Rp . In other words, we are looking for the
multipole expansion outside the sphere of radius Rs containing all the point sources.
Since the monopoles possess the ﬁxed strength and do not interact, the total
potential is equal to
T (r) =
N
p=1
qp
r − Rp
(2.23)
being a trivial case of the superposition sum. Next, by applying the formula (2.22)
for t = s = 0, namely,
1
r − Rp
= Y0
0 (r − Rp) =
∞
t=0
t
s=−t
ys
t (Rp)Ys
t (r), (2.24)
valid at r > Rs for all p, one ﬁnds easily
T (r) =
∞
t=0
t
s=−t
AtsYs
t (r), Ats =
N
p=1
qpys
t (Rp). (2.25)
For the truncated (t ≤ tmax) series (2.25), the following error estimate exists:
T (r) −
tmax
t=0
t
s=−t
AtsYs
t (r) ≤ A
(Rs/r)tmax+1
r − Rs
, A =
N
p=1
|qp|. (2.26)
15.
Multipole Expansion Method in Micromechanics of Composites 111
These results constitute the multipole expansion theorem [19]. The more involved
problem for the multiple ﬁnite-size, interacting inclusions is considered below.
2.4 FCM Boundary Value Problem
Let temperature ﬁeld T = T (0) in a matrix, T = T (p) in the pth inclusion of radius
Rp and conductivity λ = λp. On the interfaces rp = Rp, perfect thermal contact
(2.12) is supposed. Here, rp, θp, ϕp are the local spherical coordinates with the
origin Op in the center of the pth inclusion.
2.4.1 Direct (Superposition) Sum
In accordance with the superposition principle,
T (0)
(r) = Tf ar (r) +
N
p=1
T
(p)
dis (rp) (2.27)
where Tf ar = G · r = Gi xi is the linear far ﬁeld, and
T
(p)
dis (rp) =
∞
t=1
t
s=−t
A
(p)
ts Ys
t (rp) (2.28)
is a disturbance ﬁeld caused by pth inclusion centered in Op: T
(p)
dis (rp) → 0 with
rp → ∞.
2.4.2 Local Series Expansion
In a vicinity of Oq, the following expansions are valid:
Tf ar (rq) =
∞
t=0
t
s=−t
c
(q)
ts ys
t (rq), (2.29)
where c
(q)
00 = G · Rq, c
(q)
10 = G3, c
(q)
11 = G1 − iG2, c
(q)
1,−1 = −c
(q)
11 and c
(q)
ts = 0
otherwise. In (2.27), T
(q)
dis is already written in qth basis. For p = q, we apply the
re-expansion formula (2.20) to get
16.
112 V. I. Kushch
T
(p)
dis (rq) =
∞
t=0
t
s=−t
a
(q)
ts ys
t (rq), a
(q)
ts = (−1)t+s
N
p=q
∞
k=1
k
l=−k
A
(p)
kl Yl−s
k+t (Rpq).
(2.30)
By putting all the parts together, we get
T (0)
(rq) =
∞
t=1
t
s=−t
A
(q)
ts Ys
t (rq) +
∞
t=0
t
s=−t
a
(q)
ts + c
(q)
ts ys
t (rq) (2.31)
and the problem is reduced to the considered above single inclusion study.
2.4.3 Inﬁnite Linear System
By substituting T (0) (2.31) and T (q) (2.13) written in local coordinates into (2.12),
we come to the set of equations with unknowns A
(q)
ts , quite analogous to (2.17).
Namely,
(ωq + 1 + 1/t)
(ωq − 1)
(t − s)! (t + s)!
Rq
2t+1
A
(q)
ts + a
(q)
ts = −c
(q)
ts (ωq = λq/λ0); (2.32)
or, in an explicit form,
(ωq + 1 + 1/t)
(ωq − 1)
(t − s)! (t + s)!
Rq
2t+1
A
(q)
ts (2.33)
+ (−1)t+s
N
p=q
∞
k=1
k
l=−k
A
(p)
kl Yl−s
k+t (Rpq) = −c
(q)
ts .
A total number of unknowns in (2.33) can be reduced by a factor two by taking
account of A
(p)
k,−l = (−1)
l
A
(p)
kl .
The theoretical solution (2.33) we found is formally exact—but, in contrast to
(2.17), leads to the inﬁnite system of linear algebraic equations. The latter can be
solved, with any desirable accuracy, by the truncation method provided a sufﬁcient
number of harmonics (with t ≤ tmax) is retained in solution [17, 27]. Hence, the
numerical solution of the truncated linear system can be regarded as an asymp-
totically exact, because any accuracy can be achieved by the appropriate choice
of tmax. The smaller distance between the inhomogeneities is, the higher harmon-
ics must be retained in the numerical solution to ensure the same accuracy of
computations.
17.
Multipole Expansion Method in Micromechanics of Composites 113
2.4.4 Modiﬁed Maxwell’s Method for Effective Conductivity
Since we have A
(q)
ts found from (2.33), one can evaluate the temperature ﬁeld in
any point in and around the inclusions. Moreover, this model allows to evalu-
ate an effective conductivity of composite with geometry represented by FCM. In
fact, it was Maxwell [57] who ﬁrst suggested this model and derived his famous
formula by equating “the potential at a great distance from the sphere” (in fact, total
dipole moment) of an array of inclusions to that of the equivalent inclusion with
unknown effective conductivity. In so doing, Maxwell neglected interaction between
the inclusions—but wrote “...when the distance between the spheres is not great
compared with their radii..., then other terms enter into the result which we shall not
now consider.” Our solution contains all the terms and hence one can expect better
accuracy of the Maxwell’s formula. In our notations, it takes the form
λef f
λ0
=
1 − 2c A10
1 + c A10
, (2.34)
where λef f is the effective conductivity of composite with volume content c of
spherical inclusions, the mean dipole moment A10 = 1
N
N
p=1 A
(p)
10 and A
(p)
10 are
calculated from (2.33) for G3 = 1.
Recently, this approach was explored in [63]. The reported there numerical data
reveal that taking the interaction effects into account substantially improves an accu-
racy of (2.34). Among other FCM-related publications, we mention [26] and similar
works where an effective conductivity was estimated up to O(c2) from the “pair-of-
inclusions” model.
2.5 Representative Unit Cell Model
The third model we consider in our review is so-called “unit cell” model of
composite. Its basic idea consists in modeling an actual micro geometry of com-
posite by some periodic structure with a unit cell containing several inclusions. It
is known in literature as “generalized periodic”, or “quasi-random” model: in what
follows, we call it the Representative Unit Cell (RUC) model. This model is advan-
tageous in that it allows to simulate the micro structure of composite and, at the
same time, take the interactions of inhomogeneities over entire composite space into
account accurately. This makes the cell approach appropriate for studying the local
ﬁelds and effective properties of high-ﬁlled and strongly heterogeneous composites
where the arrangement and interactions between the inclusions substantially affects
the overall material behavior. RUC model can be applied to a wide class of compos-
ite structures and physical phenomena and, with a rapid progress in the computing
technologies, is gaining more and more popularity.
18.
114 V. I. Kushch
Noteworthy, this model stems from the famous work by Lord Rayleigh [73] who
considered “a medium interrupted by spherical obstacles arranged in rectangular
order” and has evaluated its effective conductivity by taking into account the dipole,
quadrupole and octupole moments of all inclusions. Almost a century later, the
complete multipole-type analytical solutions are obtained for three cubic arrays of
identical spheres [59, 60, 75, 82, 90]. In a series of more recent papers ([5, 29, 79,
88], among others), the conductivity problem for the random structure composite
was treated as a triple-periodic problem with random arrangement of particles in the
cubic unit cell.
2.5.1 RUC Geometry
The RUC model is essentially the above considered FCM model, periodically con-
tinued (replicated) in three orthogonal directions with period a, without overlapping
of any two inclusions. In fact, we consider an unbounded solid containing a number
N of periodic, equally oriented simple cubic (SC) arrays of inclusions. For a given
geometry, any arbitrarily placed, oriented along the principal axes of lattice cube
with side length a can be taken as RUC. It contains the centers of exactly N inclu-
sions, randomly (but without overlapping) placed within a cell. The inclusions may
partially lie outside the cube and, vise versa, a certain part of cube may be occupied
by the inclusions which do not belong to the cell, Fig.1a. Equally, one can take
the unit cell as a cuboid with curvilinear boundary (but parallel opposite faces): for
convenience, we assume with no loss in generality that the cell boundary S0 entirely
belongs to the matrix, see Fig.1b.
It should be noted that the model problem is formulated and solved for a whole
composite bulk rather than for the cube with plane faces. The RUC concept is nothing
more than convenient “gadget” for introducing the model geometry and averaging the
periodic strain and stress ﬁelds—and we use it for this purpose. We deﬁne geometry
of the cell by its side length a and position Rq = Xiqii of qth inclusion center
(a) (b)
Fig. 1 RUC model of composite
19.
Multipole Expansion Method in Micromechanics of Composites 115
(q = 1, 2, . . . , N) where ii are the unit axis vectors of the global Cartesian coordinate
system Ox1x2x3. Number N can be taken large sufﬁciently to simulate arrangement
of disperse phase in composite. We assume the inclusions equally sized, of radius
R, and made from the same material, their volume content is c = N 4
3 πR3/a3. In
what follows, the parameter Rpq = Rq − Rp is understood as the minimal distance
between the inclusions of pth and qth SC arrays.
Several methods ([79, 83, 89], among others) have been developed to generate the
random structure RUC statistically close to that of actual disordered composite. The
generated arrangement of particles, likewise the real composite micro structure, can
be characterized by several parameters: packing density, coordination number, radial
distribution function, nearest neighbor distance, etc. [7, 83]. Another parameter,
often introduced in this type models, is the minimum allowable spacing δmin =
minp,q( Rpq /2R−1) [9]. It is also known as impenetrability parameter, in terms of
the cherry-pit model [83]. A small positive value is usually assigned to this parameter
in order to separate inclusions and thus alleviate analysis of the model problem.
2.5.2 RUC Model Problem
The macroscopically uniform temperature ﬁeld in the composite bulk is considered.
This means constancy of the volume-averaged, or macroscopic, temperature gradient
∇T and heat ﬂux q vectors. Here and below, f = V −1
V f dV and V = a3 is
the cell volume; ∇T is taken as the load governing parameter. In this case, period-
icity of geometry results in quasi-periodicity of the temperature ﬁeld and periodicity
of the temperature gradient and heat ﬂux:
T (r + aii ) = T (r) + a ∇T · ii ; (2.35)
∇T (r + aii ) = ∇T (r) ; q (r + aii ) = q (r) .
2.5.3 Temperature Filed
The conditions (2.35) are satisﬁed by taking T in the form T (r) = ∇T ·r+Tdis (r),
Tdis being now the periodic disturbance ﬁeld. In the matrix domain, we write it as
a sum of linear mean ﬁeld and disturbances form the inﬁnite, periodic arrays of
particles:
T (0)
(r) = G · r +
N
p=1
T
∗(p)
dis (rp), (2.36)
The Eq.(2.36) is similar to (2.27), where the single inclusion disturbance terms T
(p)
dis
are replaced with their periodic counterparts given by the sums over all the lattice
nodes k = ki ii (−∞ < ki < ∞):
20.
116 V. I. Kushch
T
∗(p)
dis (rp) =
k
T
(p)
dis rp + ak , (2.37)
In view of (2.37) and (2.27), T
∗(p)
dis can be expressed in terms of the periodic harmonic
potentials Y∗
ts:
T
∗(p)
dis (rp) =
∞
t=1
t
s=−t
A
(p)
ts Y∗
ts(rp), where Y∗
ts(rp) =
k
Ys
t (rp + ak).
(2.38)
In fact, this is a direct formal extension of the FCM model when a number of
particles becomes inﬁnitely large—and, at the same time, direct extension of the
Rayleigh’s [73] approach. For almost a century, the Rayleigh’s solution was ques-
tioned due to conditional convergence of (2.38) for t = 1. The limiting process
has been legitimized by [59, 82] who resolved the convergence issue of dipole lat-
tice sums. An alternate, the generalized periodic functions based approach has been
applied by [75, 90]. In [15], the solution has been found in terms of doubly periodic
functions, in [88] the RUC problem was solved by the boundary integral method.
Not surprisingly, all the mentioned methods give the resulting sets of linear equations
consistent with
(ωq + 1 + 1
t )
(ωq − 1)
(t − s)!(t + s)!
Rq
2t+1
A
(q)
ts + (−1)t+s
N
p=1
∞
k=1
k
l=−k
A
(p)
kl Y∗
k+t,l−s(Rpq)
(2.39)
= −δt1 δs0G3 + δs1 (G1 − iG2) − δs,−1 (G1 + iG2) .
Among them, the multipole expansion method provides, probably, the most straight-
forward and transparent solution procedure. In fact, the system (2.39) is obtained
from (2.33) by replacing the matrix coefﬁcients Yl−s
k+t (Rpq) with the corresponding
lattice sums
Y∗
k+t,l−s(Rpq) =
k
Yl−s
k+t Rpq + ak . (2.40)
Convergence of the series (2.40) was widely discussed in literature and several fast
summation techniques have been developed for them ([17, 59, 88], among others)
and we refer there for the details.
As would be expected, the Y∗
ts deﬁnition (2.38) for t = 1 also suffers the above-
mentioned convergence problem. Indeed, obtained with aid of (2.20) the multipole
expansion
Y∗
1s(r) = Ys
1 (r) +
∞
k=0
k
l=−k
(−1)k+l
Y∗
k+1,s−l(R)yl
k(r) (2.41)
21.
Multipole Expansion Method in Micromechanics of Composites 117
also involves the conditionally convergent (“shape-dependent”) dipole lattice sum
Y∗
20(0). McPhedran et al. [59] have argued that the Rayleigh’s [73] result
Y∗
20(0) = 4π/3a3 is consistent with the physics of the problem. Alternatively, Y∗
1s(r)
can be deﬁned by means of periodic fundamental solution S1 [21] given by the triple
Fourier series. Speciﬁcally, we deﬁne
Y∗
10 = −D3 (S1) ; Y∗
11 = −Y∗
1,−1 = −D2 (S1) ; (2.42)
where Di are the differential operators (2.10). It appears that this deﬁnition is equiv-
alent to (2.41): differentiation of S1 multipole expansion [21] gives, in our notations,
D3 (S1) = −Y0
1 (r) +
4π
3a3
x3 −
∞
k=2
k
l=−k
(−1)k+l
Y∗
k+1,−l(0)yl
k(r). (2.43)
As expected, exactly the same result follows from the formula (2.41) where y0
1(r) is
replaced with x3 and Y∗
20(0)—with its numerical value, 4π/3a3.
2.5.4 Effective Conductivity
The second rank effective conductivity tensor Λ∗ = {λ∗
i j } is deﬁned by (1.1). In
order to evaluate λ∗
i j for a given composite, one has to conduct a series of numerical
tests, with three different ∇T , and evaluate the macroscopic heat ﬂux it causes.
Speciﬁcally, λ∗
i j = − qi for ∇T = ij , so we need an explicit expression of the
macroscopic temperature gradient and heat ﬂux corresponding to our temperature
solution (2.36).
Evaluation of the macroscopic gradient, ∇T is ready. First, we recall that we take
the unit cell of RUC with S0 ∈ V0 and, hence, T = T (0) in (1.3). Next, we observe
that for the periodic part of solution (2.36) in the boundary points ra ∈ S0 and
rb = ra+aij ∈ S0 belonging to the opposite cell faces we have Tdis (rb) = Tdis (ra)
whereas the normal unit vector changes the sign: n (rb) = −n (ra). Hence, the
integrals of Tdis over the opposite faces cancel each other and the total integral over
S0 equals to zero. Integration of the linear part of T (0) is elementary: the gradient
theorem yields
1
V S0
(G · r) ndS =
1
V V
∇ (G · r) dV = G. (2.44)
Comparison with (1.3) gives the expected ∇T = G provided T obeys (2.35).
22.
118 V. I. Kushch
This is general result: the derived formula is invariant of the shape, properties
andarrangement of inclusions, interfacebondingtypeandshapeof theunit cell.
In the subsequent Sections, this equality will be applied without derivation.
For q evaluation, we employ the formula (1.9). In the considered here isotropic
case, qn (r) = qn (xk) ik = −λ0n, it takes
q = − 0 · ∇T −
λ0
V
N
q=1 Sq
Rq
∂T (0)
∂rq
− T (0)
ndS. (2.45)
The unit vector n is expressed in terms of surface spherical harmonics as
n = χ1
1e2 − 2χ−1
1 e1 + χ0
1e3. whereas the local expansion of the integrand in right
hand side of (2.45) is given by
Rq
∂T (0)
∂rq
− T (0)
=
∞
t=0
t
s=−t
−(2t + 1)A
(q)
ts
(t − s)!
Rt+1
q
+(t − 1) a
(q)
ts + c
(q)
ts
Rt
q
(t + s)!
χs
t (θq, ϕq). (2.46)
Due to orthogonality of the surface spherical harmonics (2.6), the surface integral in
(2.45) equals to zero for all terms in Eq.(2.31) with t = 1. Moreover, r
∂ys
1
∂r = ys
1 and
hence only the dipole potentials Ys
1 contribute to (2.45). From here, we get the exact
ﬁnite formula involving only the dipole moments of the disturbance ﬁeld, A
(q)
1s :
q
λ0
= −G +
4π
a3
N
q=1
Re 2A
(q)
11 e1 + A
(q)
10 e3 . (2.47)
In view of (2.39), the coefﬁcients A
(q)
ts are linearly proportional to G:
λ0
4π
a3
N
q=1
Re 2A
(q)
11 e1 + A
(q)
10 e3 = δ · G. (2.48)
The components of the δ tensor are found by solving Eq.(2.39) for G = ij . These
equations, together with Eq.(1.1), provide evaluation of the effective conductivity
tensor as
∗
= 0 + δ . (2.49)
23.
Multipole Expansion Method in Micromechanics of Composites 119
3 Composite with Spherical Inclusions: Elasticity Problem
3.1 Background Theory
3.1.1 Vectorial Spherical Harmonics
Vectorial spherical harmonics S
(i)
ts = S
(i)
ts (θ, ϕ) are deﬁned as [64]
S(1)
ts = eθ
∂
∂θ
χs
t +
eϕ
sin θ
∂
∂ϕ
χs
t ; (3.1)
S
(2)
ts =
eθ
sin θ
∂
∂ϕ
χs
t − eϕ
∂
∂θ
χs
t ;
S
(3)
ts = er χs
t (t ≥ 0, |s| ≤ t).
The functions (3.1) constitute a complete and orthogonal on sphere set of vectorial
harmonics with the orthogonality properties given by
1
S S
S
(i)
ts · S
( j)
kl dS = α
(i)
ts δtkδslδi j , (3.2)
where α(1)
ts = α(2)
ts = t(t+1) αts and α(3)
ts = αts given by (2.6). Also, these functions
possess remarkable differential
r∇ · S
(1)
ts = −t(t + 1)χs
t ; ∇ · S
(2)
ts = 0; r∇ · S
(1)
ts = 2χs
t ; (3.3)
r∇ × S
(1)
ts = −S
(2)
ts ; r∇ × S
(2)
ts = S
(1)
ts + t(t + 1)S
(3)
ts ; r∇ × S
(3)
ts = S
(2)
ts ;
and algebraic
er × S(1)
ts = −S(2)
ts ; er × S(2)
ts = S(1)
ts ; er × S(3)
ts = 0; (3.4)
properties. In the vectorial—including elasticity—problems, the functions (3.1) play
the same role as the surface harmonics (2.5) in the scalar problems. With aid of
(3.3), (3.4), separation of variables in the vectorial harmonic Δf = 0 and bihar-
monic ΔΔg = 0 equations is straightforward [17, 30] and yields the correspond-
ing countable sets of partial solutions—vectorial solid harmonics and biharmonics,
respectively.
3.1.2 Partial Solutions of Lame Equation
The said above holds true for the Lame equation
24.
120 V. I. Kushch
2(1 − ν)
(1 − 2ν)
∇(∇ · u) − ∇ × ∇ × u = 0 (3.5)
being the particular case of vectorial biharmonic equation. In (3.5), u is the dis-
placement vector and ν is the Poisson ratio. The regular partial solutions of (3.5)
u(i)
ts = u(i)
ts (r) are deﬁned as [30]
u
(1)
ts =
rt−1
(t + s)!
S
(1)
ts + tS
(3)
ts , u
(2)
ts = −
rt
(t + 1)(t + s)!
S
(2)
ts , (3.6)
u
(3)
ts =
rt+1
(t + s)!
βt S
(1)
ts + γt S
(3)
ts , βt =
t + 5 − 4ν
(t + 1)(2t + 3)
, γt =
t − 2 + 4ν
(2t + 3)
.
The singular (inﬁnitely growing at r → 0 and vanishing at inﬁnity) functions U
(i)
ts
are given by U
(i)
ts = u
(i)
−(t+1), s, with the relations S
(i)
−t−1,s = (t −s)!(−t −1+s)!S
(i)
ts
taken into account. The functions u(i)
ts (r) and U(i)
ts (r) are the vectorial counterparts
of scalar solid harmonics (2.4).
At the spherical surface r = R, the traction vector Tn = σ · n can be written as
1
2μ
Tr (u) =
ν
1 − 2ν
er (∇ · u) +
∂
∂r
u +
1
2
er × (∇ × u) , (3.7)
μ being the shear modulus. For the vectorial partial solutions (3.6), it yields [30]
1
2μ
Tr (u
(1)
ts ) =
(t − 1)
r
u
(1)
ts ;
1
2μ
Tr (u
(2)
ts ) =
(t − 1)
2r
u
(2)
ts ; (3.8)
1
2μ
Tr (u(3)
ts ) =
rt
(t + s)!
bt S(1)
ts + gt S(3)
ts ;
where bt = (t + 1)βt − 2(1 − ν)/(t + 1) and gt = (t + 1)γt − 2ν. In view of (3.6),
representation of Tr (u
(i)
ts ) in terms of vectorial spherical harmonics (3.1) is obvious.
The total force T and moment M acting on the spherical surface S of radius R are
given by the formulas
T =
Sr
Tr dS, M =
Sr
r × Tr dS, (3.9)
It is straightforward to show that T = M = 0 for all the regular functions u
(i)
ts . Among
the singular solutions U
(i)
ts , we have exactly three functions with non-zero resultant
force T:
T U
(3)
10 = 16μπ(ν − 1)e3; T U
(3)
11 = −T U
(3)
1,−1 = 32μπ(ν − 1)e1. (3.10)
25.
Multipole Expansion Method in Micromechanics of Composites 121
By analogy with Y0
0 , U
(3)
1s can be regarded as the vectorial monopoles. The resultant
moment is zero for all the partial solutions but U
(2)
1s for which we get
M U
(2)
10 = −8μπe3; M U
(2)
11 = M U
(2)
1,−1 = −16μπe1. (3.11)
3.2 Single Inclusion Problem
In the elasticity problem, we deal with the vectorial displacement ﬁeld u (u = u(0)
in a matrix, u = u(1) in the spherical inclusion of radius R) satisfying (3.5). On the
interface S, perfect mechanical contact is assumed:
[[u]] = 0; [[Tr (u)]] = 0; (3.12)
where Tr is given by (3.7). The elastic moduli are (μ0, ν0) for matrix material and
(μ1, ν1) for inclusion, the non-uniform displacement far ﬁeld u f ar is taken as the
load governing parameter.
3.2.1 Series Solution
The displacement in the inclusion u(1) is ﬁnite and so allows expansion into a series
over the regular solutions u
(i)
ts (r) (3.6):
u(1)
(r) =
i,t,s
d
(i)
ts u
(i)
ts (r)
⎛
⎝
i,t,s
=
3
i=1
∞
t=0
t
s=−t
⎞
⎠ , (3.13)
where d
(i)
ts are the unknown constants. The components of the displacement vector
are real quantities, so the property u(i)
t,−s = (−1)su(i)
ts gives d(i)
t,−s = (−1)sd(i)
ts . In the
matrix domain, we write u(0) = u f ar +udis, where the disturbance part udis(r) → 0
with r → ∞ and hence can be written in terms of the singular solutions U
(i)
ts only:
u(0)
(r) = u f ar (r) +
i,t,s
A
(i)
ts U
(i)
ts (r) (3.14)
where A
(i)
ts are the unknown coefﬁcients. By analogy with (2.14), the series term is
thought as the multipole expansion of udis.
26.
122 V. I. Kushch
3.2.2 Far Field Expansion
Due to regularity of u f ar , we can expand it into a series (3.13) with coefﬁcients
c
( j)
ts . With aid of (3.6), we express u f ar at r = R in terms of vectorial spherical
harmonics (3.1)
u f ar (r) =
j,t,s
c
(i)
ts u
(i)
ts (r) =
j,t,s
c
(i)
ts
(t + s)!
3
i=1
U M
i j
t (R, ν0)S
(i)
ts (θ, ϕ) (3.15)
where UMt is a (3 × 3) matrix of the form
UMt (r, ν) = U M
i j
t (r, ν) = rt−1
⎧
⎪⎨
⎪⎩
1 0 r2βt (ν)
0 − r
t+1 0
t 0 r2γt (ν)
⎫
⎪⎬
⎪⎭
. (3.16)
Now, we multiply (3.15) by S(i)
ts and integrate the left-hand side (either analytically
or numerically) over the interface S. In view of (3.2), analytical integration of the
right-hand side of (3.15) is trivial and yields
J(i)
ts =
(t + s)!
4πR2α(i)
ts S
u f ar · S(i)
ts dS =
3
j=1
U M
i j
t (R, ν0) c
( j)
ts (3.17)
From the above equation, we get the expansion coefﬁcients in matrix-vector form as
cts = UMt (R, ν0)−1
Jts (3.18)
where cts = c
(i)
ts
T
and Jts = J
(i)
ts
T
. In the particular case of linear u f ar =
E · r, where E = Ei j is the uniform far-ﬁeld strain tensor, the explicit analytical
expressions for the expansion coefﬁcients are
c
(3)
00 =
(E11 + E+
22 E33)
3γ0(ν0)
, c
(1)
20 =
(2E33 − E11 − E22)
3
,
c
(1)
21 = E13 − i E23, c
(1)
22 = E11 − E22 − 2i E12;
(3.19)
c
(i)
2,−s = (−1)sc
(i)
2s and all other c
(i)
ts are equal to zero.
3.2.3 Resolving Equations
Now, we substitute (3.13) and (3.14) into the ﬁrst condition of (3.12) and use the
orthogonality of S
(i)
ts to reduce it to a set of linear algebraic equations, written in
matrix form as (UGt = UM−(t+1))
27.
Multipole Expansion Method in Micromechanics of Composites 123
(t − s)!(t + s)!UGt (R, ν0) · Ats + UMt (R, ν0) · cts = UMt (R, ν1) · dts. (3.20)
The second, traction continuity condition gives us another set of equations:
(t − s)!(t + s)!TGt (R, ν0) · Ats + TMt (R, ν0) · cts = ωTMt (R, ν1) · dts, (3.21)
where ω = μ1/μ0. In (3.21), the TM is (3 × 3) matrix
T Mt (r, ν) = T M
i j
t (r, ν) = rt−2
⎧
⎪⎨
⎪⎩
t − 1 0 r2bt (ν)
0 −r(t−1)
2(t+1) 0
t(t − 1) 0 r2gt (ν)
⎫
⎪⎬
⎪⎭
. (3.22)
where gt and bt are deﬁned by (3.8); TGt = TM−(t+1), Ats = A
(i)
ts
T
and dts =
d
(i)
ts
T
.
For all indices t ≥ 0 and |s| ≤ t, the coefﬁcients Ats and dts can be found from
linear system (3.20), (3.21). For computational purposes, it is advisable to eliminate
dts from there and obtain the equations containing the unknowns Ats only:
(t − s)!(t + s)!(RMt )−1
RGt · Ats = −cts, (3.23)
where
RGt = ω [UMt (R, ν1)]−1
UGt (R, ν0) − [TMt (R, ν1)]−1
TGt (R, ν0),
RMt = ω [UMt (R, ν1)]−1
UMt (R, ν0) − [TMt (R, ν1)]−1
TMt (R, ν0). (3.24)
This transformation is optional for a single inclusion problem but can be rather useful
for the multiple inclusion problems where the total number of unknowns becomes
very large.
The equations with t = 0 and t = 1 deserve extra attention. First, we note that
U
(2)
00 = U
(3)
00 ≡ 0 and so we have only one equation (instead of three) in (3.23). It
can be resolved easily to get
1
R3
4μ0 + 3k1
3k0 − 3k1
a
(1)
00 = −c
(3)
00 (3.25)
where the relation a0
γ0
= 3k
2μ (k being the bulk modulus) is taken into consideration.
Noteworthy, Eq.(3.25) gives solution of the single inclusion problem in the case of
equiaxial far tension: E11 = E22 = E33. For t = 1, the ﬁrst two columns of the
matrix TMt (3.22) become zero: also, a1+2b1 = 0. From (3.23), we get immediately
A
(2)
1s = A
(3)
1s = 0.
The solution we obtain is complete and valid for any non-uniform far ﬁeld.
For any polynomial far ﬁeld of order tmax, this solution is exact and conservative,
i.e., is given by the ﬁnite number of terms with t ≤ tmax. For example, in the
28.
124 V. I. Kushch
Eshelby-type problem, the expansion coefﬁcients with t ≤ 2 are nonzero only. The
solution procedure is straightforward and remarkably simple as compared with the
scalar harmonics-based approach (see, e.g., [72]). In fact, use of the vectorial spher-
ical harmonics makes the effort of solving the vectorial boundary value problems
comparable to that of solving scalar boundary value problems. Also, solution is writ-
ten in the compact matrix-vector form, readily implemented by means of standard
computer algebra.
3.3 Re-Expansion Formulas
The re-expansions of the vectorial solutions U
(i)
ts and u
(i)
ts (3.5) are [30]: singular-to-
regular (S2R)
U
(i)
ts (r + R) =
3
j=1
∞
k=0
k
l=−k
(−1)k+l
η
(i)( j)
tksl (R)u
( j)
kl (r), r < R ; (3.26)
where
η
(i)( j)
tksl = 0, j > l; η
(1)(1)
tksl = η
(2)(2)
tksl = η
(3)(3)
tksl = Ys−l
t+k ; (3.27)
η(2)(1)
tksl = i
s
t
+
l
k
Ys−l
t+k−1; η(3)(2)
tksl = −4 (1 − ν) η(2)(1)
tksl , k ≥ 1;
η
(3)(1)
tksl =
l
k
η
(3)(2)
t,k−1,sl − Zs−l
t+k − Ys−l
t+k−2
×
(t + k − 1)2
− (s − l)2
2t + 2k − 1
+ C−(t+1),s + Ck−2,l ;
regular-to-regular (S2R):
u
(i)
ts (r + R) =
i
j=1
t+i− j
k=0
k
l=−k
(−1)k+l
ν
(i)( j)
tksl (R)u
( j)
kl (r); (3.28)
where
ν
(i)( j)
tksl = 0, j > l; ν
(1)(1)
tksl = ν
(2)(2)
tksl = ν
(3)(3)
tksl = ys−l
t−k; (3.29)
ν(2)(1)
tksl = i
s
t + 1
−
l
k
ys−l
t−k+1; ν(3)(2)
tksl = −4 (1 − ν) ν(2)(1)
tksl ;
29.
Multipole Expansion Method in Micromechanics of Composites 125
ν(3)(1)
tksl =
l
k
ν(3)(2)
t,k−1,sl − zs−l
t−k − ys−l
t−k+2
(t − k + 2)2
− (s − l)2
2t − 2k + 3
− Cts + Ck−2,l ;
and singular-to-singular (S2S):
U
(i)
ts (r + R) =
3
j=1
∞
k=t−i+ j
k
l=−k
(−1)t+k+s+l
μ
(i)( j)
tksl (R)U
( j)
kl (r), r > R ;
(3.30)
where
μ
(i)( j)
tksl = 0, j > l; μ
(1)(1)
tksl = μ
(2)(2)
tksl = μ
(3)(3)
tksl = ys−l
k−t ; (3.31)
μ
(2)(1)
tksl = i
s
t
−
l
k + 1
ys−l
k−t+1; μ
(3)(2)
tksl = −4 (1 − ν) μ
(2)(1)
tksl ;
μ
(3)(1)
tksl = −
l
k + 1
μ
(3)(2)
t,k+1,sl + zs−l
k−t
− ys−l
k−t+2
(t + k − 2)2
− (s − l)2
2k − 2t + 3
+ C−(t+1),s + C−(k+3),l .
In these formulas, Zs
t = r2
2t−1 Ys
t and zs
t = r2
2t+3 ys
t are the singular and regular,
respectively, scalar solid biharmonics and Cts = (t + 1)2
− s2 βt .
These formulas are the vectorial counterparts of (2.20)–(2.22): being combined
with FMM [19] scheme, they provide the fast multipole solution algorithm for
elastic interactions in the multiple inclusion problem.
For the Stokes interactions in suspension of spherical particles, similar work is
done in [77].
3.4 FCM
Analysis of the FCM elasticity problem is analogous to that of conductivity, so we
outline the procedure and formulas. For simplicity sake, we assume the far displace-
ment ﬁeld to be linear: u f ar = E · r.
3.4.1 Direct (Superposition) Sum
We use the superposition principle to write
30.
126 V. I. Kushch
u(0)
(r) = u f ar (r) +
N
p=1
u
(p)
dis(rp), (3.32)
where
u
(p)
dis(r) =
i,t,s
A
(i)(p)
ts U
(i)
ts (r) (3.33)
is the displacement disturbance ﬁeld caused by pth inclusion: u
(p)
dis(rp) → 0 as
rp → ∞.
3.4.2 Local Expansion Sum
In a vicinity of Oq, the following expansions are valid:
u f ar (r) = u f ar (Rq) + u f ar (rq) = ε∞
· Rq +
∞
t=0
t
s=−t
c
(i)
ts u
(i)
ts (rq), (3.34)
where c
(i)
tst are given by (3.19). Displacement u
(q)
dis in (3.32) is written in the local
coordinate system of the qth inhomogeneity and ready for use. For p = q, we apply
the re-expansion formula (3.26) to get
u(0)
(r) = ε∞
· Rq +
i,t,s
A
(i)(q)
ts U
(i)
ts (rq) + a
(i)(q)
ts u
(i)
ts (rq) , (3.35)
where
a
(i)(q)
ts =
N
p=q j,k,l
(−1)k+l
A
( j)(p)
kl η
( j)(i)
ktls (Rpq). (3.36)
In matrix form,
a
(q)
ts =
N
p=q k,l
ηktls(Rpq)
T
· A
(p)
kl (3.37)
where A
(q)
ts = A
(i)(q)
ts
T
, a
(q)
ts = a
(i)(q)
ts
T
and ηtksl = (−1)k+l η
(i)( j)
tksl .
3.4.3 Inﬁnite System of Linear Equations
With the displacement within qth inhomogeneity represented by the series (3.13)
with coefﬁcients d
(q)
ts d
(i)(q)
ts
T
, we come to the above considered single inclusion
problem. The resulting inﬁnite system of linear equations has the form
31.
Multipole Expansion Method in Micromechanics of Composites 127
(t−s)!(t+s)!(RM
(q)
t )−1
RG
(q)
t ·A
(q)
ts +
N
p=q k,l
ηktls(Rpq)
T
·A
(p)
kl = −cts, (3.38)
where RM
(q)
t = RMt (Rq, ν0, νq) and RG
(q)
t = RGt (Rq, ν0, νq) are given by
(3.24). Likewise (2.33), this system can be solved by the truncation method.
Again, the obtained solution is straightforward and remarkably simple: see, for
comparison, solution of two-sphere problem [8]. This approach enables an efﬁcient
analytical solution to a wide class of 3D elasticity problems for multiple-connected
domains withspherical boundaries, inparticular, studyof elasticinteractions between
the spherical nano inclusions with Gurtin-Murdoch type interfaces [54].
3.4.4 FCM and Effective Elastic Moduli
We deﬁne, by analogy with FCM conductivity problem, an equivalent inclusion
radius as R3
ef f = N/c, c being a volume fraction of inclusions, and compare, in
spirit of Maxwell’s approach, an asymptotic behavior of disturbances caused by the
ﬁnite cluster of inclusions and “equivalent” inclusion. To this end, we apply the (S2S)
re-expansion (3.30), giving us for r > maxp Rp
N
p=1
u
(p)
dis(r) =
i,t,s
e
(i)
ts U
(i)
ts (r), (3.39)
where
ets =
N
p=1 k,l
μktls(−Rp)
T
· A
(p)
kl (3.40)
and μtksl = μ
(i)( j)
tksl .
Now, we equate ets given by (3.40) to ats in (3.23) to determine the effective
moduli of composite. Considering the equiaxial far tension ε∞
11 = ε∞
22 = ε∞
33 gives
us, in view of (3.25), an expression for the effective bulk modulus kef f
kef f =
3k0 + 4μ0 c A
(1)
00
3 1 − c A
(1)
00
, (3.41)
where A(1)
00 = 1
N
N
p=1 A
(1)(p)
00 is the mean dipole moment. In the case we neglect
interactions between the inclusions, (3.41) reduces to the mechanical counterpart of
the original Maxwell’s formula (e.g., [58]).
32.
128 V. I. Kushch
3.5 RUC
The stress ﬁeld in the composite bulk is assumed to be macroscopically uniform,
which means constancy of the macroscopic strain ε and stress σ tensors. We
take ε = E as input (governing) load parameter. Alike the conductivity problem,
periodic geometry of composite results in quasi-periodicity of the displacement ﬁeld
and periodicity of the strain and stress ﬁelds:
u (r + aii ) = u (r) + aE · ii ; (3.42)
ε (r + aii ) = ε (r) ; σ (r + aii ) = σ (r) .
3.5.1 Displacement Field
The conditions (3.42) are fulﬁlled by taking u (r) = ε · r + udis (r), where udis is
the periodic disturbance displacement ﬁeld. In the matrix domain, we write u in the
form analogous to (2.36):
u(0)
(r) = E · r +
N
p=1
u
∗(p)
dis (rp), (3.43)
where
u
∗(p)
dis (rp) =
k
u
(p)
dis rp + ak (3.44)
and
u
(p)
dis(r) =
i,t,s
A
(i)(p)
ts U
(i)
ts (r). (3.45)
Again, by analogy with (2.38), u
∗(p)
dis can be expressed in terms of the periodic
functions U
∗(i)
ts [30]:
u
∗(p)
dis (rp) =
∞
i,ts
A
(p)
ts U
∗(i)
ts (rp), U
∗(i)
ts (rp) =
k
U
(i)
ts (rp + ak). (3.46)
An alternate, mathematically equivalent set of vectorial periodic functions have been
written [76] in terms of fundamental periodic solutions [21]. The resulting linear
system closely resembles that for FCM (3.38):
33.
Multipole Expansion Method in Micromechanics of Composites 129
(t−s)!(t+s)!(RM
(q)
t )−1
RG
(q)
t ·A
(q)
ts +
N
p=1 k,l
η∗
ktls(Rpq)
T
·A
(p)
kl = −cts, (3.47)
where c
(i)
ts are given by (3.19). The matrix coefﬁcients η∗
ktls(Rpq) are the lattice sums
of corresponding expansion coefﬁcients η∗
ktls(Rpq) (3.27). Their evaluation is mostly
based on the relevant results for scalar potential (2.40). The only new feature here is
the biharmonic lattice sum
Z∗
k+t,l−s(Rpq) =
k
Zl−s
k+t Rpq + ak ; (3.48)
for Zs
t deﬁnition, see Sect.3.3. This sum closely relates the fundamental solution S2
in [21]: its evaluation with aid of Evald’s technique is discussed there.
3.5.2 Effective Stiffness Tensor
The fourth rank effective elastic stiffness tensor C∗ = C∗
i jkl is deﬁned by (1.10).
In order to evaluate C∗
i jkl for a given geometry of composite, one must conduct
a series of numerical tests with different macro strains Ei j and evaluate the macro
stress σ Eq.(1.12). Speciﬁcally, C∗
i jkl = σi j for εmn = δmkδnl. For this purpose,
we need the explicit expressions of average strain and stress corresponding to our
displacement solution.
Evaluation of the macroscopic strain tensor, ε is elementary. First, we recall that
we have taken RUC with S0 ∈ V0, so u = u(0) in (1.12). Next, we observe that for
the periodic part of solution in the boundary points ra ∈ S0 and rb = ra + aij ∈ S0
belonging to the opposite cell faces we have udis (rb) = udis (ra) whereas the
normal unit vector changes the sign: n (rb) = −n (ra). Hence, the integrals of udis
over the opposite faces cancel each other and the total integral over S0 equals to zero.
Integration of the linear part of u(0) is elementary: the divergence theorem gives the
expected ε = E.
A suitable for our purpose expression of the macroscopic stress tensor σ is given
by (1.13). Noteworthy, surface integration in (1.13) is greatly simpliﬁed by taking
u(i)
ts as a trial displacement vector u . It follows from (3.19) that u(3)
00 and u(1)
2s are
the linear function of coordinates. For example, u
(3)
00 = rγ0S
(3)
00 = γ0r =γ0ukk; also,
Tn(u
(3)
00 ) = 3k
r u
(3)
00 , k being the bulk modulus. We get from Eq.(1.13)
σii = C(0)
iikk εkk +
1
V
N
q=1 Sq
Tn(u(0)
) −
3k0
r
u(0)
·
u
(3)
00
γ0
dS. (3.49)
Now, we put here the local expansion of u(0) given by Eq.(3.35) and the analogous
expansion of Tn u(0) :
34.
130 V. I. Kushch
Tn u(0)
(rq) =
i,t,s
A
(i)(q)
ts Tn U
(i)
ts (rq) + a
(i)(q)
ts + c
(i)
ts Tn u
(i)
ts (rq) . (3.50)
For the explicit expression of Tn(U
(i)
ts ) and Tn(u
(i)
ts ) in terms of vectorial spherical
harmonics S
(i)
ts , see [54]. By taking orthogonality of these harmonics on the sphere
into account we ﬁnd that the only function giving non-zero contribution to the integral
in (3.49) is U
(1)
00 = − 2
r2 S
(3)
00 for which Tn U
(1)
00 = −4μ
r U
(1)
00 = 8μ
r3 S
(3)
00 . Thus, we
obtain
Sq
Tn(u(0)
) −
3k0
r
u(0)
·
u
(3)
00
γ0
dS
= A
(1)(q)
00
2
R2
(4μ0 + 3k0)
Sq
S
(3)
00 · S
(3)
00 dS = 8π (4μ0 + 3k0) A
(1)(q)
00 .
By using in the same way the (simple shear mode) functions
u(1)
20 = u33 − (u11 + u22)/2;
u(1)
21 = u13 + u31 /2 + i(u23 + u32)/2;
u(1)
22 = u11 − u22 /4 + i u12 + u21 /4;
for which Tr (u
(1)
2s ) = 2μ
r u
(1)
2s , we come to the ﬁnite exact formulas
S11 + S22 + S33 =
(1 + ν0)
(1 − 2ν0)
(E11 + E22 + E33) +
12π
a3
(1 − ν0)
(1 − 2ν0)
N
q=1
A
(1)(q)
00 ;
2S33 − S11 − S22 = 2E33 − E11 − E22 −
16π
a3
(1 − ν0)
N
q=1
A
(3)(q)
20 ;
S11 − S22 − 2iS12 = E11 − E22 − 2iE12 −
32π
a3
(1 − ν0)
N
q=1
A
(3)(q)
22 ;
S13 − iS23 = E13 − iE23 −
8π
a3
(1 − ν0)
N
q=1
A
(3)(q)
21 . (3.51)
where Si j = σi j /2μ0. The coefﬁcients A
(i)(q)
ts are linearly proportional to E. The
σi j are uniquely determined from Eqs.(3.47, 3.51) for Ekl given and, thus, these
equations together with (1.10) are sufﬁcient for evaluation of the effective stiffness
tensor, C∗. (3.51) involves only the expansion coefﬁcients A
(i)(q)
i−1,s which can be
regarded as the dipole moments. The effective elastic moduli of composite with
simple cubic array of spherical inclusions have been found by [31, 76], for the RUC
type structure—by [17, 78].
35.
Multipole Expansion Method in Micromechanics of Composites 131
4 Composite with Spheroidal Inclusions
4.1 Scalar Spheroidal Solid Harmonics
The spheroidal coordinates (ξ, η, ϕ) relate the Cartesian coordinates (x1, x2, x3)
by [23]
x1 + ix2 = dξη exp(iϕ), x3 = dξη, (4.1)
where
ξ
2
= ξ2
− 1, η2
= 1 − η2
(1 ≤ ξ < ∞, −1 ≤ η ≤ 1, 0 ≤ ϕ < 2π). (4.2)
At Re(d) > 0, the formulas (4.1) and (4.2) deﬁne a family of confocal prolate
spheroids with inter-foci distance 2d: to be speciﬁc, we expose all the theory for this
case. In the case of oblate spheroid, one must replace ξ with iξ and d with (−id) in
these and all following formulas. For d → 0 and dξ → r, the spheroidal coordinates
system degenerates into spherical one, with η → cos θ.
Separation of variables in Laplace equation in spheroidal coordinates gives us the
sets of partial solutions, or solid spheroidal harmonics: regular
f s
t (r, d) = P−s
t (ξ)χs
t (η, ϕ) =
(t − s)!
(t + s)!
Ps
t (ξ)χs
t (η, ϕ) (4.3)
and irregular
Fs
t (r, d) = Q−s
t (ξ)χs
t (η, ϕ) =
(t − s)!
(t + s)!
Qs
t (ξ)χs
t (η, ϕ) (4.4)
Here, Qs
t are the associate Legendre’s functions of second kind [23]. The functions
(4.3) and (4.4) obey the properties analogous to (2.7). The functions Fs
t → 0 with
r → ∞ and, by analogy with Ys
t , can be regarded as spheroidal multipole poten-
tials. We mention the multipole type re-expansions between Ys
t and Fs
t [13] which,
in our notations, take the form
Fs
t (r, d) = (−1)s
∞
k=t
K(1)
tk (d)Ys
k (r) ( r > d); (4.5)
Ys
t (r) = (−1)s
∞
k=t
K
(2)
tk (d)Fs
k (r, d);
36.
132 V. I. Kushch
where
K
(1)
tk (d) =
d
2
k+1 √
π
Γ k−t
2 + 1 Γ k+t
2 + 3
2
, (4.6)
K
(2)
tk (d) =
2
d
k+1
(−1)(k−t)/2 k + 1
2 Γ k+t
2 + 1
2
√
πΓ k−t
2 + 1
for (t−k) even and equal to zero otherwise. The analogous relations are also available
for the regular solid harmonics, ys
t and f s
t [39].
4.2 Single Inclusion: Conductivity Problem
Let an unbounded solid contains a single prolate spheroidal inclusion with boundary
deﬁned by ξ = ξ0. The matrix-inclusion thermal contact obeys the conditions (2.9)
where qr is replaced with qξ = −λ∇T ·eξ = d−1(ξ
2
−η2)−1/2∂T/∂ξ. The solution
ﬂow is quite analogous to that for the spherical inclusion, so we outline it brieﬂy.
4.2.1 Series Solution
The temperature ﬁeld inside the inclusion is given by a series
T (1)
(r) =
∞
t=0
t
s=−t
dts f s
t (r, d). (4.7)
The temperature ﬁeld outside the inclusion is a sum of far and disturbance ﬁelds:
T (0)
(r) = Tf ar (r) + Tdis(r), Tdis(r) =
∞
t=1
t
s=−t
Ats Fs
t (r, d). (4.8)
The second term in (4.8) can be thought as the spheroidal multipole expansion of the
disturbance ﬁeld Tdis. Noteworthy, at some distance from inclusion (namely, where
r > d) it can be also expanded, by applying formula (4.5), over the spherical
multipoles Ys
t . The Tf ar series expansion in a vicinity of inclusion is analogous to
(4.7). In view of (2.6), the cts coefﬁcients are equal to
cts =
(2t + 1)
4πPs
t (ξ0)
2π
0
dϕ
1
−1
Tf ar χs
t (η, ϕ) dη. (4.9)
37.
Multipole Expansion Method in Micromechanics of Composites 133
4.2.2 Resolving Equations
The temperature continuity at ξ = ξ0 gives, in view of χs
t (η, ϕ) orthogonality (2.6),
a set of linear algebraic equations
Qs
t (ξ0)Ats + Ps
t (ξ0)cts = Ps
t (ξ0)dts. (4.10)
The second, normal ﬂux continuity condition gives us also
Q s
t (ξ0)Ats + P s
t (ξ0)cts = ωP s
t (ξ0)dts, (4.11)
where ω = λ1/λ0 and stroke means derivative with respect to argument. The ﬁnal
formula for the coefﬁcients Ats is
1
(ω − 1)
ω
Qs
t (ξ0)
Ps
t (ξ0)
−
Q s
t (ξ0)
P s
t (ξ0)
Ats = −cts. (4.12)
4.3 Re-expansion Formulas
We deﬁne the inclusion-related local coordinate system in a way that coordinate
surface coincides with the surface of inclusion. Spheroidal shape of inclusion dictates
the origin and, in contrast to spherical case, orientation of this system. A general
transformation of coordinates can be splitted into a sum of translation and rotation,
i.e. r1 = R + O · r2 where O is a symmetrical positively deﬁnite matrix with
det O = 1. Analogously, the general re-expansion formula is given by superposition
of two more simple formulas, one written for translation and another—for rotation.
4.3.1 Translation
Inthecaseofco-axial(O = I)coordinatesystems(d1, ξ1, η1, ϕ1)and(d2, ξ2, η2, ϕ2)
centered at the points O1 and O2, respectively, the re-expansion formulas (addition
theorems) of three kinds for the spheroidal solid harmonics are [32, 35, 37]:
Fs
t (r1, d1) =
∞
k=0
k
l=−k
ηtk,s−l (R, d1, d2) f l
k (r2, d2) ; (4.13)
f s
t (r1, d1) =
t
k=0
k
l=−k
μtk,s−l (R, d1, d2) f l
k (r2, d2) ; (4.14)
Fs
t (r1, d1) =
∞
k=t
k
l=−k
νtk,s−l (R, d1, d2) Fl
k (r2, d2) . (4.15)
38.
134 V. I. Kushch
A simple way to derive these formulas consists in combining the formulas (4.5),
(4.6) with the relevant re-expansions for spherical harmonics (2.20)–(2.22). Say, for
(4.13) this procedure yields
η
(1)
tks = atk
∞
r=0
d1
2
2r
Mtkr (d1, d2) Ys
t+k+2r (R) , (4.16)
where
atk = (−1)k+l
π k +
1
2
d1
2
t+1
d2
2
k
, (4.17)
Mtkr =
r
j=0
(d2/d1)2 j
j!(r − j)!Γ (t + r − j + 3/2) Γ (k + j + 3/2)
(4.18)
and Γ (z) is the gamma-function [1]. For d1 = d2, this expression reduces to
Mtkr =
(t + k + r + 2)r
r! Γ (t + r + 3/2) Γ (k + r + 3/2)
, (4.19)
where (n)m is the Pochhammer’s symbol. Derived this way the coefﬁcients in (4.14)
and (4.15) are
μ
(1)
tks = k +
1
2
d1
2
−t
d2
2
k σ
r=0
d1
2
2r
ys
t−k−2r (R) (4.20)
×
r
j=0
(−1)r− j Γ (t + j − r + 1/2) (d2/d1)2 j
j!(r − j)! Γ (k + j + 3/2)
and
ν
(1)
tks = k +
1
2
d1
2
t+1
d2
2
−(k+1) σ
r=0
d1
2
2r
ys
k−t−2r (R) (4.21)
×
r
j=0
(−1)j Γ (k − j + 1/2) (d2/d1)2 j
j!(r − j)! Γ (t + r − j + 3/2)
,
respectively. Here, σ = |t − k| − |s|. They are consistent with the formulas reported
by [13].
It appears, however, that formula (4.13) with coefﬁcients (4.16) is valid only for
R > d1 + d2; this fact is due to the geometry restriction in (4.5) and (2.20) used
for derivation. A general, geometrical restrictions-free expression [32] is
39.
Multipole Expansion Method in Micromechanics of Composites 135
η
(2)
tks =
atk
√
π
2
d3
t+k+1 ∞
r=0
Fs
t+k+2r (R, d3) t + k + 2r +
1
2
(4.22)
×
r
j=0
(−1)r− j
(r − j)!
d1
d3
2 j
Γ (t + k + r + j + 1/2) Mtkj (d1, d2)
The series (4.13) with coefﬁcients (4.22) for d3 > d1 converges in all points inside
the spheroid ξ2 = ξ20 with the center at a point O2 and inter-foci distance 2d2 if
point O1 lies outside the spheroid with semiaxes d2ξ20 and d2ξ20 + d1 (ξ12 > ξ0
12).
Here,
ξ0
12 = cosh arctanh
d2ξ20
d2ξ20 + d1
(4.23)
where (d12, ξ12, η12, ϕ12) are spheroidal coordinates of vector R in a system with
origin in the point O2 and d12 = (d2ξ20 + d1) /ξ0
12. This is condition of non-
intersecting the spheroidal surface ξ2 = ξ20 and inﬁnitely thin spheroid with inter-
foci distance 2d1 centered at point O1 and holds true for any two non-intersecting
spheroids of ﬁnite size.
In the case R > d1 + d2, both the representations, η
(1)
tk,s−l and η
(2)
tk,s−l are valid
and using the simpler expression (4.16) is preferable. For R < d1 + d2, η
(1)
tk,s−l
diverges and η
(2)
tk,s−l should be used instead. Noteworthy, convergence rate of (4.23)
is geometry-dependent and the numerical difﬁculties may arise, e.g., for the closely
placed very elongated spheroids. In this situation, using the numerical integration
formula
ηtk,s−l =
(2t + 1)
4πPl
k(ξ20)
2π
0
dϕ2
1
−1
Fs
t (r + R, d1) χl
k(η2, ϕ2) dη2 (4.24)
analogous to (4.9) would be the most appropriate option.
4.3.2 Rotation
The re-expansion of spheroidal solid harmonics (4.3) and (4.4) due to the rotation of
the coordinate system (R = 0, d1 = d2 = d) is determined by
f s
t (r1, d) =
t
k=0
k
l=−k
f l
k (r2, d) (−1)s+l
k +
1
2
(4.25)
×
∞
r=k
(−1)
t−r
2 Γ t+r
2 + 1
2
t−r
2 ! r−k
2 !Γ r+k
2 + 3
2
(r − l)!(r + l)!
(r − s)!(r + s)!
Sr−s,r−l
2r (w);
40.
136 V. I. Kushch
Fs
t (r1, d) =
∞
k=t
k
l=−k
Fl
k (r, d) (−1)s+l
k +
1
2
(4.26)
×
∞
r=k
(−1)
t−r
2 Γ t+r
2 + 1
2
r−t
2 ! k−r
2 !Γ r+t
2 + 3
2
Sr−s,r−l
2r (w);
where primes over the sums denote that they contain only terms with even (t − k)
and (t − r). Also, Ss,l
t are the spherical harmonics [3] in four-dimensional space,
w = wi is the unit four-dimensional vector determining uniquely the rotation
matrix
O =
⎛
⎜
⎝
w2
2 − w2
1 − w2
3 + w2
4 2 (w2w3 − w1w4) 2 (w1w2 + w3w4)
2 (w2w3 + w1w4) w2
3 − w2
1 − w2
2 + w2
4 2 (w1w3 − w2w4)
2 (w1w2 − w3w4) 2 (w1w3 + w2w4) w2
1 − w2
2 − w2
3 + w2
4
⎞
⎟
⎠ .
(4.27)
These results are similar to those derived by [13]. Coupled with (4.13)–(4.15), they
provide the representation of spheroidal solid harmonics in any arbitrary positioned
and oriented coordinate system and thus form a theoretical basis of solving the poten-
tial theory problems for multiply connected domains with spheroidal boundaries by
the Multipole Expansion Method.
4.4 FCM
Let consider an unbounded solid containing N spheroidal inclusions of conductivity
λq centered in the points Oq. Geometry of qth inclusion (q = 1, 2, . . . , N) is deﬁned
by two numbers: ξ0 = ξq0 and d = dq. Its position and orientation are given by the
vector Rq, and matrix Oq, respectively. The local Cartesian (x1q, x2q, x3q) and
spheroidal (dq, ξq, ηq, ϕq) coordinates are related by (4.1); r = Rq + Oq · rq. The
linear far ﬁeld Tf ar = G · r is prescribed.
Temperature in the matrix solid is given by the superposition sum (2.27), where
the disturbance ﬁeld caused by pth inclusion is written now in terms of spheroidal
multipoles:
T
(p)
dis (rp) =
∞
t=1
t
s=−t
A
(p)
ts Fs
t (rp, dp). (4.28)
In a vicinity of Oq, the following expansions are valid:
Tf ar (rq) =
∞
t=0
t
s=−t
c
(q)
ts f s
t (rq), (4.29)
41.
Multipole Expansion Method in Micromechanics of Composites 137
where c
(q)
00 = G·Rq, c
(q)
10 = Gi Oi3qdq, c
(q)
11 = 2dq Gi (Oi1q −iOi2q), c
(q)
1,−1 = −c
(q)
11
and c
(q)
ts = 0 otherwise. The term T
(q)
dis is already written in qth basis; for p = q, we
apply the re-expansion formulas for irregular solid harmonics to get
T
(p)
dis (rq) =
∞
t=0
t
s=−t
a
(q)
ts f s
t (rq), a
(q)
ts =
N
p=q
∞
k=1
k
l=−k
A
(p)
kl ηl−s
k+t (Rpq, Opq).
(4.30)
Here, ηl−s
k+t (Rpq, Opq) is the expansion coefﬁcient obtained by consecutive applica-
tion of (4.13) and (4.25). In their calculation, one of three options—(4.13), (4.22) or
(4.24)—is used depending on the relative position of pth and qth particles.
By putting all the parts together, we get
T (0)
(rq) =
∞
t=1
t
s=−t
A
(q)
ts Fs
t (rq) +
∞
t=0
t
s=−t
a
(q)
ts + c
(q)
ts f s
t (rq). (4.31)
Substitution of (4.31) and T (q) in the form (4.7) but written in qth local basis into
(2.12) gives an inﬁnite set of linear equations with unknowns A
(q)
ts , analogous to
(4.12) (ωq = λq/λq):
1
(ωq − 1)
ωq
Qs
t (ξq0)
Ps
t (ξq0)
−
Q s
t (ξq0)
P s
t (ξq0)
A
(q)
ts + a
(q)
ts = −c
(q)
ts . (4.32)
4.5 RUC
Likewise (2.33), the above solution can be used for evaluation of the effective
conductivity of composite with spheroidal inclusions by combining it with Maxwell’s
model. An alternate, advanced tool for this purpose is RUC model: here, we discuss it
brieﬂy. For simplicity sake, we assume all the spheroids entering the unit cell oriented
in x3-direction: considering the case of arbitrarily oriented spheroids involves some
extra algebra but does not meet any other difﬁculties [39].
4.5.1 Periodic Potentials
ToapplytheproceduredescribedinSect.2.5,weﬁrstintroducetheperiodicpotentials
analogous to Y∗
ts (2.38):
F∗
ts (r, d) =
k
Fs
t (r + ak, d) , (4.33)
42.
138 V. I. Kushch
where summation is made over all the integer k1, k2 and k3. The solution in the
matrix domain is given by the (2.36), (2.37), where now the pth lattice disturbance
T
∗(p)
dis (rp) =
∞
t=1
t
s=−t
A
(p)
ts F∗
ts(rp, dp). (4.34)
The solution in the form (2.36), (2.37) satisﬁes the periodicity conditions. In fact,
what we need to complete the solution is to ﬁnd local expansion of the functions
F∗
ts(rp, dp) in a vicinity of qth inclusion in terms of spheroidal solid harmonics. In
the case p = q, we apply the formula (4.13) to all the terms of the sum (4.33) but
one with k = 0 to obtain, after change of summation order,
F∗
ts(rq, dq) = Fs
t rq, dq +
∞
k=0 |l|≤k
η∗
tk,s−l 0, dq, dq f l
k rq, dq , (4.35)
where the expansion coefﬁcients are the triple inﬁnite (lattice) sums
η∗s−l
tk (R, d1, d2) =
k=0
ηs−l
kt (R + ak, d1, d2) . (4.36)
In the case p = q, rp = Rpq + rq and
F∗
ts(rp, dp) =
∞
k=0 |l|≤k
ηs−l
tk Rpq, dp, dq + η∗
tk,s−l Rpq, dp, dq f l
k rq, dq .
(4.37)
Recall, in RUC model Rpq is taken as a minimal distance between any two
particles of pth and qth lattices, so Rpq < Rpq + ak for any k = 0. As was
discussed above, the ﬁrst term, ηs−l
tk in (4.33) can be evaluated from the appropriate
formula. Provided the RUC size a is sufﬁciently large, the formula (4.13) can be
used for evaluating the lattice sum η∗s−l
tk . Speciﬁcally,
η∗
tk,s−l Rpq, dp, dq =
k=0
(1)
ηs−l
tk Rpq + ak, dp, dq (4.38)
= atk
∞
r=0
d1
2
2r
Mtkr dp, dq Y∗
t+k+2r,s−l Rpq ,
where Y∗
t+k+2r,s−l Rpq are the standard lattice sums of spherical multipoles (2.40).
After we found the local expansions (4.35) and (4.37), the problem is effectively
reduced to a set of single inclusion problems. An inﬁnite linear set of equations with
unknowns A
(q)
ts has the form (4.32), where now
43.
Multipole Expansion Method in Micromechanics of Composites 139
a
(q)
ts =
N
p=1
∞
k=1
k
l=−k
A
(p)
kl η∗
tk,s−l Rpq, dp, dq . (4.39)
4.5.2 Effective Conductivity
The effective conductivity tensor ∗
of composite is given by (1.1). In view of
the temperature ﬁeld periodicity, averaging the temperature gradient in composite
with spheroidal inclusions follows the same way as in the spherical case and yields
∇T = G. The macroscopic ﬂux q is given by (1.9) where integration is made
now over the spheroidal surfaces Sq : ξq = ξq0. To simplify derivation, we perform
it for N = 1 omitting the q index and, then, will write the formula for a general case.
For the composite with isotropic matrix we consider, the normal component heat
ﬂux qn = q · n at the spheroidal surface equals
qn = qξ = −λ∇T · eξ = −λ
ξh
d
∂T
∂ξ
(4.40)
In this case, (1.9) simpliﬁes to
q
λ0
= −G −
1
V S
T (0)
n −
∂T (0)
∂n
r dS. (4.41)
The surface integration uses the local expansion (4.31), from where
T (0)
=
∞
t=1
t
s=−t
(t − s)!
(t + s)!
Ats Qs
t (ξ) + (ats + cts) Ps
t (ξ) χs
t , (4.42)
∂T
∂n
=
ξh
d
∞
t=1
t
s=−t
(t − s)!
(t + s)!
Ats Q s
t (ξ) + (ats + cts) P s
t (ξ) χs
t .
Here, χs
t = χs
t (η, ϕ); ats are given by (4.39). At the interface S : ξ = const,
r = d − 2ξχ−1
1 e1 + ξχ1
1e2 + ξχ0
1e3 , (4.43)
n = eξ = h − 2ξχ−1
1 e1 + ξχ1
1e2 + ξχ0
1e3 .
By substituting these formulas into (4.41) we get
1
h
T (0)
n −
∂T (0)
∂n
r = 2 ξξ
∂T (0)
∂ξ
− ξT (0)
χ−1
1 e1 (4.44)
+ ξT (0)
− ξξ
∂T (0)
∂ξ
χ1
1e2 + ξ T (0)
− ξ
∂T (0)
∂ξ
χ0
1e3
44.
140 V. I. Kushch
Before integrating this expression, we note that
f 0
1 (r, d) − ξ
∂ f 0
1 (r, d)
∂ξ
≡ 0; ξ f 1
1 (r, d) − ξξ
∂ f 1
1 (r, d)
∂ξ
≡ 0. (4.45)
Also, it is directly testable that
ξ ξQ 0
1 − Q0
1 =
1
ξ
;
1
2
ξQ1
1 − ξξQ 1
1 =
1
ξ
; (4.46)
and hence
F0
1 (r, d) − ξ
∂F0
1 (r, d)
∂ξ
= −
1
ξ
2
χ0
1(η, ϕ); (4.47)
ξF1
1 (r, d) − ξξ
∂F1
1 (r, d)
∂ξ
=
1
ξ
χ1
1(η, ϕ).
The formula (4.41) readily transforms to
q
λ0
= −G −
1
V
d2
2π
0
1
−1
T (0)
n −
∂T (0)
∂n
r
ξ0
h
dηdϕ.
By taking Eqs.(4.42)–(4.47) and orthogonality of the surface harmonics χs
t into
account we ﬁnd readily that
2π
0
1
−1
T (0)
− ξ
∂T (0)
∂ξ
χ0
1dηdϕ = −
4π
3ξ
2
A10; (4.48)
2π
0
1
−1
ξξ
∂T (0)
∂ξ
− ξT (0)
χ−1
1 dηdϕ =
4π
3ξ
A11;
and, ﬁnally,
q
λ0
= −G +
4πd2
3a3
Re (A10e3 − 2A11e1) . (4.49)
In the limiting case where a spheroid degenerates into a sphere, Eq.(4.49) is
expected to reduce to (2.47). It is pertinent to mention here that (4.49) can be
derived directly from Eq.(2.47)—and this derivation is much easier as compared
with that performed above. First, we recognize that the overall structure of Eq.(4.49)
is pre-determined by (1.9), so we only need to ﬁnd the dipole moments entering
this formula linearly. Next, (4.5) provides the necessary relationship between the
45.
Multipole Expansion Method in Micromechanics of Composites 141
moments of spherical and spheroidal multipole ﬁelds. For t = 1, the scaling factor
equals (−1)sd2/3: as would be expected, by introducing this factor into (2.47) we
immediately get (4.49).
Noteworthy, the effective conductivity of composite with spheroidal inclusions
depends not only on the volume fraction and conductivity of disperse phase but also
on the shape, arrangement and orientation of inclusions. Even for simplest cubic
symmetry case, this composite is anisotropic at macro level [35]. The inﬁnitely thin
oblate spheroid can be used to model penny-shape crack or superconducting platelet.
Overall conductivity of solid is greatly affected by presence of these inhomogeneities
although their volume content is equal to zero [40].
4.6 Elasticity Problem
4.6.1 Vectorial Partial Solutions of Lame Equation
The following regular vectorial partial solutions f
(i)
ts have been introduced by
[33, 34]:
f
(1)
ts = e1 f s−1
t−1 − e2 f s+1
t−1 + e3 f s
t−1; (4.50)
f
(2)
ts =
1
(t + 1)
e1(t − s + 1) f s−1
t + (t + s + 1)e2 f s+1
t − e3s f s
t ;
f(3)
ts = e1 − (x1 − ix2)D2 f s−1
t+1 − (ξ2
0 − 1)D1 f s
t + (t − s + 1)(t − s + 2)βt f s−1
t+1
+ e2 (x1 + ix2)D1 f s+1
t+1 − (ξ2
0 − 1)D2 f s
t + (t + s + 1)(t + s + 2)βt f s+1
t+1
+ e3 x3D3 f s
t+1 − ξ2
0D3 f s
t − (t − s + 1)(t + s + 1)βt f s
t+1 .
In (4.50), ei are the complex Cartesian vectors (2.11) and Di are the differential
operators (2.10). The irregular vectorial partial solutions F(i)
ts are obtained from (4.50)
by replacing the indext with −(t + 1) and f s
t with Fs
t . In (4.50), f(1)
ts and f(2)
ts are
the vectorial harmonic functions whereas f
(3)
ts is the vectorial biharmonic function.
It contains the harmonic term ξ2
0∇ f s
t added in spirit of [70] to simplify the f(3)
ts and
Tξ(f
(3)
ts ) expressions at the interface ξ = ξ0.
The vectorial harmonics (3.1) do not apply to spheroid; instead we will use the
vectorial surface harmonics in the form C
( j)
ts (η, ϕ) = ej χ
sj
t (η, ϕ), where s1 =
s − 1, s2 = s + 1 and s3 = s [43]. At the spheroidal surface ξ = ξ0, the functions
f(i)
ts can be written as
f
(1)
ts = P−s+1
t−1 C
(1)
t−1,s − P−s−1
t−1 C
(2)
t−1,s + P−s
t−1C
(3)
t−1,s (4.51)
f
(2)
ts =
1
(t + 1)
(t − s + 1)P−s+1
t C
(1)
ts + (t + s + 1)P−s−1
t C
(2)
ts − sP−s
t C
(3)
ts ;
46.
142 V. I. Kushch
f
(3)
ts = (t − s + 2)ξ0 P−s+1
t + (t − s + 2) − 1 + (t − s + 1)βt P−s+1
t+1 C
(1)
t+1,s
− (t − s)ξ0 P−s−1
t + (t + s + 2) − 1 + (t + s + 1)βt P−s−1
t+1 C
(2)
t+1,s
+ (t − s + 1)ξ0 P−s
t − Cts P−s
t+1 C
(3)
t+1,s
where Ps
t = Ps
t (ξ0), C
( j)
ts = C
( j)
ts (η, ϕ) and Cts is deﬁned in (3.31). In compact
form,
f(i)
ts
S
=
3
j=1
U M
ji
ts (ξ0, ν) C
( j)
t+ j−2,s. (4.52)
Analogously, for the irregular solutions we have
F
(i)
ts
S
=
3
j=1
UG
ji
ts (ξ0, ν) C
( j)
t− j+2,s. (4.53)
At the spheroidal surface ξ = const, the traction vector Tn = σ · n can be
written as
1
2μ
Tξ(u) =
ν
1 − 2ν
eξ (∇ · u) +
ξη
d
∂
∂ξ
u +
1
2
eξ × (∇ × u) . (4.54)
For the vectorial partial solutions (4.50), this yields
1
2μ
Tξ f
(i)
ts
S
=
3
j=1
T M
ji
ts (ξ0, ν) C
( j)
t+ j−2,s; (4.55)
1
2μ
Tξ F
(i)
ts
S
=
3
j=1
T G
ji
ts (ξ0, ν) C
( j)
t− j+2,s.
For the explicit expressions of T M
ji
ts and T G
ji
ts , see [34, 37].
The net force vector T is non-zero for the functions F(3)
1s only:
T F
(3)
10 = 16μπd(ν−1)e3; T F
(3)
11 = −T F
(3)
1,−1 = −32μπd(ν−1)e1 (4.56)
Three functions with non-zero net moment M are
M F
(2)
10 = −
2μπ
3
d2
e3; M F
(2)
11 = M F
(2)
1,−1 =
4μπ
3
d2
e1. (4.57)
Hence, the singular solutions S
(3)
1s and S
(3)
1s enter the series expansion only if the total
force and torque, respectively, is non-zero.
47.
Multipole Expansion Method in Micromechanics of Composites 143
4.6.2 Single Inclusion Problem
The problem statement is analogous to that in Sect.3.2, with Tξ instead of Tr in
the interface conditions (3.12). The far load in the form of displacement ﬁeld u f ar
and the displacement in the inclusion u(1) are given by the series (3.13) and (3.15),
respectively, where the regular solutions u
(i)
ts (3.6) are replaced with their spher-
oidal counterparts, f(i)
ts . In the case of linear u f ar = E · r, the non-zero expansion
coefﬁcients c
(i)
ts are
c
(3)
00 =
d
3γ0(ν0)
(E11 + E22 + E33), c
(1)
20 =
d
3
(2E33 − E11 − E22), (4.58)
c
(1)
21 = −c
(1)
2,−1 = d (E13 − i E23) , c
(1)
22 = c
(1)
2,−2 = d (E11 − E22 − 2i E12) .
In the matrix domain, u(0) = u f ar + udis, where the disturbance ﬁeld udis(r) is
written as the multipole expansion series
udis(r) =
i,t,s
A
(i)
ts F
(i)
ts (r, d). (4.59)
We substitute (4.59), together with (3.13) and (3.15), into the ﬁrst of conditions
(3.12). By applying (4.52) and (4.53), we get
i,t,s
c
(i)
ts
3
j=1
U M
ji
ts (ξ0, ν0) C
( j)
t+ j−2,s (4.60)
+
i,t,s
A
(i)
ts
3
j=1
UG
ji
ts (ξ0, ν0) C
( j)
t− j+2,s =
i,t,s
d
(i)
ts
3
j=1
U M
ji
ts (ξ0, ν1) C
( j)
t+ j−2,s.
The orthogonality property of the complex-valued vectors C
( j)
ts enables reducing the
vectorial functional equality (4.60) to an inﬁnite set of linear algebraic equations.
Convenient for the computer algebra form of this system is
UGt (ξ0, ν0)At + UMt (ξ0, ν0)ct = UMt (ξ0, ν1)dt (t = 1, 2, . . .); (4.61)
where the vector At contains the unknowns A
(i)
t+i−2,s, the vectors at and dt include
a
(i)
t−i+2,s and d
(i)
t−i+2,s, respectively. Obtaining the second set of equations from the
traction vector continuity condition
TGt (ξ0, ν0)At + TMt (ξ0, ν0)ct = TMt (ξ0, ν1)dt . (4.62)
follows the same way (for more details, see [34]).
48.
144 V. I. Kushch
The solution we obtain is complete and valid for any non-uniform far ﬁeld. For
the polynomial far ﬁeld of order tmax, this solution is exact and conservative, i.e., is
given by the ﬁnite number of terms with t ≤ tmax. This result is consistent with [28];
in particular, tmax = 1 gives us a complete solution of the Eshelby problem. And, to
complete this section, we note that the derived solution is also valid in the limiting
case of inﬁnitely thin oblate spheroid often used to model the penny-shaped cracks.
The normal opening mode stress intensity factor (SIF) KI is deﬁned by
KI = lim
r→0
√
2πrσ33 =
√
πd lim
ξ→1
ξσ33, (4.63)
where r is the distance from the point in the plane z = 0 outside the crack to the
crack’s tip. An asymptotic analysis of the stress ﬁeld near the crack’s tip gives a
series expansion of SIF:
d
π
KI (ϕ)
2μ
=
∞
t=0
t
s=−t
(−1)
(t+s)
2 A
(1)
ts +
is
(t + 1)
A
(2)
t+1,s (4.64)
+
4(1 − ν)
t(2t − 1)
− (1 − 2ν) A
(3)
ts exp (isϕ) ,
where the prime over the internal sum means that it contains only the terms with
(t + s) even. For the details of derivation, see [38].
4.6.3 Re-expansion Formulas for the Lame Solutions
Translation. Let r1 = R + r2 Then,
F
(i)
ts (r1) =
3
j=1
∞
k=0
k
l=−k
η
(i)( j)
tksl (R, d1, d2) f
( j)
kl (r2, d2) , (4.65)
where
η(1)(2)
tksl = η(1)(3)
tksl = η(2)(3)
tksl = 0; η(i)(i)
tksl = ηs−l
t+2−i,k−2+i ; (4.66)
η
(2)(1)
tksl =
s
t
+
l
k
ηs−l
t,k−1 η
(3)(2)
tksl = 2
s
t
+
l
k
ηs−l
t−1,k;
η
(3)(1)
tksl = 2
l
k
s
t
+
l
(k − 1)
+ Ck−2,l − C−(t+1),s ηs−l
t−1,k−1 + (2k − 1)
×
∞
m=0
(−1)m X3
d2
ηs−l
t−1,k+2m − d1(ξ10)2
ηs−l
t,k+2m + d1(ξ20)2
ηs−l
t−1,k+2m+1 .
49.
Multipole Expansion Method in Micromechanics of Composites 145
In (4.66) ηs−l
tk are the expansion coefﬁcients for the scalar spheroidal harmonics Fs
t
(4.13). These, as well as the other (R2R and S2S) expansions have been derived by
[33].
Rotation. The re-expansion formulas for the partial irregular solutions F
(i)
ts due to
rotation of coordinate frame r1 = O12 · r2 are:
F
(i)
ts (r1, d1) =
3
j=1
t+i− j
k=0
k
l=−k
R
(i)( j)
tksl (w12, d1, d2) F
( j)
kl (r2, d2) , (4.67)
where
R
(i)( j)
tksl =
i
α= j
t+i−α
p=k+ j−α
K(1)(i)(α)
t, p+α−i, s (d1) K
(2)(α)( j)
p, k+ j−α,l (d2) S
p−s,p−l
2p (w12) (4.68)
+ δi3δj1(2k − 1)
t
n=k
(ξ10)2
R
(3)(3)
tnsl − (ξ20)2
R
(2)(2)
tnsl
and
K
(β)(i)( j)
tks = 0 for i < j; K
(β)(i)(i)
tks = K
(β)
t−i+2,k−i+2; (4.69)
K
(β)(2)(1)
tks =
s
k
−
s
t
K
(β)
tk , K
(β)(3)(2)
tks = 4(1 − ν)
s
k
−
s
t
K
(β)
t−1,k−1;
K
(β)(3)(1)
tks = C−(k+1),s − C−(t+1),s K
(β)
t−1,k−1 −
s
(k − 1)
K
(β)(3)(2)
tks .
Here, K
(β)
tk are given by the formulas (4.6), β = 1, 2. In (4.67), we keep in mind that
the vectorial functions standing in the opposite sides of equality are written in their
local coordinates and components. These formulas are written for the most general
case d1 = d2 and ξ10 = ξ20. The analogous formulas for the regular solutions are
exact and ﬁnite: for their explicit form, see [34, 39].
4.6.4 FCM and RUC
Now, we have in hands all the necessary theory to solve the elasticity problems for
multiple spheroidal inclusions. We take the displacement ﬁeld in the matrix domain
in the form (3.32), where now multipole expansion of the disturbance caused by p-th
inclusion is written as
u
(p)
dis(rp) =
i,t,s
A
(i)(p)
ts F
(i)
ts (rp, dp). (4.70)
50.
146 V. I. Kushch
Fulﬁlling the interface conditions gives us the linear set of equations similar to (4.61),
(4.62)
UGt (ξq0, ν0)A
(q)
t + UMt (ξq0, ν0) a
(q)
t + c
(q)
t = UMt (ξq0, νq)d
(q)
t ; (4.71)
TGt (ξq0, ν0)A
(q)
t + TMt (ξq0, ν0) a
(q)
t + c
(q)
t = TMt (ξq0, νq)d
(q)
t .
Here, ct is given by (4.58) and a
(q)
t is the contribution of all other inclusions (with
p = q) to the ﬁeld around the qth inclusion:
a
(q)
t =
p=q
∞
k=1
η
(p)(q)
kt A
(p)
k , (4.72)
in scalar form,
a
(i)(q)
ts =
N
p=q
3
j=1
∞
k=0
k
l=−k
A
( j)(p)
kl η
( j)(i)
klts Rpq, dp, dq . (4.73)
Here, we assumed all the spheroids equally oriented: Opq = I. The case of arbitrarily
oriented spheroids is considered elsewhere [39]. By analogy with (3.39)–(3.41),
one can use this model to evaluate the effective stiffness of composite in spirit of
Maxwell’s method.
Extension of this solution to the periodic, RUC type model is analogous to that
for the spherical inclusions and so we do not repeat it here. In fact, it mostly consists
in replacing the expansion coefﬁcients (4.66) with their periodic counterparts in the
matrix of linear system (4.71).
4.6.5 Effective Stiffness Tensor
The effective stiffness tensor C∗ of composite is given by (1.10). In view of the
displacement ﬁeld periodicity, averaging the strain in composite with spheroidal
inclusions follows the same way as in the spherical case and yields ε = E. The
macroscopic stress σ is given by Eq.(1.13) where integration is made now over the
spheroidal surfaces Sq : ξq = ξq0. The integration procedure closely resembles that
exposed in Sect.3 and is straightforward although somewhat laborious.
An alternate approach to obtaining the expressions for effective properties was
discussed already in this Section, in the conductivity context. This approach extends
to the elasticity problem: namely, an expression for the macroscopic stress in spher-
ical particle composite (3.51) transforms to the analogous formula for the aligned
spheroidal particle composite by taking into account that for d → 0
V(1)
00 (r, d) ≈ N0U(1)
00 (r); V(3)
2,s(r, d) ≈ NsU(3)
2,s(r);
51.
Multipole Expansion Method in Micromechanics of Composites 147
where the scaling factor Ns = (−1)sd2/3. By inserting this factor into (3.51) we
obtain immediately the desired formulas:
σ11 + σ22 + σ33
3k0
= (E11 + E22 + E33) + 1 +
4μ0
3k0
N
q=1
dp A
(1)(q)
00 ;
(4.74)
2 σ33 − σ11 − σ22
2μ0
= (2E33 − E11 − E22) − 4 (1 − ν0)
N
q=1
dp A
(3)(q)
20 ;
σ11 − σ22 − 2i σ12
2μ0
= (E11 − E22 − 2iE12) − 8 (1 − ν0)
N
q=1
dp A
(3)(q)
22 ;
σ13 − i σ23
2μ0
= (E13 − iE23) + 2 (1 − ν0)
N
q=1
dp A
(3)(q)
21 .
where dp = 4π dp
2
/3a2 and k = 2μ(1+ν)
3(1−2ν) .
5 Spherical Particles Reinforced Composite with
Transversely-Isotropic Phases
In the Cartesian coordinate system Ox1x2x3 with Ox3 axis being the anisotropy
axis of transversely isotropic material, an explicit form of the generalized Hooke’s
law is
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
σ11
σ22
σ33
σ23
σ13
σ12
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
=
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
C11 C12 C13 0 0 0
C12 C11 C13 0 0 0
C13 C13 C33 0 0 0
0 0 0 2C44 0 0
0 0 0 0 2C44 0
0 0 0 0 0 (C11 − C12)
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
ε11
ε22
ε33
ε23
ε13
ε12
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
. (5.1)
Here, two-indices notation Ci j is adopted. The components of stress tensor σ satisfy
the equilibrium equations ∇ · σ = 0 and the small elastic strain tensor ε is related to
the displacement vector u by ε = 1
2 ∇u + (∇u)T
.
5.1 Background Theory
Based on representation of general solution in terms of three potential functions [70],
Kushch [43] has introduced the following, full for ν1 = ν2 set of regular vectorial
solutions v
( j)
ts :
52.
148 V. I. Kushch
v
( j)
ts (r) = f s−1
t (rj , dj )e1 − f s+1
t (rj , dj )e2 +
kj
√
νj
f s
t (rj , dj )e3 ( j = 1, 2);
(5.2)
v
(3)
ts (r) = f s−1
t (r3, d3)e1 + f s+1
t (r3, d3)e2; t = 0, 1, 2, . . . ; |s| ≤ t + 1.
In (5.2), ν3 = 2C44/ (C11 − C12) whereas ν1 and ν2 are the roots of equation
C11C44ν2
− (C44)2
− C11C33 − (C13 + C44)2
ν + C33C44 = 0. (5.3)
Expressions of k1 and k2 are
kj =
C11νj − C44
C13 + C44
=
νj (C13 + C44)
C33 − νj C44
, j = 1, 2 . (5.4)
The modiﬁed Cartesian rj and prolate spheroidal coordinates ξj , ηj , ϕj are given
for νj < 1 by
x1 + ix2 = x1 j + ix2 j = dj
¯ξj ¯ηj exp(iϕj ), x3 =
√
νj x3 j =
√
νj dj ξj ηj ; (5.5)
In the case νj > 1, the oblate spheroidal coordinates must be used. The system (5.5)
is chosen in a way that ξj = ξj0 = const at the spherical surface r = R; i.e., S is
the ξ-coordinate surface of (5.5). We provide this by deﬁning
dj = R/ξj0, ξj0 = νj / νj − 1 . (5.6)
In this case, moreover, we have ηj = θ and ϕj = ϕ for r = R, where (r, θ, ϕ) are
the ordinary spherical coordinates corresponding to the Cartesian ones (x1, x2, x3).
This is the key point: no matter how complicated solution in the bulk is, at
the interface we get the linear combination of regular spherical harmonics
Ys
t (θ, ϕ). Under this circumstance, fulﬁlling the contact conditions at interface
is straightforward.
The explicit form of the irregular vectorial solutions V
( j)
ts is given by the Eq.(5.2),
with the replace f s
t by Fs
t . According to [23], Fs
t = f s
t ≡ 0 for |s| > t. This
condition makes it impossible to represent some irregular solutions in the form (5.2).
To resolve this issue, Kushch [43] has introduced the following, additional to (4.4)
functions of the form
Ft+k
t (r, d) =
1
(2t + k)!
Qt+k
t (ξ) Pt+k
t (η) exp [i (t + k) ϕ] , (5.7)
53.
Multipole Expansion Method in Micromechanics of Composites 149
(k = 0, 1, 2, . . .) where
Pt+k
t (p) =
(2t + k)!
(1 − p2)(t+k)/2
1
p
1
p
· · ·
1
p
t+k
Pt (p) (dp)t+k
=
(2t + k)!
(1 − p2)(t+k)/2
It+k (5.8)
for 0 ≤ p ≤ 1; for p < 0, Pt+k
t (p) = (−1)k Pt+k
t (−p). It is straightforward
to show that the functions (5.7) are the irregular solutions of Laplace equation. In
contrast to (4.4), they are discontinuous at x3 = 0. In the general series solution,
however, these breaks cancel each other and give the continuous and differentiable
expressions of the displacement and stress ﬁelds. Remarkably, the functions Ft+k
t
are introduced in a way that for them are valid all the principal results including the
re-expansion formulas (4.13) and (4.15).
At the spherical surface r = R, the functions V
(i)
ts and v
(i)
ts can be written in the
compact form as
V(i)
ts
S
=
3
j=1
UG
ji
ts C
( j)
ts , v(i)
ts
S
=
3
j=1
U M
ji
ts C
( j)
ts , (5.9)
where C
( j)
ts (θ, ϕ) is deﬁned in (4.51). In (5.9), the matrix
UGts = UG
i j
ts =
⎛
⎜
⎜
⎝
Qs−1
t (ξ10) Qs−1
t (ξ20) Qs−1
t (ξ30)
−Qs+1
t (ξ10) −Qs+1
t (ξ20) Qs+1
t (ξ30)
k1√
ν1
Qs
t (ξ10) k2√
ν2
Qs
t (ξ20) 0
⎞
⎟
⎟
⎠ ; (5.10)
UMts has the form (5.10), where Qs
t are replaced with Ps
t .
To satisfy the stress boundary conditions, we need the similar representation for
the traction vector Tn = σ · n. For the explicit expressions of Tn(v
( j)
ts ) at the surface
S, see [43]. These and analogous expressions for Tn(V
( j)
ts ) also can be written in the
compact form
Tn(V
( j)
ts )
S
=
3
j=1
T G
ji
ts C
( j)
ts , Tn(v
( j)
ts )
S
=
3
j=1
T M
ji
ts C
( j)
ts . (5.11)
For the deﬁniteness sake, we assume here and below ν1 = ν2. In the case of equal
roots ν1 = ν2, solution (5.2) is not general because of f
(1)
ts ≡ f
(2)
ts . In this case, to get
a complete set of independent solutions, v
(2)
ts can be taken in the form [43]
54.
150 V. I. Kushch
v
(2)
ts (r) = d1 x3∇ −
C13 + 3C44
C13 + C44
i3 f s
t (r1, d1) +
√
ν1d1 (ξ10)2
∇ f s
t−1(r1, d1).
(5.12)
For the expression of the corresponding traction vector, see [70].
5.2 Series Solution
Let us consider an inﬁnite solid with a single spherical inclusion of radius R
embedded. The matrix and inclusion are made from transversely isotropic materials
and perfectly bonded:
u+
− u−
S
= 0; Tn u+
− Tn u−
S
= 0. (5.13)
InthisSection,alltheparametersassociatedwiththematrixandinclusionaredenoted
by the superscript “−” and “+”, respectively. We assume the anisotropy axes of
both the matrix and inclusion materials to be arbitrarily oriented and introduce
the material-related Cartesian coordinate systems Ox−
1 x−
2 x−
3 and Ox+
1 x+
2 x+
3 with
common origin in the center of inclusion. The point coordinates and the vector
components in these coordinate systems are related by
x+
i = Oi j x−
j , u+
i = Oi j u−
j (5.14)
where O is the rotation matrix. Transformation of the vectors ii uses the formula
i+
i = Ω∗
i j i−
j , where O∗
= D−1
OD and D =
⎛
⎝
1 1 0
−i i 0
0 0 1
⎞
⎠ . (5.15)
The displacement ﬁeld within the inclusion u+ can be expanded into a series over
the regular solutions v
( j)
ts (5.2):
u+
=
j,t,s
d
( j)
ts v
( j)
ts r+
,
⎛
⎝
j,t,s
=
3
j=1
∞
t=0 |s|≤t+1
⎞
⎠ (5.16)
whered
( j)
ts aretheexpansioncoefﬁcientstobedeterminedfromthecontactconditions
(5.13). The displacement vector in the matrix domain is a sum of far ﬁeld u f ar =
E · r− and disturbance udis whose multipole type expansion in terms of V
( j)
ts is
given by
u−
= u f ar + udis = E · r−
+
j,t,s
A
( j)
ts V
( j)
ts r−
. (5.17)
55.
Multipole Expansion Method in Micromechanics of Composites 151
Expression (5.16) is ready for use; the similar expansion of u f ar follows from
(5.2). Speciﬁcally,
u f ar =
j,t,s
c
( j)
ts v
( j)
ts r−
, (5.18)
where
c
(1)
10 =
d−
1 ν−
1
k−
1 ν−
2 − k−
2 ν−
1
E33ν−
2 + k−
2 (E11 + E22) ;
c
(1)
11 = −c
(1)
1, −1 =
d−
1 ν−
1
k−
1
(E13 − i E23) ;
c(1)
12 = c(1)
1, −2 = (E11 − E22 − 2i E12) ; (5.19)
c
(2)
10 = −
ν−
2 d−
2
k−
1 ν−
2 − k−
2 ν−
1
E33ν−
1 + k−
1 (E11 + E22) ;
c(3)
11 = c(3)
1, −1 =
ν−
3 d−
3
k−
1
(1 − k−
1 ) (E13 − i E23) ;
all other coefﬁcients c
(i)
ts are equal to zero.
We note ﬁrst that the functions V
(i)
0s are the fundamental solutions representing
actionofthepointbodyforcesinaninﬁnitesolid.Becausenobodyforcesissuggested
in the problem statement, we get immediately A
(i)
0s ≡ 0. The remaining coefﬁcients
A
(i)
ts and D
(i)
ts will be determined from the interface boundary conditions (5.13). We
use (5.9) to write
u−
=
j,t,l
3
α=1
UG
jα−
tl A(α)
tl + U M
jα−
tl e(α)
tl C
( j)
tl θ−
, ϕ−
(5.20)
and
u+
=
i,t,s
3
α=1
U Miα+
ts d(α)
ts C(i)
ts θ+
, ϕ+
. (5.21)
Note that u− (5.20) and u+ (5.21) are still written in the different coordinate
systems. Therefore, before substituting them into (5.13), u+ has to be expressed
in terms of the variables θ−, ϕ− and vectors e−
j . For this purpose, we apply the
Bateman’s transformation formula of the surface spherical harmonics due to rotation
of coordinate basis [3] and (5.15) to derive:
56.
152 V. I. Kushch
C
(i)
ts (θ+
, ϕ+
) =
3
j=1
Ω∗
i j
|l j |≤t+1
(t + lj )!
(t + si )!
S
t−si ,t−l j
2t (w) C
( j)
tl θ−
, ϕ−
, (5.22)
where Ssl
2t are the spherical harmonics in four-dimensional space and w is the vector
of Euler’s parameters related to the rotation matrix O by (4.27). By substitution
(5.22) into (5.21), we get
u+
=
j,t,l
⎡
⎣
3
i=1
O∗
i j
|s|≤t+1
(t + lj )!
(t + si )!
S
t−si ,t−l j
2t (w)
3
α=1
U Miα+
ts d(α)
ts
⎤
⎦ C
( j)
tl θ−
, ϕ−
.
(5.23)
Now, we put u− (5.20) and transformed expression of u+ (5.23) into the ﬁrst of
conditions (5.13) and make use of the orthogonality property of spherical harmonics
χs
t on the surface S to decompose vectorial functional equality u+ = u− into a set
of linear algebraic equations. It is written in the matrix-vector form as
UG−
tl · Atl + UM−
tl · etl =
|s|≤t+1
UM∗
tsl · dts, (5.24)
t = 0, 1, 2, . . . ; |l| ≤ t + 1;
where
UM∗
tsl = WtslUM+
ts, W
ji
tsl = O∗
i j
(t + lj )!
(t + si )!
S
t−si ,t−l j
2t (w) , (5.25)
Atl = A
(i)
tl
T
, dtl = d
(i)
tl
T
, etl = e
(i)
tl
T
.
Obtainingthesecondsetofequationsfollowsthesameprocedurewhere,insteadof
(5.9), the representation (5.11) of the normal traction vectors Tn(v
( j)
ts ) and Tn(V
( j)
ts )
on the surface r = R should be used. After transformations, we obtain
TG−
tl · Atl + TM−
tl · etl =
|s|≤t+1
TM∗
tsl · dts, (5.26)
where TM∗
tsl = WtslTM+
ts. Form of the matrices TGtl and TMtl is clear form
(5.11). The Eqs.(5.24) and (5.26) together form a complete set of linear equations
from where A
(i)
ts and d
(i)
ts can be determined. For more details, see [43].
5.3 FCM and RUC
Let us consider now an unbounded domain containing N non-touching spherical
particles of radius Rq with the centres located in the points Oq, q = 1, 2, . . . , N and
57.
Multipole Expansion Method in Micromechanics of Composites 153
the elastic stiffness tensors C+
q . We introduce the local material-related coordinate
systems Oqx+
1qx+
2qx+
3q which origin and orientation with respect to the global Carte-
sian coordinate system Ox−
1 y−z− is deﬁned by the vector Rq and the rotation matrix
Oq. The matrix-inclusion interface boundary conditions (q = 1, 2, . . . , N) are
u+
q − u−
Sq
= 0; Tn u+
q − Tn u−
Sq
= 0; (5.27)
the stress state of the heterogeneous solid is governed, as before, by the linear far
displacement ﬁeld.
In (5.27), u+
q is the displacement vector in the volume of qth inclusion: by analogy
with (5.16),
u+
q =
j,t,s
d
(q)( j)
ts v
( j)
ts r+
q , (5.28)
The displacement vector u− in the matrix domain is written as a superposition of
linear far ﬁeld and the disturbance ﬁelds induced by each separate inclusion (3.32):
In turn, the disturbance term u
(p)
dis(r) allows the multipole expansion in the form
u
(p)
dis r−
p =
j,t,s
A
(p)( j)
ts V
( j)
ts r−
p , (5.29)
where A
(p)( j)
ts as well as d
(q)( j)
ts in (5.28) are the unknown coefﬁcients. The limiting
behavior of u− is u− → E · r with r → ∞.
The separate terms of the superposition sum are written in the different coordinate
systems. To enable application the procedure described in the previous Section, we
need to express u− in variables of the local coordinate system. This transform uses
the re-expansion formulae for the irregular vectorial solutions V
( j)
ts due to translation
of coordinate system:
V
( j)
ts r−
p =
∞
k=0 |l|≤k+1
ηtk,s−l Rpq, d−
pj , d−
qj v
( j)
kl r−
q , (5.30)
t = 0, 1, 2, . . . ; |s| ≤ t + 1;
The formulas (5.30) follow directly from the corresponding result for the scalar
harmonic functions Fs
t (4.13). The explicit form of the coefﬁcients ηtks is given by
the formulas (4.16), (4.22) or (4.24).
We apply (5.30) to all the sum terms (5.29) but that one with p = q written
initially in the variables of this local coordinate system. After some algebra, we ﬁnd
u−
(r−
q ) =
j,t,s
A
(q)( j)
ts V
( j)
ts r−
q + a
(q)( j)
ts + c
(q)( j)
ts v
( j)
ts r−
, (5.31)
58.
154 V. I. Kushch
where
a
(q)( j)
ts =
∞
k=0 |l|≤k+1
N
p=1p=q
ηkt,l−s Rpq, d−
pj , d−
qj A
(p)( j)
kl (5.32)
and c
(q)( j)
ts are the expansion coefﬁcients of the linear part of u− given by the formula
(5.19), with replace d−
j to d−
qj = Rq/ξ−
j0.
After the local expansion of u− in the vicinity of the point Oq was found, the
remaining part of solving procedure follows the described above way. In fact, by
applying the re-expansion formula (5.30) we reduced the initial, multiple inclusion
problem to a coupled set of N problems for a solid with a single inclusion in the
non-uniform far ﬁeld. The resulting inﬁnite set of linear algebraic equations is
UG
(q)−
tl · A
(q)
tl + UM
(q)−
tl · a
(q)
tl + c
(q)
tl =
|s|≤t+1
UM
(q)∗
tsl · d
(q)
ts ,
TG
(q)−
tl · A
(q)
tl + TM
(q)−
tl · a
(q)
tl + c
(q)
tl =
|s|≤t+1
TM
(q)∗
tsl · d
(q)
ts , (5.33)
q = 1, 2, . . . , N; t = 0, 1, 2, . . . ; |l| ≤ t + 1;
where a
(q)
tl = a
(q)( j)
ts , a
(q)( j)
ts , a
(q)( j)
ts
T
and a
(q)( j)
ts are given by (5.32). Its approx-
imate solution can be obtained by the truncation method, when the unknowns and
equations with t ≤ tmax only are retained in the (5.33). The solution is convergent
for tmax → ∞ provided that the non-touching conditions Rpq > Rp + Rq hold
true for each pair of inclusions. Thus, (5.33) can be solved for A
(q)
tl and d
(q)
ts with
any desirable accuracy by taking tmax sufﬁciently large.
The above formalism applies also to solution of the RUC model problem. To this
end, it is sufﬁcient to replace V
( j)
ts with its periodic counterpart
V
∗( j)
ts (r) =
k
V
( j)
ts (r − ak) (5.34)
in (5.29) and a
(q)
ts (5.32)—with
a
(q)
ts =
∞
k=0 |l|≤k+1
N
p=1
η∗
kt,l−s Rpq, d−
pj , d−
qj A
(p)
kl , (5.35)
where η∗
kts is the lattice sum (4.36). These sums appear in solution of the conductivity
problem for a composite with transversely isotropic phases [35]. There, the conver-
gence rate of the series (4.36) is discussed and the fast summation technique has
been proposed. The only difference here is the extended variation range of indices s
59.
Multipole Expansion Method in Micromechanics of Composites 155
and l. These series converge for all indices in the range |s| ≤ t + 1 and |l| ≤ k + 1
provided the inclusions do not overlap.
5.4 Effective Stiffness Tensor
The macroscopic elastic stiffness tensor is deﬁned by (1.10) where we consider RUC
a representative volume element of composite. In this case, integration of the local
strain and stress ﬁelds can be done analytically. The components of the effective
stiffness tensor are found as C∗
i jkl = σi j , where the stress σ is calculated for
εkl = 1, εk l = 0 (k = k , l = l ). It has been shown in Chap. 5 that E has a
meaning of macroscopic strain tensor. Hence, C∗
i jkl = σi j Emn=δmkδnl .
To compute the macroscopic stress (1.12), we employ Eq.(1.13) valid for the
arbitrary orientation of inclusions and general type anisotropy of constituents. Inte-
gration in (1.13) has to be done over the matrix volume only: with the local series
expansions (5.31) taken into account, this task is straightforward. Moreover, it fol-
lows from the Betti’s theorem that these integrals are equal to zero for all regular
solutions v
( j)
ts . Among the singular solutions V
( j)
ts , only those with t = 1 contribute
to σi j . After some algebra analogous to that in Sect.8.1, we get the exact explicit
formulas [44]:
σ11 = C−
1k εkk − C−
11 ν−
1 A
(1)
10 + ν−
2 A
(2)
10 +
C−
44
2
(1 + k−
j )
ν−
j
ReA
( j)
12 ;
(5.36)
σ22 = C−
2k εkk − C−
22 ν−
1 A
(1)
10 + ν−
2 A
(2)
10 −
C−
44
2
(1 + k−
j )
ν−
j
ReA
( j)
12 ;
σ33 = C−
3k εkk − C−
33
⎛
⎝
k−
1
ν−
1
A(1)
10 +
k−
2
ν−
2
A(2)
10
⎞
⎠ ;
σ12 = C−
66 ε12 +
C−
44
2
(1 + k−
j )
ν−
j
ImA
( j)
12 ;
σ13 − i σ23 = C−
44 ( ε13 − i ε23 )
+
C−
44
2
(1 + 2k−
1 )A
(1)
11 + (1 + 2k−
2 )A
(2)
11 − A
(3)
11 ;
where
A
( j)
1s =
4π
3a3
N
q=1
d−
q
2
R3
q A
(q)( j)
1s
60.
156 V. I. Kushch
Again, as expected, these formulas involve only the dipole moment of the disturbance
ﬁeld caused by each inclusion contained in RUC.
6 Fibrous Composite with Interface Cracks
In this and subsequent Sections, we consider a series of two-dimensional (2D) mul-
tiple inclusion problems. This geometry can be viewed as the cross-section of uni-
directional ﬁbrous composite (FRC) for which, in the case of transverse loading,
the 2D model is adequate. In 2D, the powerful method of complex potentials (e.g.,
[62, 67]) provides an efﬁcient analysis of a wide range of the boundary value prob-
lems including those stated on the multiply-connected domains. This fact makes the
method complex potentials very useful in micromechanics of ﬁbrous composites
and, in particular, in 2D version of Multipole Expansion Method ([6, 17, 24], among
others).
6.1 Background Theory
In 2D plane, the point (x1, x2) it conveniently associated with the complex variable
z = x1 + ix2. In the exponential form, z = ρ exp(iθ), where the modulus ρ = |z|
and argument θ = Arg(z) are the polar coordinates corresponding to the Cartesian
x1 and x2. The complex-valued, analytical in a vicinity of the point z0 function f (z)
can be expanded into Laurent series
f (z) =
∞
∞
an (z − z0)n
, (6.1)
being inherently the 2D multipole expansion of f (z). The series (6.1) contains the
negative powers only if z0 is the singularity point of f (z). By direct analogy with
(2.3), the powers of z can be regarded as the solid harmonics, regular for n ≥ 0 and
singular otherwise. Moreover, at the circular line ρ = R, we get zn = Rn exp(inθ)
where Fourier harmonics exp(inθ) are viewed as the surface harmonics.
We also mention the re-expansion formulas analogous to (2.20)–(2.22). The most
famous one is the Newtonian binomial:
(z + Z)n
=
n
k=0
n
k
Zn−k
zk
, (6.2)
where
n
k
= n!/k!(n − k)! are the binomial coefﬁcients. In our context, (6.2) can
be viewed as translation of regular solid harmonics (R2R). The local expansion of
61.
Multipole Expansion Method in Micromechanics of Composites 157
singular harmonics (S2R) takes the form
(z + Z)−n
=
∞
k=0
n + k − 1
k
Z−(n+k)
zk
, |z| < |Z| ; (6.3)
translation of singular harmonics (S2S) is given by
(z + Z)−n
=
∞
k=n
k − 1
n − 1
Zk−n
z−k
, |z| > |Z| . (6.4)
These results are sufﬁcient to solve the conductivity problem for a multiply-
connecteddomainwithcircularboundariesinaway,quiteanalogoustothatdescribed
in Sect.1. This multipole solution can be further extended, in obvious manner, to the
periodic and RUC type inﬁnite arrays of inclusions, etc. For the details, we refer to
[17, 69], among others, where this work was done. In what follows, we focus on the
elasticity problem.
6.2 2D RUC Geometry
Two-dimensional RUC model of unidirectional FRC (Fig.2) contains the centers of
N aligned in x3-direction and circular in cross-section ﬁbers. Within a cell, the ﬁbers
are placed randomly but without overlapping. The ﬁbers shown by the dashed line
do not belong to the cell while occupy a certain area within it. The whole composite
bulk is obtained by replicating the cell in two orthogonal directions. Geometry of the
cell is deﬁned by its side length a and the coordinates (X1q, X2q) of qth ﬁber center
(q = 1, 2, . . . , N) in the global Cartesian coordinate system Ox1x2. For simplicity
Fig. 2 RUC model of ﬁbrous
composite
62.
158 V. I. Kushch
sake, we assume the ﬁbers equally sized, of radius R = 1, and made from the same
material. The ﬁber volume content is c = Nπ/a2.
We introduce the local, ﬁber-related coordinate systems Oqx1qx2q with origins
in Zq and the associated complex variables zq = x1q + ix2q. The global complex
variable z = zq +Zq, where Zq = X1q +iX2q, q = 1, 2, . . . , N. The local variables
zp = z − Z p relate each other by zq = zp − Z pq. Here, Z pq = X1pq + iX2pq is
the complex number determining relative position of the ﬁbers with indices p and
q inside the cell. Also, we introduce the complex number Z∗
pq deﬁning the minimal
distance between the arrays of ﬁbers with indices p and q. Here, we do not assume
that the both ﬁbers are belonging to the same RUC, see Fig.2. In these notations,
the non-touching condition of any two ﬁbers in entire composite space is written as
Z∗
pq > 2R.
This model is thoroughly studied ([9, 17, 22, 47, 69], among many others) in
the case of perfect matrix-ﬁber interfaces Lq, q = 1, 2, . . . , N. Here, we consider
more general problem where one part L
(q)
c of interface Lq deﬁned by the endpoints
z
(q)
j = exp(iθ
(q)
j ) ( j = 1, 2) (Fig.3) is separated and another part L
(q)
b = LqL
(q)
c
is perfectly bonded.
To simplify the subsequent algebra, we introduce the crack-related complex
variables ζq = zq/z
(q)
c , where z
(q)
c = exp(iθ
(q)
c ) is the crack midpoint: θ
(q)
c =
(θ
(q)
1 +θ
(q)
2 )/2. The interface crack size is measured by the angle θ
(q)
2 −θ
(q)
1 = 2θ
(q)
d ;
in the prefect bonding case, θ
(q)
d = 0.
6.3 Model Problem
We consider the plane strain problem (u3 = 0). Both the matrix and ﬁber materials
are taken isotropic and linearly elastic. The complex displacement u = u1 + iu2
corresponds to the Cartesian displacement vector u = (u1, u2)T
. We denote u = u0
Fig. 3 A ﬁber with interface
crack
x1q
x2q
z
1
(q)
z2
(q)
2q
Lc
( )q
Lb
(q)
q
d
(q)
63.
Multipole Expansion Method in Micromechanics of Composites 159
in the matrix material with a shear modulus μ0 and Poisson ratio ν0; uq, μ1 and ν1
refer to displacement and elastic moduli, respectively, of qth ﬁber. The components
of the stress tensor σ = σi j are given by
σi j
2μ
= εi j + δi j
(3 − κ)
2(κ − 1)
(ε11 + ε22) , (6.5)
where εi j are the components of the strain tensor and κ = 3−4ν for the plane strain
problem. In the adopted by us open-crack model, the traction-free crack surface is
assumed. The relevant boundary conditions are:
[[u]]L
(q)
b
= [[Tr ]]L
(q)
b
= 0, Tr |L
(q)
c
= 0, q = 1, 2, . . . , N. (6.6)
where Tr = σrr + iσrθ is the complex traction at the circular interface L(q).
We consider the macroscopically uniform stress state of the composite bulk, which
implies constancy of the volume-averaged strain E = Ei j = εi j and stress
S = Si j = σi j tensors, where f = A−1
A f d A and A = a2 is the cell area.
We take E a load governing parameter. Under the assumptions made, periodicity
of geometry gives rise to periodicity of local strain and stress ﬁelds ([10, 17, 68];
among others)
εi j (z + a) = εi j (z + ia) = εi j (z) ; σi j (z + a) = σi j (z + ia) = σi j (z) . (6.7)
The corresponding to (6.7) displacement ﬁeld is a quasi-periodic function of
coordinates:
u(z + a) − u(z) = (E11 + iE12)a; u(z + ia) − u(z) = (E12 + iE22)a. (6.8)
Hence, (6.8) can be decomposed into a sum of the linear part u∞ being the far ﬁeld
determined entirely by the E tensor and the periodic disturbance ﬁeld caused by the
inhomogeneities.
6.4 Displacement Solution
The general displacement solution in a vicinity of the partially debonded ﬁber (6.6)
can be written in the form (e.g., [51])
2μj u j (ζ) = κj ϕj (ζ) − ζ −
1
ζ
ϕj (ζ) − ωj
1
ζ
, (6.9)
j = 0 for matrix and j = 1 for ﬁber. Representation (6.9) is valid for any inhomoge-
neous far ﬁeld and so can be applied equally to the single- and multiple-ﬁber problem.
64.
160 V. I. Kushch
In (6.9), ζ is the complex plane variable, ϕj and ωj are the complex potentials and
κj = 3 − 4νj . Also, the prime means a derivative with respect to the argument
and overbar means a complex conjugate. Expression (6.9) is advantageous in that
it simpliﬁes greatly at the circle L deﬁned by the condition |z| = 1. The complex
interface traction Tr = σrr + iσrθ also takes a simple form for t ∈ L, in terms of the
derivative complex potentials ϕ (z) and ω (z).
The potentials ϕr and ωr of the regular in a vicinity of the point z = 0 displacement
ﬁeld u = ur (z) are given by power series
ϕr (z) =
∞
n=0
an zn
, ωr (z) =
1
n=−∞
cn zn
. (6.10)
Provided ur (t) is known, the series expansion coefﬁcients an and cn are given by
κak − δk1a1 = Ik , k > 0; ck = −Ik, k < 0; c1 = a1; (6.11)
where δkl is the Kronecker delta and Ik are the Fourier coefﬁcients
Ik =
2μ
2π
2π
0
ur (t)t−k
dθ. (6.12)
6.5 Single Partially Debonded Fiber
Kushch et al. [51] have suggested the following form of the potentials ϕj and ωj in
(6.9) for the matrix and ﬁber area, respectively:
ϕ0(ζ) =
(1 − α)
2
f (ζ) +
(1 − β)
2
h(ζ)Rλ(ζ); (6.13)
ω0(ζ) = −
(1 − α)
2
f (ζ) +
(1 + β)
2
h(ζ)Rλ(ζ);
ϕ1(ζ) =
(1 + α)
2
f (ζ) +
(1 + β)
2
h(ζ)Rλ(ζ);
ω1(ζ) = −
(1 + α)
2
f (ζ) +
(1 − β)
2
h(ζ)Rλ(ζ).
Here,
α =
μ1(κ0 + 1) − μ0(κ1 + 1)
μ1(κ0 + 1) + μ0(κ1 + 1)
, β =
μ1(κ0 − 1) − μ0(κ1 − 1)
μ1(κ0 + 1) + μ0(κ1 + 1)
(6.14)
are known as the bi-material constants [12],
65.
Multipole Expansion Method in Micromechanics of Composites 161
Rλ(ζ) = (ζ − ζd)
1
2 +iλ
(ζ − ζd)
1
2 −iλ
, (6.15)
f (ζ) and h(ζ) are the analytical functions to be found. In (6.15), ζd = exp(iθd) and
λ = − log 1−β
1+β /2π. The boundary conditions (6.6) are fulﬁlled exactly provided
the potentials ϕj and ωj taken in the form (6.13). The solution (6.9), (6.13) is valid
for the arbitrary non-uniform far ﬁeld ur = u(ϕr , ωr ) considered as input parameter.
The potentials f (ζ) and h(ζ) in (6.13) are written as Laurent series:
f (ζ) =
k
fk ζk
, h(ζ) =
k
hk ζk
. (6.16)
The fk coefﬁcients are given by the simple formulas
fk = −ck, k < 0; fk = ak, k > 1; f1 =
ReM1
M2 + M3
+ i
ImM1
M2 − M3
; (6.17)
for the explicit expression of Mj , see [51]. The hk coefﬁcients are given by the series
hk =
(1 + α)
(1 − β)
∞
l=k+1
Xl−k−1(ζd, −λ)al, k > 0; (6.18)
hk =
(1 + α)
(1 + β)
ζd
−2iλ
k
l=−∞
Xk−l(ζd, λ)cl, k < 0;
where
Xn(ζd, λ) = (−1)n
n
k=0
Gk(λ)Gn−k(λ)ζ2k−n
d , Gk(λ) =
k
j=1
1 + 2iλ
2 j
− 1 .
(6.19)
6.6 Finite Array of Partially Debonded Fibers
In accordance with the superposition principle, we write the total displacement ﬁeld
u0 in the matrix domain as a sum of the far ﬁeld u∞ and the disturbance ﬁelds u
(p)
s
caused by each individual ﬁber:
u0(z) = u∞
(z) + us(z), us(z) =
N
p=1
z
(p)
c u
(p)
s (ζp). (6.20)
66.
162 V. I. Kushch
In (6.20), ζp = zp/z
(p)
c ; the disturbance displacements are summed up in the global
coordinate system. We divide the local expansion of u0(z) in a vicinity of qth ﬁber
into the regular u
(q)
r and singular u
(q)
s parts:
u0(ζq) = u
(q)
r (ζq) + u
(q)
s (ζq), (6.21)
Here, u0(ζq) and u
(q)
r (ζq) are given by (6.9), with the potentials (6.13) and (6.10),
respectively. The disturbance ﬁeld vanishes at inﬁnity: u
(q)
s (ζq) → 0 for ζq → ∞.
The regular part u
(q)
r (ζq) is a sum of the far ﬁeld and the disturbance ﬁelds from all
ﬁbers excluding that one with p = q:
z
(q)
c u
(q)
r (ζq) = u∞
(z) +
N
p=q
z
(p)
c u
(p)
s (ζp). (6.22)
Provided the right hand side of (6.22) is known, the u
(q)
r series expansion coefﬁ-
cients a
(q)
k and c
(q)
k can be found from (6.11) where, in view of (6.22), Ik (6.12) are
calculated by integrating along the interface Lq:
I
(q)
k =
2μ0
2πz
(q)
c
2π
0
⎧
⎨
⎩
u∞
(z) +
N
p=q
z
(p)
c u0 ζp − u
(p)
r ζp
⎫
⎬
⎭
t−k
q dθq, (6.23)
− ∞ < k < ∞, q = 1, 2, . . . , N.
The Eqs.(6.23), (6.11) and (6.17), (6.18) taken together form an inﬁnite system of
linear algebraic equations, from where all the expansion coefﬁcients are determined
uniquely provided u∞ is known.
6.6.1 Evaluation of the Integrals in (6.23)
The integrals entering (6.23) can be evaluated either analytically or numerically. In
what follows, u∞(z) is assumed to be linear function of coordinates, i.e.,
u∞
(z) = Γ1z − Γ2z. (6.24)
where Γ1 and Γ2 are the arbitrary complex constants. Its analytical integration is
elementary and yields
67.
Multipole Expansion Method in Micromechanics of Composites 163
I
(q)
k =
2μ0
2πz
(q)
c
2π
0
u∞
(Zq + z
(q)
c tq)t−k
q dθq =
⎧
⎪⎪⎨
⎪⎪⎩
−2μ0Γ2 z
(q)
c
−2
, k = −1;
2μ0u∞(Zq)/z
(q)
c , k = 0;
2μ0Γ1, k = 1;
(6.25)
and I
(q)
k ≡ 0 otherwise.
Numerical integration is straightforward but not necessarily the perfect way of
evaluating the sum terms in (6.23). First, computational cost of this procedure is rela-
tively high. Second, the fact is that with Z pq (and, hence, ζp) increase, u0 ζp tends
to u
(p)
r ζp . This case requires a special attention: evaluation of u
(p)
s by subtraction
of two close numbers is not advisable because it may lead to substantial numerical
error. To avoid this problem, we derive an asymptotic expansion of u
(p)
s using the
following Laurent series [51]:
h(ζ)Rλ(ζ) =
n g
(1)
n ζn, |ζ| > 1;
n g
(2)
n ζn, |ζ| < 1;
(6.26)
In (6.26),
g(1)
n =
∞
m=0
Rm(ζd, λ)hn+m−1, g(2)
n = −(ζd)2iλ
∞
m=0
Rm(ζd, −λ)hn−m, (6.27)
where
Rn(ζd, λ) = (−1)n
n
k=0
Hk(λ)Hn−k(λ)ζ2k−n
d , Hk(λ) =
k
j=1
3 + 2iλ
2 j
− 1 .
(6.28)
In fact, it sufﬁces to derive the asymptotic expansion of the singular potentials
ϕ
(p)
s = ϕ0 − ϕ
(p)
r and ω
(p)
s = ω0 − ω
(p)
r . By combining the formulas (6.13), (6.26)
(6.10) and (6.17), one ﬁnds
ϕ
(p)
s ζp =
(1 − α)
2
f (ζp) +
(1 − β)
2
h(ζp)Rλ(ζp) −
∞
n=0
a
(p)
n ζn
p (6.29)
=
∞
n=1
a
(p)
−n ζ−n
p ,
where
a
(p)
−n =
(1 − α)
2
f
(p)
n +
(1 − β)
2
g
(1)(p)
n (n = 1, 2, . . .). (6.30)
68.
164 V. I. Kushch
Analogously,
ω
(p)
s ζp =
∞
n=1
c
(p)
n ζ n
p , (6.31)
where
c
(p)
n = −
(1 − α)
2
f
(p)
n +
(1 + β)
2
g
(2)(p)
n − δn1a
(p)
1 (n = 1, 2, . . .). (6.32)
In these notations, u
(p)
s takes the same form as in the case of perfectly bonded
ﬁbers, i.e.
2μ0u
(p)
s (ζp) =
∞
n=1
κ0a
(p)
−n ζ −n
p + ζp − ζp
−1
a
(p)
−n ζp
−(n+1)
− c
(p)
n ζp
−n
.
(6.33)
The expression (6.33) is appropriate for I
(q)
k evaluation provided Z pq is sufﬁciently
large. Moreover, in this case integration can be done analytically, with aid of the re-
expansion formula (6.3) written for ζp as
ζ−n
p =
k
η
pq
nk ζ k
q , ζq < Z pq ; (6.34)
where
η
pq
nk = (−1)k (n + k − 1)!
(n − 1)!k!
z
(p)
c
n
z
(q)
c
k
Z−(n+k)
pq (6.35)
for k ≥ 0 and equal to zero otherwise. After some algebra, we get the explicit
expression of I
(q)
k (6.23):
I
(q)
k = 2μ0Γ1δk1 − 2μ0Γ2 z
(q)
c
−2
δk,−1 (6.36)
+
N
p=q
z
(p)
c
z
(q)
c
∞
n=1
κ0 A
pq
nk a
(p)
−n + n(B
pq
nk + C
pq
nk )a
(p)
−n + D
pq
nk c
(p)
n ,
where
A
pq
nk =
η
pq
nk , k > 0;
0, otherwise;
(6.37)
B
pq
nk =
⎧
⎨
⎩
(−1)k+1 (n−k+2)!
(n+1)!(1−k)! z
(p)
c
n+2
z
(q)
c
−k
Z
−(n−k+2)
pq , k ≤ 1;
0, otherwise;
(6.38)
69.
Multipole Expansion Method in Micromechanics of Composites 165
C
pq
nk =
⎧
⎨
⎩
(−1)k (n−k)!
(n−1)!(−k)! z
(p)
c
n+2
z
(q)
c
−k
Z pq
2
Z
−(n−k+2)
pq , k < 0;
0, otherwise;
(6.39)
D
pq
nk =
η
pq
n,−k, k < 0;
0, otherwise.
(6.40)
Theoretically, the obtained formulas are valid for any two non-touching ﬁbers
with indices p and q. However, for the closely placed ﬁbers ( Z pq ≈ 2R) the
series (6.33) and (6.34) converge rather slow: in this case, direct numerical integra-
tion is preferable. The following empirical rule provides the reasonable compromise
between computational effort and accuracy: for Z pq ≤ 2.5R, the integrals (6.23)
are evaluated numerically whereas for Z pq > 2.5R the explicit analytical formula
(6.36) is applied.
6.7 RUC Model of Fibrous Composite with Interface Cracks
Now, we consider the model problem for RUC geometry, with the macroscopic strain
E as a governing parameter. The periodicity conditions (6.7), (6.8) are fulﬁlled by
taking the displacement in matrix domain as a sum of linear mean ﬁeld u∞ and
periodic disturbance ﬁeld u∗
s . Speciﬁcally,
u0(z) = u∞
(z) + u∗
s (z), u∗
s (z) =
N
p=1
z
(p)
c u
∗(p)
s (ζp). (6.41)
In comparison with (6.20), the single ﬁber disturbance terms us
p are replaced with
their periodic counterparts given by the sums over all the square lattice nodes
k = {k1, k2} (−∞ < k1, k2 < ∞) :
u
∗(p)
s (ζp) =
k
u
(p)
s
zp + Wk
z
(p)
c
, Wk = (k1 + ik2)a. (6.42)
In view of (6.33), u
∗(p)
s can be expressed in terms of the periodic complex (harmonic)
potentials S∗
n (z) and their biharmonic S∗∗
n (z) counterparts:
S∗
n (z) =
k
(z + Wk)−n
; S∗∗
n (z) =
k
|z + Wk|2
(z + Wk)−(n+2)
(6.43)
([17, 65], among others). In particular,
70.
166 V. I. Kushch
ϕ
∗(p)
s (ζp) =
∞
n=1
a
(p)
−n z
(p)
c
n
S∗
n (zp). (6.44)
The above procedure, with two amendments, applies to this problem. First, we
require u0(z) (6.41) to obey the periodicity conditions (6.8). This condition gives us
the far ﬁeld u∞(z) (6.24) coefﬁcients Γ1 and Γ2. It has been established elsewhere
[17, 65] that
S∗
n (z) = S∗
n (z + a) = S∗
n (z + ia) − δn12πi/a; (6.45)
S∗∗
n (z) = S∗∗
n (z + a) = S∗∗
n (z + ia);
where δnm is the Kronecker delta. By substituting (6.41) into (6.8) and taking (6.45)
into consideration we ﬁnd
Γ1 =
E11 + E22
2
+ ReΓΣ ; Γ2 =
E22 − E11
2
+ i E12 + ΓΣ ; (6.46)
where
ΓΣ =
π
V
N
p=1
κ0a
(p)
−1 z
(p)
c
2
− a
(p)
−1 z
(p)
c
2
+ c
(p)
1 . (6.47)
Second, the formula (6.23) should be modiﬁed to take into account interactions of
an inﬁnite array of ﬁbers. To avoid the discussed above integration issues, we write
it as
I
(q)
k =
2μ0
2πz
(q)
c
2π
0
⎧
⎨
⎩
u∞
(z) +
N
p=q
z
(p)
c u
(p)
s ζp (6.48)
+
N
p=1
z
(p)
c
k=0
u
(p)
s
zp + Wk
z
(p)
c
⎫
⎬
⎭
t−k
q dθq.
Here, the ﬁrst sum contains contributions from the nearest neighboring ﬁbers of pth
and qth arrays deﬁned by Z∗
pq, see Fig.2. It can be integrated either analytically or
numerically, in accordance with the rule formulated in Sect.6.6. The second sum
contains contributions from the “far” ﬁbers. Provided a number of ﬁbers in the cell
is sufﬁciently large, the cell size a 2R and Zq − Z p 2R for all ﬁbers
contributing to this sum. In this case analytical integration is justiﬁed and yields
I
(q)
k =
N
p=1
z
(p)
c
z
(q)
c
∞
n=1
κ0 A
∗pq
nk a
(p)
−n + n(B
∗pq
nk + C
∗pq
nk )a
(p)
−n + D
∗pq
nk c
(p)
n (6.49)
71.
Multipole Expansion Method in Micromechanics of Composites 167
In (6.49), the coefﬁcients A
∗pq
nk , B
∗pq
nk , C
∗pq
nk and D
∗pq
nk are given by the
formulas from (6.37) to (6.40), respectively, with replacing the Z
−(n+k)
pq to Σ
pq∗
n+k
and Z pq
2
Z
−(n−k+2)
pq to Σ
pq∗∗
n−k , where
Σ
pq∗
n =
k=0
(Z∗
pq + Wk)−n
, Σ
pq∗∗
n =
k=0
Z∗
pq + Wk
2
(Z∗
pq + Wk)n+2
(6.50)
are the standard harmonic and biharmonic lattice sums, respectively ([65]). Now,
with u∞(z) and I
(q)
k expressed in terms of a
(p)
−n and c
(p)
n (formulas (6.24), (6.46),
(6.47) and (6.49), respectively), the problem is reduced to considered above [51].
6.8 Effective Stiffness Tensor
The obtained analytical solution provides an accurate evaluation of the local strain
and stress ﬁelds in any point of RUC and thus enables a comprehensive study of
stress concentration, stress intensity factors and energy release rate at the interface
crack tips in FRC. On the other hand, the strain and stress ﬁelds can be integrated
analytically to get the ﬁnite expression of the macroscopic stiffness tensor C∗ (1.10).
From the plane strain problem, the effective transverse elastic moduli C∗
1111, C∗
1122,
C∗
2222 and C∗
1212 can be determined.
To simplify the integration procedure, we write the bulk and shear components
of the strain tensor as
ε11 + ε22 = 2Re
∂u
∂z
; ε22 − ε11 + 2iε12 = −2
∂u
∂z
. (6.51)
In what follows, we will use also the Gauss formula written in complex variables as
A
∂u
∂z
dV =
1
2 L
u(n1 − in2)dL, (6.52)
where L is the boundary of A and (n1, n2)T is the outer normal to L unit vector.
First, by integrating the bulk stress
σ11 + σ22
2
=
4μ
(κ − 1)
Re
∂u
∂z
(6.53)
we get
A
σ11 + σ22
2
=
4μ0
(κ0 − 1) A
Re
∂u0
∂z
dV +
4μ1
(κ1 − 1)
N
q=1 Aq
Re
∂uq
∂z
dV (6.54)
72.
168 V. I. Kushch
where Aq = πR2 is the area of qth ﬁber cross-section and A0 = a2 − NπR2 is the
matrix area inside the cell: A = N
q=0 Aq. Next, by applying the formula (6.52) we
obtain
A
σ11 + σ22
2
=
4μ0
(κ0 − 1)
⎛
⎝
L0
−
N
q=1 Lq
⎞
⎠ Re [u0 (n1 − in2)] dL (6.55)
+
4μ1
(κ1 − 1)
N
q=1 Lq
Re uq (n1 − in2) dL,
where L0 is the outer boundary of the cell. In the case Lq involves the interface crack
L
(q)
c , u0 and uq in (6.55) are integrated along the matrix and ﬁber, respectively, side
of the crack.
In view of (6.8), integration along L0 is elementary and yields
L0
Re [u0 (n1 − in2)] dL = a2
(E11 + E22) . (6.56)
We recognize also that at the interface Lq, the integrands simplify to
4μj
(κj − 1)
Re u j (n1 − in2) = 2Re
κj ϕj (tq) − ωj (1/tq)
(κj − 1)
t−1
q . (6.57)
In view of (6.57), integration along Lq is straightforward. With (6.13) and (6.32)
taken into consideration we come, after some algebra, to
Lq
Re
4μ1uq
(κ1 − 1)
−
4μ0u0
(κ0 − 1)
(n1 − in2) dL = 2π
(κ0 + 1)
(κ0 − 1)
c
(q)
1 , (6.58)
where c
(q)
1 is given by (6.32). Now, collecting all the terms gives us the exact formula:
σ11 + σ22
2
=
2μ0 (E11 + E22)
(κ0 − 1)
+
2π
a2
(κ0 + 1)
(κ0 − 1)
N
q=1
c
(q)
1 . (6.59)
Averaging the shear part of stress tensor is quite analogous. It follows from (6.51)
that
σ22 − σ11 + 2iσ12 = 2μ(ε22 − ε11 + 2iε12) = −2μ
∂u
∂z
. (6.60)
By applying the formula (6.52) and performing the transformations similar to those
exposed above, we get also
73.
Multipole Expansion Method in Micromechanics of Composites 169
σ22 − σ11 − 2i σ12 = 2μ0 (E22 − E11 − 2iE12) (6.61)
+
2π
a2
(κ0 + 1)
N
q=1
a
(q)
−1 z
(q)
c
2
,
where a
(q)
−1 is given by (6.30). Together with (1.10), relations (6.59) and (6.61) enable
evaluation of the effective transverse elastic moduli C∗
1111, C∗
1122, C∗
2222 and C∗
1212
of unidirectional FRC with interface cracks [53]. To ﬁnd C∗
2323 and C∗
1313, one has to
consider longitudinal shear in the ﬁber axis (x3) direction. In mathematical sense, this
problem is equivalent to the transverse conductivity (2D Laplace) problem, solved
recently in [52].
7 Composite with Elliptic in Cross-Section Fibers
In this Section, we consider a plane containing a ﬁnite array of elliptic inclusions.
No restrictions is imposed on their number, size, aspect ratio, elastic properties and
arrangement. For the sake of simplicity, the inclusions are assumed equally ori-
ented; extension of the below analysis to the case of arbitrarily oriented inclusions is
straightforward. We apply MEM to solve the elasticity problem: for the multipole-
type solution of the counterpart conductivity problem, see [86, 87].
7.1 Single Elliptic Inclusion in Non-uniform Far Field
Let consider an isotropic elastic plane with a single elliptic inclusion. The Cartesian
coordinate system Ox1x2 is deﬁned so that its origin coincides with the centroid
of ellipse whereas the Ox1 and Ox2 axes are directed along the major and minor
axes of the ellipse. An aspect ratio of the ellipse is e = l2/l1, where l1 and l2 are the
major and minor, respectively, semi-axes of the ellipse. Another derivative geometric
parameter is the inter-foci distance 2d, where d = l2
1 − l2
2.
7.1.1 Background Theory
We introduce the complex variables of two kinds. The ﬁrst one is z = x1 + ix2, the
second variable ξ = ζ + iη is deﬁned by
z = ω(ξ) = d cosh ξ. (7.1)
Equation(7.1) speciﬁes an elliptic coordinate system with ζ and η as “radial” and
“angular” coordinates, respectively. So, the boundary of the ellipse is the coordinate
74.
170 V. I. Kushch
line given by the equation
ζ = ζ0 =
1
2
ln
1 + e
1 − e
; (7.2)
i.e., the points at matrix-elliptic ﬁber interface are the functions of angular coordinate
η only. This fact makes the elliptic complex variable ξ particularly useful in the
problems formulated on domains with elliptic boundaries/interfaces.
The complex displacement u = u1 + iu2 is expressed in terms of complex poten-
tials ϕ and ψ as
u = κϕ (z) − (z − z) ϕ (z) − ψ (z). (7.3)
The expression (7.3) is slightly different in form but equivalent to that originally
suggested in [67]. Cartesian components of the corresponding to u (7.3) stress tensor
σ are given by
σ11 + σ22 = 4μ ϕ (z) + ϕ (z) ; (7.4)
σ22 − σ11 + 2iσ12 = 4μ (z − z)ϕ (z) − ϕ (z) + ψ (z) .
The displacement u and traction Tn are assumed to be continuous through the
elliptic matrix-inclusion interface S : ζ = ζ0. Satisfying these conditions can be
greatly simpliﬁed by writing the complex displacement and traction in terms of their
curvilinear (actually, normal and tangential to interface ζ = ζ0) components:
u = uζ + iuη and Tn = σζζ + iσζη. (7.5)
In terms of complex potentials [67],
uζ + iuη =
(ξ)
| (ξ)|
[κϕ (z) − (z − z) ϕ (z) − ψ (z)]; (7.6)
σζζ − iσζη = 2G ϕ (z) + ϕ (z) −
(ξ)
(ξ)
[(z − z)ϕ (z) − ϕ (z) + ψ (z)] ,
where, from (7.1), (ξ) = dz/dξ = d sinh ξ.
7.1.2 Formal Solution
The key point is the proper choice of the form of potential functions ϕ and ψ. We
take ϕ, by analogy with [61], as
75.
Multipole Expansion Method in Micromechanics of Composites 171
ϕ =
n
Anυ−n
. (7.7)
The ψ potential, by analogy with the 3D case (4.50), is taken in the form [45]
ψ = ψ0 − ψ1, ψ0 =
n
Bnυ−n
, ψ1 =
sinh ζ0
sinh ξ
υ
υ0
−
υ0
υ n
nAnυ−n
, (7.8)
where An and Bn are the complex coefﬁcients, υ = exp ξ and υ0 = exp(ζ0). The
potentials ϕi and ψi for inclusion are also given by (7.7) and (7.8), with replacing
An and Bn to Cn and Dn, respectively.
With ϕ in the form (7.7) and ψ in the form (7.8), the expressions of u and Tn (7.6)
at the interface ζ = ζ0 are simpliﬁed dramatically: speciﬁcally,
u ζ=ζ0 = κϕ − ψ0 =
n
κAnυ−n
− Bnυ−n (7.9)
and
Tn
2G
ζ=ζ0 = ϕ − ψ0 =
n
(−n) Anυ−n
− Bnυ−n . (7.10)
For the details of derivation, see [45]. By virtue of (7.9), from the displacement
continuity condition one ﬁnds
n
(κ0 Ane−nζ0−inη
− Bne−nζ0+inη
) =
n
(κ1Cne−nζ0−inη
− Dne−nζ0+inη
),
(7.11)
where κi = κ(νi ). Orthogonality of Fourier harmonics exp(inη) enables splitting
the functional equality (7.11) into an inﬁnite set of linear algebraic equations
κ0 Anυ−n
0 − B−nυn
0 = κ1Cnυ−n
0 − D−nυn
0 . (7.12)
By applying the same procedure to the interface traction continuity condition, we
get another set of linear equations:
Anυ−n
0 + B−nυn
0 = ω(Cnυ−n
0 + D−nυn
0 ), (7.13)
where ω = μ1/μ0.
It is advisable, for computational purpose, to introduce new scaled variables An =
Anυ−n
0 , etc.; we obtain
76.
172 V. I. Kushch
κ0 An − B−n = κ1Cn − D−n, (7.14)
An + B−n = ω(Cn + D−n), −∞ < n < ∞.
The form of Eq.(7.14) is remarkably simple, if not simplest (see, for comparison,
[61]) which clearly indicates rational choice of the potential functions (7.8).
The obtained solution is general and contains the extra degrees of freedom which
must be excluded by imposing the constraints drawn from physical considerations.
One obvious condition consists in that the displacement ﬁeld must be regular, i.e.,
continuous and ﬁnite inside the inclusion. It means the Laurent series expansions of
corresponding complex potentials contain the terms with non-negative powers of z
only. It has been shown elsewhere [45] that the following relations between Cn and
Dn with positive and negative index n,
Cn = C−n; Dn = D−n + 2n sinh(2ζ0)C−n, n > 0; (7.15)
provide regularity of the displacement and stress ﬁelds inside the inclusion.
The displacement solution in the matrix domain comprises the regular and irreg-
ular parts: u(0) = ur + us. Here, ur is the regular far ﬁeld whereas the disturbance
us → 0 as |z| → ∞. The potentials ϕ and ψ also can be splitted onto irregular and
regular parts:
ϕ = ϕs
+ ϕr
, ψ = ψs
+ ψr
. (7.16)
The expression of ϕs and ψs is given by Eqs.(7.7) and (7.8), respectively, where we
keep the terms with negative powers of υ only to provide the required asymptotic
behavior, so
An = Bn ≡ 0 for n ≤ 0. (7.17)
On the contrary, ur is assumed to be regular, with the potentials
ϕr
=
n
anυ−n
, ψr
=
n
bn − 2nan
sinh ζ0
sinh ξ
sinh(ξ − ζ0) υ−n
, (7.18)
where an and bn comply (7.15) as well.
7.1.3 Resolving Linear System
Representation of the linear displacement ﬁeld corresponding to the constant far
strain tensor E
ur
= (E11x1 + E12x2) + i(E12x1 + E22x2) (7.19)
77.
Multipole Expansion Method in Micromechanics of Composites 173
takes the form (7.3) with the potentials (7.18), where
a−1 =
d
4
E11 + E22
(κ0 − 1)
; b−1 = a−1υ−2
0 +
d
4
(E22 − E11 + 2i E12); (7.20)
a1 and b1 are given by (7.15) and all other an and bn for n = ±1 are equal to zero. The
displacement ur and corresponding traction Tr
n at the interface ζ = ζ0 take the form
(7.9) and (7.10), respectively. Applying the procedure analogous to that described
above gives us an inﬁnite linear system
κ0 Anυ−n
0 − B−nυn
0 + κ0anυ−n
0 − b−nυn
0 = κ1Cnυ−n
0 − D−nυn
0 ; (7.21)
Anυ−n
0 + B−nυn
0 + anυ−n
0 + b−nυn
0 = ω(Cnυ−n
0 + D−nυn
0 ).
In the single-inclusion problem, we assume ur (or, the same, an and bn) to be
known. In this case, the equations (7.21) together with (7.15) and (7.17) form a
closed set of linear algebraic equations possessing a unique solution. By substituting
(7.15) and (7.17) into (7.21) we come to the linear system
κ0 An − κ1Cn + (Dn − 2n sinh 2ζ0Cn)υ2n
0 = −κ0an + b−nυ2n
0 ; (7.22)
Bn + κ1Cnυ2n
0 − Dn = κ0a−nυ2n
0 − bn;
An − ωCn − ω(Dn − 2n sinh 2ζ0Cn)υ2n
0 = −an − b−nυ2n
0 ;
Bn − ωCnυ2n
0 − ωDn = −a−nυ2n
0 − bn;
n = 1, 2, . . . .
with the unknowns An, Bn, Cn and Dn (n > 0) and with the coefﬁcients an and bn
entering the right-hand side vector. For the Eshelby-type problem, these coefﬁcients
are given by (7.20). The corresponding resolving system (7.22) consists of four
equations for n = 1.
7.1.4 Stress Intensity Factors
The solution we derived is valid for any 0 < e < 1. To complete this section, we
consider the limiting case e → 0 where an ellipse degenerates into the cut |x1| ≤ d
in the complex plane (another limit, e → 1 where an ellipse becomes a circle, is
trivial). By putting ω = 0 we get a straight crack, the stress ﬁeld around which is
known to have singularity at the crack tips. In the linear fracture mechanics, the stress
intensity factor (SIF) deﬁned as
KI + i KII = lim
z→d
2π (z − d) (σ22 + iσ12) (7.23)
78.
174 V. I. Kushch
is used to quantify the stress ﬁeld around the crack tip. Taking this limit in the above
solution is straighforward: for e → 0 we have, from (7.2), ζ0 → 0 and υ0 → 1.
After simple algebra, we get the formula
KI + i KII = −2G0 π/d
∞
n=1
n An + Bn , (7.24)
valid for the arbitrary, not necessarily uniform, far load.
7.2 Finite Array of Inclusions
Now, we consider a plane containing N non-overlapping equally oriented elliptic
inclusions with the semi-axes l1p,l2p and elastic moduli μp and νp centered in the
points Z p = X1p + i X2p. The variables of local, inclusion-associated coordinate
systems are related by
zp = Z pq + zq, where zp = x1p + ix2p and Z pq = Zq − Z p. (7.25)
We deﬁne the local curvilinear coordinates ξp = ζp +iηp by analogy with (7.1), i.e.,
zp = dp cosh ξp. In these variables, the geometry of the pth inclusion is speciﬁed by
a pair of parameters (ξ0p, dp), where dp = l1p
2
− l2p
2
. The matrix-inclusion
interfaces ξp = ξ0p are perfectly bonded. The stress in and around the inclusions is
induced by the far ﬁeld ur taken in the form (7.19).
7.2.1 Direct (Superposition) Sum
We use the superposition principle to write the solution for a multiply-connected
matrix domain:
u(0)
= ur
(z) +
N
p=1
us
p(z − Z p), (7.26)
where us
p is the disturbance from pth inclusion, decaying at |z| → ∞. The corre-
sponding complex potentials ϕs
p and ψs
p ahave the form (7.7) and (7.8), where, by
analogy with (7.17), Anp = Bnp = 0 for n ≤ 0.
The sum in (7.26) contains the terms written in variables of different coordinate
systems. In order to fulﬁl the interface bonding conditions, we need to ﬁnd local
expansion of (7.26). Our aim is to transform
us
p = κ0ϕs
p zp − zp − zp ϕs
p zp − ψs
p zp , (7.27)
79.
Multipole Expansion Method in Micromechanics of Composites 175
where
ϕs
p =
∞
n=0
Anpυ−n
p , (7.28)
ψs
p = ψs
0p − ψs
1p =
∞
n=0
Bnp − 2nAnp
sinh ζ0p
sinh ξp
sinh(ξp − ζ0p) υ−n
p ,
into ur
pq, written in the same form as us
p, but in the qth coordinate basis, namely
ur
pq = κ0ϕr
pq zq − zq − zq ϕr
pq zq − ψr
pq zq , (7.29)
with
ϕr
pq =
n
anpqυ−n
q , (7.30)
ψr
pq = ψr
0pq − ψr
1pq =
n
bnpq − 2nanpq
sinh ζ0q
sinh ξq
sinh(ξq − ζ0q) υ−n
q .
7.2.2 Re-expansion Formulas
For this purpose, we use the re-expansion formulas for irregular complex poten-
tials [45]
υ−n
p =
m
η
pq
nmυ−m
q , n = 1, 2, . . . ; (7.31)
Here, υp = exp ξp = zp/dp ± zp/dp
2
− 1, zp = zq + Z pq; the expansion
coefﬁcients η
pq
nm = ηnm Z pq, dp, dq
η
(1)pq
nm = (−1)m
n
dp
dpq
n ∞
j=0
υ
−(n+m+2 j)
pq
j
l=0
(−1)j−l
( j − l)!
dp
dpq
m+2l
(7.32)
× Mnml dp, dq
(n + m + l + j − 1)!
( j − l)!
.
where dpq = dp + dq and υpq = Z pq/dpq + Z pq/dpq
2
− 1,
Mnml dp, dq =
l
k=0
dp/dq
2k
k! (l − k)! (k + n)! (m + l − k)!
. (7.33)
80.
176 V. I. Kushch
In the case zp > dp and zq < Z pq and Z pq > (dp + dq), the expansion
coefﬁcients simplify to
η
(2)pq
nm = ndn
p (−1)m
∞
l=0
d2l+m
q Mnml dp, dq
(n + m + 2l − 1)!
2Z pq
n+m+2l
. (7.34)
The series (7.31) converges within an ellipse centered in Zq with inter-foci
distance dpq and passing the pole of pth elliptic coordinate system closest to Zq.
This convergence area is sufﬁcient to solve for any two non-overlapping ellipses. For
well-separated inclusions, both (7.34) and (7.32) give the same numerical value of
ηnm. Therefore, when we solve numerically for many inclusions, the computational
effort-saving strategy is to apply (7.32) to closest neighbors whereas interaction of
the rest, more distant inclusions is evaluated using more simple formula (7.34). In
the analogous to (7.31) addition theorem derived in [86], the expansion coefﬁcients
are expressed in terms of hypergeometric function.
Also, we mention two useful consequences of the formula (7.31). The ﬁrst of them
can be obtained by differentiating both parts of (7.31) with respect to zq. It gives us
υ−n
p
sinh ξp
=
dp
dq m
m
n
η
pq
nm
υ−m
q
sinh ξq
, (7.35)
being,infact,anadditiontheoremforthealternatesetofbasicfunctions[45].Another
differentiation of (7.31), this time with respect to Z pq, results in
υ−n
p
sinh ξp
=
n
μ
pq
nmυ−m
q , (7.36)
where μ
pq
nm =
dp
n
d
dZ pq
η
pq
nm. For μnm we also have two (general and simpliﬁed) expres-
sions obtained by differentiating (7.32) and (7.34), respectively.
7.2.3 Local Expansion
By applying (7.31) to ϕs
p, one obtains
ϕs
p =
∞
n=0
Anpυ−n
p =
n
anpqυ−n
q = ϕr
pq, (7.37)
where
anpq =
∞
m=1
Ampη
pq
mn (7.38)
81.
Multipole Expansion Method in Micromechanics of Composites 177
and η
pq
mn are the expansion coefﬁcients given by (7.32). With anpq in the form (7.38),
the ﬁrst terms in (7.27) and (7.29) coincide, κ0ϕs
p = κ0ϕr
pq.
Determination of bnpq is more involved. From (7.37) we ﬁnd also ϕs
p (zp) =
ϕr
pq(zq) and thus the second term in (7.27) can be written as
zp − zp ϕs
p = Z pq − Z pq ϕr
pq + zq − zq ϕr
pq. (7.39)
To provide us
p = ur
pq, we determine bnpq in (7.30) from
ψs
p = ψr
pq + Z pq − Z pq ϕr
pq. (7.40)
To this end, all the terms in (7.40) should be expanded into a series of υq. For the
details of derivation procedure, see [45]. Here, we give the ﬁnal expression of bnpq
for n < 0:
bnpq =
∞
m=1
Bmpη
pq
mn +
∞
m=1
Amp
m
2
υ0p − υ−1
0p
2
μ
pq
m+1,n (7.41)
+ n υ−2
0q − 1 − n 1 − υ−2
0p η
pq
mn + υ0q − υ−1
0q
2
×
∞
k=1
(2k − n)η
pq
m,2k−n +
2
dq
Z pq − Z pq
∞
k=0
(2k + 1 − n)η
pq
m,2k+1−n ;
for n > 0, in accordance with (7.15),
bnpq = b−n,pq + n υ2
0q − υ−2
0q anpq. (7.42)
Now, we come back to (7.26) and write
N
p=1
us
p(zp) = us
q(zq) + ur
q(zq), (7.43)
where ur
q(zq) = p=q ur
pq(zq) has the form (7.29), (7.30) with replace ϕr
pq to
ϕr
q = p=q ϕr
pq, ψr
pq to ψr
q = p=q ψr
pq; also,
anq =
p=q
anpq, bnq =
p=q
bnpq (7.44)
No problems arise with local expansion of the linear term in (7.26):
ur
(z) = Uq + ur
(zq), (7.45)
82.
178 V. I. Kushch
where Uq = (X1q E11 + X2q E12) + i(X1q E12 + X2q E22) is the constant and the
formulas (7.19) and (7.19) apply to expand ur (zq).
7.2.4 Resolving System
The resolving set of equations is:
κ0 Anq − κqCnq + (Dnq − 2n sinh 2ζ0qCnq)υ2n
0q = −κ0anq + b−n,qυ2n
0q ; (7.46)
Bnq + κqCnqυ2n
0q − Dnq = κ0a−n,qυ2n
0q − bnq;
Anq − ωqCnq − ωq(Dnq − 2n sinh 2ζ0qCnq)υ2n
0q = −anq − b−n,qυ2n
0q ;
Bnq − ωqCnqυ2n
0q − ωq Dnq = −a−n,qυ2n
0q − bnq;
n = 1, 2, . . . ; q = 1, 2, . . . , N;
where ωq = μq/μ0; Cnq and Dnq are the expansion coefﬁcients of solution in the
qth inclusion. To get it in an explicit form for direct solver one needs to substitute
(7.30) and (7.41) into (7.44) and then into (7.46). Alternatively, the simple iterative
solving procedure can be applied here: given some initial guess of Anq, Bnq, Cnq and
Dnq for 1 ≤ q ≤ N, we compute anq and bnq from (7.38), (7.41) and (7.44), then
substitute into the right-hand side of (7.46) and solve it for the next approximation
of unknown coefﬁcients, etc. This procedure converges for a whole range of input
parameters excluding the case of nearly touching inclusions where an appropriate
initial approximation must be taken to provide convergence of numerical algorithm.
An extension of the above analysis to the inﬁnite arrays of elliptic inclusions
is obvious. The appropriate periodic potentials for the conductivity problem have
been obtained in [86, 87]. The RUC model of elastic solid with various statistical
(both uniform and clustered) distributions of cracks is considered in [49, 50]. The
developed there theory, with minor modiﬁcations, applies to the RUC model of
composite reinforced by the equally oriented, elliptic in cross-section ﬁbers.
8 Fibrous Composite with Anisotropic Constituents
In[48],themultipoleexpansionbasedapproachhasbeendevelopedtostudythestress
ﬁeldandeffectiveelasticpropertiesofunidirectionalFRCcompositewithanisotropic
phases. The most general case of elastic anisotropy which can be considered in 2D
statement is the monoclinic symmetry with the Ox1x2 being the symmetry plane.
In two-index notation, the generalized Hooke’s law for this symmetry type has the
form
83.
Multipole Expansion Method in Micromechanics of Composites 179
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
σ11
σ22
σ33
σ23
σ13
σ12
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
=
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
C11 C12 C13 0 0 C16
C12 C22 C23 0 0 C26
C13 C23 C33 0 0 C36
0 0 0 C44 C45 0
0 0 0 C45 C55 0
C16 C26 C36 0 0 C66
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
⎛
⎜
⎜
⎜
⎜
⎜
⎜
⎝
ε11
ε22
ε33
2ε23
2ε13
2ε12
⎞
⎟
⎟
⎟
⎟
⎟
⎟
⎠
. (8.1)
In the case of the ﬁbers aligned in x3-direction, a composite possesses the same
anisotropy type of macroscopic elastic moduli.
8.1 Anti-Plane Shear Problem
8.1.1 Background Theory
In the case of shear deformation along the ﬁber axis, u3 is the only non-zero
component of the displacement vector:
u1 = u2 = 0; u3 = w(x1, x2). (8.2)
Also, we have two non-zero components of stress tensor, σ13 and σ23; the equilibrium
Equation ∇ · σ = 0 takes the form
∂σ13
∂x1
+
∂σ23
∂x2
= 0. (8.3)
This problem is mathematically equivalent to the transverse conductivity problem in
FRC.
The stress function W(x1, x2) is introduced [55] as follows:
σ13 = C
∂W
∂x2
, σ23 = −C
∂W
∂x1
. (8.4)
The stress ﬁeld (8.4) satisﬁes the equilibrium equation (8.3) identically. Also, we
need to provide the strain compatibility condition
∂ε13
∂x2
=
∂ε23
∂x1
=
1
2
∂2w
∂x1∂x2
. (8.5)
Inversion of (8.1) gives
2ε13 = S55σ13 + S45σ23; (8.6)
2ε23 = S45σ13 + S44σ23;
84.
180 V. I. Kushch
where S55 = C44/C2, S45 = −C45/C2, S44 = C55/C2 and C = C44C55 − C2
45 > 0.
Substitution of (8.4) and (8.6) into (8.5) yields
S44
∂2W
∂x2
1
− 2S45
∂2W
∂x1∂x2
+ S55
∂2w
∂x2
2
= 0. (8.7)
By introducing new complex variable ξ = x1 + μx2 [55], where
μ = (−C45 + iC) /C44 (8.8)
is the root of the characteristic equation
C44μ2
+ 2C45μ + C55 = 0, (8.9)
theEq.(8.7)reducesto2DLaplaceequation ∂2W
∂ξ∂ξ
= 0.Hence,thetheoryofanalytical
functions [67] applies to this problem. Speciﬁcally, W can be taken as W(x1, x2) =
ReΦ, where Φ is an analytical function of complex variable ξ. In this case also
w = −ImΦ and, thus, the boundary value problem for w can be formulated as the
potential theory problem, in terms of Φ. The traction at interface is written as
tn = σ13n1 + σ23n2 = C
∂W
∂x2
cos ϕ −
∂W
∂x1
sin ϕ =
C
2ρ
∂
∂ϕ
ReΦ, (8.10)
where n1 and n2 are the outward normal direction cosines and (ρ, ϕ) are the circular
coordinates deﬁned by x1 + ix2 = ρ exp (iϕ).
Introducing the new variable ξ = x1 + μx2 is equivalent to afﬁne trans-
formation of the complex plane. It reduces the elasticity theory problem to
that Laplace equation in the transformed coordinates. However, any afﬁne
transformation deforms the circular matrix-ﬁber interface, where the bonding
conditions must be fulﬁlled, into elliptic one.
The exposed in the precious Section theory, with some modiﬁcations, is appropri-
ate for this purpose. The series expansion solution of the potential theory problem is
Φ =
n
Dnυ−n
, υ = ξ/d ± (ξ/d)2
− 1. (8.11)
In the υ expression, sign before the square root is chosen to keep Imυ ≥ 0, d
is the matching parameter and Dn are the complex constants. The regularity of
Φ (ξ) implies D−n = Dn [45]. In this case, Φ is expressed in terms of Chebyshev
polynomial of complex variable ξ/d:
85.
Multipole Expansion Method in Micromechanics of Composites 181
υn
+ υ−n
= 2 cosh [nArccosh (ξ/d)] ; (8.12)
for n = 1, 2ξ/d = υ + 1/υ. In contrast, the multipole expansion of the disturbance
ﬁeld contains the negative powers of υ only: Φ = n Anυ−n, where An = 0 for
n ≤ 0.
An appropriate choice of parameter d provides a remarkably simple form of (8.11)
at the circular interface ρ = R. In particular, for d = R 1 + μ2
υ ρ=R =
1 − iμ
1 + iμ
1/2
R exp(iϕ) = Rμ exp(iϕ) (8.13)
so expression (8.11) at the interface appears to be the Fourier series of ϕ. Noteworthy,
d can be viewed as the anisotropy parameter: for an isotropic solid, d ≡ 0. In the
limiting case d → 0, d
2 υ → z = x1 + ix2 and d
2 Rμ → R. Hence, at least for a
weakly anisotropic material, the normalized expansion coefﬁcients An = d
2
−n
An
and Dn = d
2
n
Dn must be used in order to prevent possible numerical error accu-
mulation.
8.1.2 Single Inclusion Problem
Let consider a single inclusion of radius R embedded in an inﬁnite matrix. Both
the matrix and inclusion materials are anisotropic, with the elastic stiffness tensors
C− = C−
i j and C+ = C+
i j , respectively. Hereafter, we will mark all the matrix-
related parameters by the sign “−” and the inclusion-related ones by the sign “+”.
The uniform far ﬁeld loading is prescribed by the constant strain tensor E = Ei j ;
in the anti-plane shear problem, only E13 and E23 are non-zero. The perfect bonding
between the matrix and inclusion [[w]] = [[tn]] = 0 is assumed.
The regular displacement ﬁeld w+ in the inclusion is expanded into series (8.11):
w+
= −ImΦ+
, Φ+
=
n
Dn υ+ −n
, (8.14)
where D−n = Dn and υ± is deﬁned by (8.11), with d± = R 1 + μ± 2
.
The displacement ﬁeld w− in the matrix is written as the superposition sum of far
linear ﬁeld w−
0 and the disturbance ﬁeld w−
1 caused by the inclusion. We seek w−
in the form
w−
= −ImΦ−
, Φ−
= Γ ξ−
+
∞
n=1
An υ− −n
=
n
(An + an) υ− −n
, (8.15)
86.
182 V. I. Kushch
where Γ = Γ1 + iΓ2 and an = 1
2 δn1Γ d−, δnm being the Kronecker’s delta. The
corresponding to E linear displacement ﬁeld is w−
0 = E13x1 + E23x2. On the other
hand,
w−
0 = −Im (Γ1 + iΓ2) x1 + μ−
x2 = −Γ2x1 − Γ1
C−
C−
44
− Γ2
C−
45
C−
44
x2.
(8.16)
This yields
Γ = −
C−
44 + iC−
C−
E13 +
C−
44
C−
E23 . (8.17)
The interface bonding conditions in terms of complex potentials Φ− and Φ+ take
the form
Φ+
− Φ+
ρ=R = Φ−
− Φ−
ρ=R , (8.18)
C+
C−
∂
∂ϕ
Φ+
+ Φ+
ρ=R =
∂
∂ϕ
Φ−
+ Φ−
ρ=R .
By choosing the center of inclusion as a reference point, we get D0 = 0. All other
coefﬁcients are found from (8.18). Substitution of (8.14) and (8.15) into the ﬁrst
condition in (8.18) yields
n
Dn Rμ+
−n
e−inϕ
− Dn Rμ+
−n
einϕ
(8.19)
=
n
An Rμ−
−n
e−inϕ
− An Rμ−
−n
einϕ
+ an Rμ−
−n
e−inϕ
− an Rμ−
−n
einϕ
.
By equating the Fourier coefﬁcients in the left and right hand parts of (8.19), we
obtain a set of linear equations
(An + an) Rμ−
−n
− an Rμ−
n
= Dn Rμ+
−n
− Dn Rμ+
n
, (8.20)
n = 1, 2, . . . .
The second condition in (8.18) gives rise to another set of equations:
(An + an) Rμ−
−n
+ an Rμ−
n
=
C+
C−
Dn Rμ+
−n
+ Dn Rμ+
n
, (8.21)
n = 1, 2, . . . .
The Eqs.(8.17), (8.20) and (8.21) form a closed inﬁnite system of linear equations
with the unknowns An and Dn which can be solved with any desirable accuracy by
87.
Multipole Expansion Method in Micromechanics of Composites 183
the truncation method [27]. In this speciﬁc problem, An = Dn = 0 for n > 1; an
explicit analytical solution of the problem is readily found from two equations in
(8.20) and (8.21) for n = 1. As seen from (8.20) and (8.21), the polynomial far
displacement ﬁeld induces in the inclusion the polynomial displacement ﬁeld of the
same order, in accordance with [28].
8.1.3 Finite Array of Inclusions
Now, we consider an inﬁnite matrix domain containing a ﬁnite number N of circular
inclusions centered in the points Zq = X1q + i X2q. For simplicity, we put Z1 = 0
and take all the inclusions identical: Rq = R and C+
q = C+. The inclusions do not
overlap: Z pq > 2R1, where Z pq = Z p − Zq = X1pq + i X2pq. The conditions
in the remote points and at the interfaces ρq = R are the same as in the previous
problem and ρq is deﬁned by x1q + ix2q = ρq exp iϕq . Here, Oqx1qx2q is the
local coordinate system associated with qth inclusion. All other inclusion-related
parameters are marked by subscript “q”: so, ξ±
q = x1q +μ±x2q and υ±
q = ξ±
q /d± ±
ξ±
q /d± 2
− 1.
By analogy with (8.14), the displacement ﬁeld in qth inclusion is written as
w+
q = −ImΦ+
q , Φ+
q =
n
Dnq υ+
q
−n
. (8.22)
The solution in the matrix domain is given by the superposition sum of far linear
ﬁeld w−
0 and the disturbance ﬁelds w−
q from each individual inclusion:
w−
= −ImΦ−
, Φ−
= Γ ξ−
1 +
N
p=1
Φ−
p and Φ−
p =
∞
n=1
Anp υ−
p
−n
. (8.23)
The expansion coefﬁcients Dnq (8.22) and Anp (8.23) are determined from the inter-
face boundary conditions. For this purpose, we need the local expansion of w− in a
vicinity of qth inclusion.
An expansion of w−
0 is simple: ξ− = ξ−
1 = ξ−
q + Ξ1q, where Ξpq = X1pq +
μ− X2pq. Hence, w−
0 = −ImΓ ξ− = −ImΓ ξ−
q + W0, where W0 = −Im Γ Ξ1q
is the rigid body motion of qth inclusion. The singular in the point Zq term Φ−
q is
initially written in variables of qth local coordinate system. The terms Φ−
p in (8.23)
are regular in a vicinity and in the point Zq for p = q. Their local expansion in the
form analogous to (8.22) is obtained by applying the re-expansion formula (7.31)
[45], with the coefﬁcients η
pq
nm = ηnm Ξpq, dp, dp given by (7.32), (7.34). In fact,
we only replace in (7.31) zp with ξp = xp + μyp and Z pq with Ξpq. In the problem
we consider, dp = dq = 1 + μ2 which simpliﬁes ηnm considerably.
88.
184 V. I. Kushch
Applying (7.31) to the last sum in (8.23) yields
Φ−
= Γ Ξpq + Γ
d−
2
υ−
q + 1/υ−
q + Φ−
q +
N
p=1
p=q
∞
n=1
Anp υ−
p
−n
(8.24)
= Γ Ξpq +
n
Anq + anq υ−
q
−n
,
where
anq =
N
p=1
∞
m=1
Ampη
pq
nm + Γ
d−
2
δn,±1. (8.25)
In (8.25), η
pq
nm ≡ 0 for p = q, anq = a−n,q and Anq = 0 for n ≤ 0.
The interface conditions in terms of complex potentials take the form (8.18),
with replace Φ+ to Φ+
q and (ρ, ϕ) to ρq, ϕq . Their fulﬁlling gives the analogous
to (8.20), (8.21) inﬁnite system of linear algebraic equations of remarkably simple
form:
Anq + anq Rμ−
−n
− anq Rμ−
n
= Dnq Rμ+
−n
− Dnq Rμ+
n
, (8.26)
Anq + anq Rμ−
−n
+ anq Rμ−
n
=
C+
C−
Dnq Rμ+
−n
+ Dnq Rμ+
n
,
n = 1, 2, . . . ; q = 1, 2, . . . , N.
8.1.4 Periodic Complex Potentials
The periodic complex potentials υ∗
n are given by the 2D lattice sums:
υ∗
n(ξ) =
α,β
υ(ξ − Lαβ)
−n
, n = 1, 2, . . . ; (8.27)
where Lαβ = αa + μβa and α and β are the integer numbers: −∞ < α, β < ∞.
These functions possess a countable set of cuts centered in the points Zαβ = αa+iβb
and yield the periodicity conditions [48]
υ∗
n(x + a, y) − υ∗
n(x, y) = 0; υ∗
n(x, y + b) − υ∗
n(x, y) = δn1
dπi
bμ
. (8.28)
The local expansion of υ∗
n(ξp) in terms of υp = υ(ξp) ξp = xp + μyp is
obtained with aid of the formula (7.31):
υ∗
n(ξp) = υp
−n
+
m
η
∗pp
nm υp
−m
, (8.29)
89.
Multipole Expansion Method in Micromechanics of Composites 185
where
η
∗pp
nm =
α,β
ηnm Lαβ, d, d . (8.30)
The upper strike means absence in this sum of the term with α = β = 0. An
expansion of υ∗
n(ξp) in terms of υq for p = q also uses the re-expansion (7.31) and
yields
υ∗
n(ξp) =
m
η
∗pq
nm υq
−m
, (8.31)
where
η
∗pq
nm =
α,β
ηnm Ξpq + Lαβ, d, d . (8.32)
The following efﬁcient way of the lattice sums (8.27) evaluation takes an advan-
tage of two ηnm expressions, η
(1)pq
nm (7.32) and η
(2)pq
nm (7.34). We write (8.32) as
η
∗pq
nm =
|Ξpq +Lαβ|≤L∗
ηnm Ξpq + Lαβ, d, d
+
|Ξpq +Lαβ|>L∗
ηnm Ξpq + Lαβ, d, d , (8.33)
where L∗ is taken sufﬁciently large to provide applicability of the formula (7.34) to
all the terms of the second sum in (8.33). Next, we re-arrange (8.33) as
η
∗pq
nm =
|Ξpq +Lαβ|≤L∗
η
(1)pq
nm +
|Ξpq +Lαβ|>L∗
η
(2)pq
nm (8.34)
=
|Ξpq +Lαβ|≤L∗
η
(1)pq
nm − η
(2)pq
nm +
α,β
η
(2)pq
nm .
The ﬁrst sum in the right hand side of (8.34) is ﬁnite and no problem arise with its
evaluation. In the second sum, we change the summation order to get
α,β
η
(2)pq
nm = n (−1)m
∞
l=0
S
pq∗
n+m+2l
d
2
n+m+2l
Mnml (n + m + 2l − 1)!, (8.35)
90.
186 V. I. Kushch
where
S
pq∗
n =
α,β
Ξpq + Lαβ
−n
=
α,β
X pq + αa + μ Ypq + βa
−n
, n ≥ 2.
(8.36)
The standard lattice sums S
pq∗
n (see also (6.50)) are computed using the Evald’s
method or another fast summation technique ([17, 18, 65]; among others).
8.1.5 RUC Model
In the framework of RUC model, we consider macroscopically uniform stress ﬁeld in
FRC with anisotropic constituents. Periodicity of geometry induces the periodicity
of the local stress ﬁled
σi j (x1 + a, x2) = σi j (x1, x2 + a) = σi j (x1, x2) (8.37)
and quasi-periodicity of the displacement ﬁeld w:
w (x1 + a, x2) − w (x1, x2) = E23a and w (x1, x2 + a) − w (x1, x2) = E13a.
(8.38)
To solve this model boundary value problem, it sufﬁces to replace the singular
potentials Φ−
p in (8.23) with their periodic counterparts
w−
= −ImΦ−
, Φ−
= Γ ∗
ξ−
1 +
N
p=1
Φ∗
p and Φ∗
p =
∞
n=1
Anpυ∗
n(ξp), (8.39)
where υ∗
n(ξp) are the periodic analytical functions (8.27). First, we substitute (8.39)
into (8.38) to obtain, with the periodicity of υ∗
n (8.28) taken into account,
Γ ∗
=
d−πi
abμ−
N
p=1
A1p + Γ, (8.40)
where Γ is given by (8.17). The subsequent ﬂow of solution resembles the above
procedure, with minor modiﬁcations. To get the local expansion, the formulas (8.29)
and (8.31) are used. An inﬁnite algebraic system has the form (8.26), where in the
anq expression (8.25) the coefﬁcients η
pq
nm must be replaced with the corresponding
lattice sums η
∗pq
nm given by the formula (8.30) for p = q and by the formula (8.32)
otherwise.
91.
Multipole Expansion Method in Micromechanics of Composites 187
8.2 Plane Strain Problem
In the plane strain problem, u1 = u(x1, x2), u2 = v(x1, x2) and u3 = 0. Non-zero
components of the strain tensor
ε11 =
∂u
∂x1
, ε22 =
∂v
∂x2
, ε12 =
1
2
∂u
∂x2
+
∂v
∂x1
(8.41)
relate the stress tensor components by
⎛
⎝
σ11
σ22
σ12
⎞
⎠ =
⎛
⎝
C11 C12 C16
C12 C22 C26
C16 C26 C66
⎞
⎠
⎛
⎝
ε11
ε22
2ε12
⎞
⎠ . (8.42)
The stress equilibrium equations take the form
∂σ11
∂x1
+
∂σ12
∂x2
= 0,
∂σ12
∂x1
+
∂σ22
∂x2
= 0. (8.43)
8.2.1 General Solution
A general solution of the plane strain problem (8.43) is written in terms of stress
functions [55] as
u1 = 2Repj Φj ; u2 = 2Reqj Φj ; (8.44)
σ11 = 2Reμ2
j Φj ; σ22 = 2ReΦj ; σ12 = 2Reμj Φj .
In (8.44), Φj = Φj ξj ( j = 1, 2) are the analytical functions of the complex
variable ξj = x1 + μj x2 and Φj = ∂Φj /∂ξj . Hereafter, the summation convention
is assumed. The complex numbers μj Imμj > 0 are the roots of the characteristic
equation
C11μ4
− 2C16μ3
+ (2C12 + C66) μ2
− 2C26μ + C22 = 0 (8.45)
and
pj = C11μ2
j − C16μj + C12, qj = C12μj − C26 + C22/μj , j = 1, 2. (8.46)
Thus, the problem consists in ﬁnding two analytical functions, Φj . We assume
the perfect bonding between the matrix and inclusions: i.e., the displacement u and
normal traction tn = σ · n vectors are continuous through the interface:
[[u]] = [[tn]] = 0. (8.47)
92.
188 V. I. Kushch
In contrast to anti-plane problem, u and tn contain two non-zero components.
The ﬁrst condition in (8.47) equates the Cartesian components of u, from where
we get
Repj Φj = 0; Reqj Φj = 0. (8.48)
The normal stress continuity condition (8.47) is equivalent to [55]
ReΦj = 0; Reμj Φj = 0. (8.49)
Thus, a general solution of the plane strain problem for anisotropic solid is expressed
in terms of harmonic potentials and hence the technique developed for the anti-plane
shear problem works equally to the plane strain problem.
8.2.2 Single Inclusion Problem
Let consider a single circular inclusion embedded into an inﬁnite matrix. The uniform
far ﬁeld is prescribed by the constant strain tensor E, with the non-zero components
E11, E22 and E12 = E21. By analogy with (8.15), the matrix displacement vector
u− is the superposition sum of far ﬁeld u−
0 = E · r and disturbance ﬁeld u−
f . The
potentials in the matrix Φ−
j and inclusion Φ+
j are taken in the form
Φ−
j = Γj ξ−
j +
∞
n=1
Anj υ−
j
−n
, Φ+
j =
n
Dnj υ+
j
−n
, j = 1, 2; (8.50)
where Γj , Anj and Dnj are the complex constants. The Γj are entirely determined
by the far ﬁeld:
E11x1 + E12x2 = 2Rep−
j Γj ξ−
j ; E12x1 + E22x2 = 2Req−
j Γj ξ−
j . (8.51)
Taking account of ξ−
j = x1 + μ−
j x2 gives the resolving set of equations for Γj :
2Rep−
j Γj = E11; 2Req−
j Γj = 2Reμ−
j p−
j Γj = E12; 2Reμ−
j q−
j Γj = E22.
(8.52)
Next, we substitute (8.50) and (8.51) into (8.48), (8.49) and use (8.13) to get the
linear system analogous to (8.20), (8.21). The interface bonding conditions (8.48),
(8.49) are written in the uniﬁed form (no summation over k):
ReκjkΦj = 0 (k = 1, 2, 3, 4); (8.53)
93.
Multipole Expansion Method in Micromechanics of Composites 189
where κj1 = pj , κj2 = qj , κj3 = 1 and κj4 = μj . We transform each of these
equations to get consequently:
κ+
jkΦ+
j + κ+
jkΦ+
j = κ−
jkΦ−
j + κ−
jkΦ−
j ;
2
j=1 n
κ+
jk Dnj Rμ+
j
−n
e−inϕ
+ κ+
jk Dnj Rμ+
j
−n
einϕ
(8.54)
=
2
j=1 n
κ−
jk Anj + anj Rμ−
j
−n
e−inϕ
+ κ−
jk Anj + anj Rμ−
j
−n
einϕ
;
where anj = 1
2 δn1Γj d−
j and, ﬁnally,
2
j=1
κ−
jk Anj + anj Rμ−
j
−n
+ κ−
jkanj Rμ−
j
n
(8.55)
=
2
j=1
κ+
jk Dnj Rμ+
j
n
+ κ+
jk Dnj Rμ+
j
−n
; n = 1, 2, . . . , k = 1, 2, 3, 4.
Together with (8.52), these equations form a complete system of equations for Anj
and Dnj . In the Eshelby’s problem, Anj = Dnj = 0 for n > 1 and the solution if
given by four Eq.(8.52).
8.2.3 Array of Inclusions
An analysis of the multiple-inclusion plane strain problem is a mere compilation
of the results exposed above, so here we give only a brief summary of the relevant
formulas. The interface conditions are written in terms of harmonic potentials as
Re κ+
jkΦ+
qj − κ−
jkΦ−
j ρq =R = 0; k = 1, 2, 3, 4; q = 1, 2, . . . , N. (8.56)
Here,
Φ+
qj =
n
Dnqj υ+
qj
−n
, j = 1, 2; (8.57)
where ξ±
qj = x1q + μ±
j x2q and υ±
qj = ξ±
qj /d±
j ± ξ±
qj /d±
j
2
− 1. The local vari-
ables relate each other by ξ−
pj = ξ−
qj + Ξpqj , where Ξpqj = X1pq + μ−
j X2pq.
94.
190 V. I. Kushch
By analogy with (8.23),
Φ−
j = Γj ξ−
1 j +
N
p=1
Φ−
pj , where Φ−
pj =
∞
n=1
Anpj υ−
pj
−n
. (8.58)
The local expansion for Φ−
j is analogous to that described above (see (8.24)). After
some algebra, we get
Φ−
j = Γj Ξpqj +
∞
n=0
Anqj + anqj υ−
qj
−n
, (8.59)
where
anqj =
N
p=1
∞
m=1
Ampj η
pq
nmj +
Γj d−
j
2
δn,±1 and η
pq
nmj = ηnm Ξpqj , d−
j , d−
j .
(8.60)
The resulting inﬁnite system of linear equations is
2
j=1
κ−
jk Anqj + anqj Rμ−
j
−n
+ κ−
jkanqj Rμ−
j
n
(8.61)
=
2
j=1
κ+
jk Dnqj Rμ+
j
n
+ κ+
jk Dnqj Rμ+
j
−n
;
n = 1, 2, . . . ; q = 1, 2, . . . , N; k = 1, 2, 3, 4.
The solution of the plane strain problem for the cell type model of FRC requires only
minor modiﬁcation of the above formulas; for the details, we refer to [48].
8.3 Effective Stiffness Sensor
In order to get the analytical expression for the effective stiffness tensor C∗ (1.10)
of ﬁbrous composite with anisotropic constituents, we average the local strain and
stress ﬁelds over the RUC, where V = a2 is the cell volume (unit length is assumed
in x3-direction). So,
2V εi j =
⎛
⎝
V0
+
N
q=1 Vq
⎞
⎠ ui, j + u j,i dV, (8.62)
With aid of Gauss’ theorem, we transform the volume integral into surface one:
95.
Multipole Expansion Method in Micromechanics of Composites 191
2V εi j =
Σ
u−
i n j + u−
j ni dS (8.63)
+
N
q=1 Sq
u+
i n j + u+
j ni dS −
Sq
u−
i n j + u−
j ni dS ,
where Σ is the cell outer surface and ni are the components of the unit normal vector.
From the displacement continuity condition and decomposition u− = E · r + u−
f we
get εi j = Ei j ; as expected, E is the macroscopic strain tensor.
The macroscopic stress tensor is written as
V σi j =
V0
σ−
i j dV +
N
q=1 Vq
σ+
i j dV (8.64)
= VC−
i jkl εkl + C+
i jkl − C−
i jkl
N
q=1 Vq
ε+
kldV.
where Vq = πR2 is the volume of qth ﬁber and V0 = ab − NπR2 is the matrix
volume inside the cell: V = V0+ N
q=1Vq. By applying Gauss’ theorem, the integrals
in (8.64) are reduced to
Ikl =
Vq
ε+
kldV =
1
2 Sq
u+
k nl + u+
l nk dS. (8.65)
and can be taken analytically. In the anti-plane shear problem, only the I13 and I23
are non-zero. It is convenient to evaluate the following combination of these two:
I13 + i I23 =
1
2 Sq
w+
q (n1 + in2) dS =
R
2
2π
0
w+
q ρq =R eiϕ
dϕ. (8.66)
Taking account the explicit form of w+
q series expansion at the interface ρq = R
(8.19)
w+
q = 2i
∞
n=1
Im Dnq Rμ+
n
einϕ
+ Rμ+
−n
e−inϕ
, (8.67)
we ﬁnd
I13 + i I23 = −2πRIm D1q/Rμ+ (8.68)
This formula is sufﬁcient for evaluation of the effective moduli C∗
2323, C∗
1313 and
C∗
1323 or, in two-index notation, C∗
44, C∗
55 and C∗
45.
96.
192 V. I. Kushch
The in-plane effective moduli, namely, C∗
11, C∗
22, C∗
12, C∗
16, C∗
26 and C∗
66 are found
byintegratingthestrainandstressﬁeldsfoundfromtheplanestrainproblem.Wehave
I11 =
Vq
ε+
11dV =
1
2 Sq
u+
1 n1dS =
R
2
2π
0
u+
q ρq =R eiϕ
+ e−iϕ
dϕ, (8.69)
where, according to (8.57),
u+
q ρq =R = 2Re
2
j=1
p+
j
∞
n=0
Dnqj Rμ+
j
n
einϕ
+ Rμ+
j
−n
e−inϕ
. (8.70)
Its substitution into (8.69) gives
I11 = 2πRRe
2
j=1
p+
j D1qj Rμ+
j
+ 1/Rμ+ . (8.71)
In the same way, we ﬁnd
I22 = 2πIm
2
j=1
q+
j D1qj Rμ+
j
− 1/Rμ+ . (8.72)
and
I12 = πR
⎡
⎣Re
2
j=1
q+
j D1qj Rμ+
j
+ 1/Rμ+ (8.73)
+ Im
2
j=1
p+
j D1qj Rμ+
j
− 1/Rμ+
⎤
⎦ .
The effective moduli C∗
13, C∗
23, C∗
33 and C∗
36 are found from the generalized plane
strain problem, see [16].
Summary of the Method
Here, we summarize brieﬂy the speciﬁc features of the Multipole Expansion Method.
• The scheme of the method is simple and involves a few mandatory steps. In appli-
cation to the multiple-inclusion problem, they are:
– representation of solution in the multiply-connected domain as the superposition
sum;
97.
Multipole Expansion Method in Micromechanics of Composites 193
– local regular expansion of this sum, with aid of the relevant re-expansion
formulas, in a vicinity of each inclusion;
– fulﬁllment of the interface bonding conditions and thereby reduction of the
boundary value problem to a linear set of algebraic equations;
– numerical solution of the truncated linear system;
– evaluation of the ﬁeld variables and effective properties of composite from the
explicit algebraic formulas.
• Application of the method is case-dependent in the sense that the geometry of
speciﬁc problem dictates the form of partial solutions. In many practically impor-
tant cases, these solutions and their properties are well established. Noteworthy,
with use the appropriate math—vectorial solutions in 3D and complex potentials
in 2D theory—the method appears equally simple for the scalar and vectorial
problems.
• The method gives a complete solution of the boundary value problem including the
local ﬁelds and effective properties. The obtained by this method exact analytical
and numerical results can be regarded as the benchmarks for other, existing or
newly developed, methods of the micromechanics of composites.
• Numerical efﬁciency of the method is high due to the fact that the most work on
solution is done analytically. The computational algorithm includes three simple
steps, namely
– evaluation of the matrix coefﬁcients (minor computational effort),
– iterative solution of the linear system (major computational effort),
– evaluation of the local ﬁelds and effective moduli (negligible effort).
Remarkably, the bigger number of inclusions under study is, the more efﬁcient
becomes the algorithm: on application of the fast multipole scheme to the large-
scale models, the total computational effort scales as O(N).
• Obtained by analytical integration, the exact ﬁnite formulas for the effective prop-
erties involve only the ﬁrst, dipole moments of multipole expansion which can be
found with high accuracy from the small-size truncated linear system.
• The wide opportunities exist for further development of the method, both in terms
of theory and application area. The promising directions include the nano com-
posites, materials with hierarchical or clustered micro structure, composites with
imperfect/debonded interfaces, the multi-scale analysis of steady-state and tran-
sient phenomena, to mention only a few.
References
1. Abramovitz M, Stegun IA (1964) Handbook for mathematical functions. NBS Applied Math-
ematics Series, vol 55. Flammarion, Paris
2. Batchelor GK, O’Brien RW (1977) Thermal of electrical conduction through a granular mate-
rial. Proc R Soc Lond A 355:313–333
3. Bateman G, Erdelyi A (1953) Higher transcendental functions, vol 2. McGraw Hill, New York
98.
194 V. I. Kushch
4. Benveniste Y, Miloh T (2001) Imperfect soft and stiff interfaces in two-dimensional elasticity.
Mech Mater 33:309–323
5. Bonnecaze RT, Brady JF (1991) The effective conductivity of random suspensions of spherical
particles. Proc R Soc Lond A 432:445–465
6. Buryachenko VA, Kushch VI (2006) Effective transverse elastic moduli of composites at non-
dilute concentration of a random ﬁeld of aligned ﬁbers. Z Angew Math Phys (ZAMP) 57:491–
505
7. Buryachenko VA, Pagano NJ, Kim RY, Spowart JE (2003) Quantitative description and numer-
ical simulation of random microstructures of composites and their effective elastic moduli. Int
J Solids Struct 40:47–72
8. Chen HS, Acrivos A (1978) The effective elastic moduli of composite materials containing
spherical inclusions at nondilute concentrations. Int J Solids Struct 14:349–364
9. Chen X, Papathanasiou TD (2004) Interface stress distributions in transversely loaded contin-
uous ﬁber composites: parallel computation in multi-ﬁber RVEs using the boundary element
method. Compos Sci Technol 64:1101–1114
10. Drago A, Pindera MJ (2007) Micro-mechanical analysis of heterogeneous materials: mascro-
scopically homogeneous vs periodic microstructures. Compos Sci Technol 67:1243–1263
11. Duan HL, Wang J, Huang ZP, Karihaloo BL (2005c) Size-dependent effective elastic constants
of solids containing nanoinhomogeneities with interface stress. J Mech Phys Solids 53:1574–
1596
12. Dundurs J (1969) Discussion of a paper by D.B. Bogy. ASME J Appl Mech 36:650–652
13. Erofeenko VN (1989) Addition theorems. Nauka i Tekhnika, Minsk
14. Eshelby JD (1959) The elastic ﬁeld outside the ellipsoidal inclusion. Proc R Soc Lond A
252:561–569
15. Golovchan VT (1981) On effective thermal conductivity of granular media. Eng Phys J 40:336–
344
16. Golovchan VT (1982) Elastic characteristics of composite with anisotropic matrix and ﬁbers.
2. Generalized plane strain. Mekhanika kompozitnyh materialov 18:394–399
17. Golovchan VT, Guz AN, Kohanenko YuV, Kushch VI (1993) Mechanics of composites (in 12
vol) vol 1. Statics of materials. Naukova dumka, Kiev
18. Greengard L (1994) Fast algorithms for classical physics. Science 265:909–914
19. Greengard L, Rokhlin V (1997) A new version of the fast multipole method for the Laplace
equation in three dimensions. Acta Numer 6:229–269
20. Gurtin ME (1972) The linear theory of elasticity. Springer, Berlin
21. Hasimoto H (1959) On the periodic fundamental solutions of the Stokes equations and their
application to viscous ﬂow past a cubic array of spheres. J Fluid Mech 5:317–328
22. Helsing J (1995) An integral equation method for elastostatics of periodic composites. J Mech
Phys Solids 43:815–828
23. Hobson EW (1931) The theory of spherical and ellipsoidal harmonics. Cambridge University
Press, Cambridge
24. Horii H, Nemat-Nasser S (1985) Elastic ﬁeld of interacting inhomogeneities. Int J Solids Struct
21:731–745
25. http://scienceworld.wolfram.com/physics/MultipoleExpansion.html
26. Jeffrey DJ (1973) Conduction through a random suspension of spheres. Proc R Soc Lond A
335:355–367
27. Kantorovich LV, Krylov VI (1964) Approximate methods of higher analysis. Wiley, New York
28. Kunin IA, Sosnina EG (1971) Ellipsoidal inhomogeneity in elastic solid. DAN USSR 199:103–
109
29. Kushch VI, Artemenko OG (1983) Temperature ﬁeld evaluation in particle composite layer.
Doklady AN UrkSSR Ser A N3:74–77
30. Kushch VI (1985) Elastic equilibrium of a medium containing periodic spherical inclusions.
Soviet Appl Mech 21:435–442
31. Kushch VI (1987) Computation of the effective elastic moduli of a granular composite material
of regular structure. Soviet Appl Mech 23:362–365
99.
Multipole Expansion Method in Micromechanics of Composites 195
32. Kushch VI (1994) Thermal conductivity of a composite material reinforced by periodically
distributed spheroidal particles. Eng Phys J 66:497–504
33. Kushch VI (1995) Addition theorems for partial vectorial solutions of Lame equation in spher-
oidal basis. Int Appl Mech 31(2):86–92
34. Kushch VI (1996) Elastic equilibrium of a medium containing ﬁnite number of aligned spher-
oidal inclusions. Int J Solids Struct 33:1175–1189
35. Kushch VI (1997) Conductivity of a periodic particle composite with transversely isotropic
phases. Proc R Soc Lond A 453:65–76
36. Kushch VI (1997) Microstresses and effective elastic moduli of a solid reinforced by periodi-
cally distributed spheroidal inclusions. Int J Solids Struct 34:1353–1366
37. Kushch VI (1998) The stress state and effective thermoelastic properties of piece homogeneous
solids with spheroidal interfaces. Dr Sci Thesis, Kiev
38. Kushch VI (1998) Interacting cracks and inclusions in a solid by the multipole expansion
method. Int J Solids Struct 35:1187–1198
39. Kushch VI (1998) Elastic equilibrium of a solid containing a ﬁnite number of arbitrary oriented
spheroidal inclusions. Int J Solids Struct 35:1187–1198
40. Kushch VI, Sangani AS (2000) Conductivity of a composite containing uniformly oriented
penny-shaped cracks or perfectly conducting inclusions. Proc R Soc Lond A 456:683–699
41. Kushch VI, Sangani AS (2000) Stress intensity factor and effective stiffness of a solid contained
aligned penny-shaped cracks. Int J Solids Struct 37:6555–6570
42. Kushch VI, Sangani AS, Spelt PDM, Koch DL (2002) Finite Weber number motion of bubbles
through a nearly inviscid liquid. J Fluid Mech 460:241–280
43. Kushch VI (2003) Stress concentration in the particulate composite with transversely isotropic
phases. Int J Solids Struct 40:6369–6388
44. Kushch VI, Sevostianov I (2004) Effective elastic properties of the particulate composite with
transversely isotropic phases. Int J Solids Struct 41:885–906
45. Kushch VI, Shmegera SV, Buryachenko VA (2005) Interacting elliptic inclusions by the method
of complex potentials. Int J Solids Struct 42:5491–5512
46. Kushch VI, Shmegera SV, Buryachenko VA (2006) Elastic equilibrium of a half plane contain-
ing a ﬁnite array of elliptic inclusions. Int J Solids Struct 43:3459–3483
47. Kushch VI, Shmegera SV, Mishnaevsky L Jr (2008) Meso cell model of ﬁber reinforced com-
posite: interface stress statistics and debonding paths. Int J Solids Struct 45:2758–2784
48. Kushch VI, Shmegera SV, Mishnaevsky L Jr (2008) Stress concentration and effective stiffness
of aligned ﬁber reinforced composite with anisotropic constituents. Int J Solids Struct 45:5103–
5117
49. Kushch VI, Shmegera SV, Sevostianov I (2009) SIF statistics in micro cracked solid: effect of
crack density, orientation and clustering. Int J Eng Sci 47:192–208
50. Kushch VI, Sevostianov I, Mishnaevsky L Jr (2009) Effect of crack orientation statistics on
effective stiffness of mircocracked solid. Int J Solids Struct 46:1574–1588
51. Kushch VI, Shmegera SV, Mishnaevsky L Jr (2010) Elastic interaction of partially debonded
circular inclusions. I. Theoretical solution. Int J Solids Struct 47:1961–1971
52. Kushch VI (2010) Transverse conductivity of unidirectional ﬁbrous composite with interface
arc cracks. Int J Eng Sci 48:343–356
53. Kushch VI, Shmegera SV, Mishnaevsky L Jr (2010) Elastic interaction of partially debonded
circular inclusions. II. Application to ﬁbrous composite. Int J Solids Struct (submitted)
54. Kushch VI, Mogilevskaya SG, Stolarski H, Crouch S (2011) Elastic interaction of spherical
nanoinhomogeneities with Gurtin-Murdoch type interfaces. J Mech Phys Solids (submitted)
55. Lekhnitsky SG (1963) Theory of elasticity of an anisotropic elastic body. Holden-Day, San
Francisco
56. Lu S-Y, Kim S (1990) Effective thermal conductivity of composites containing spheroidal
inclusions. AIChE J 36:927–938
57. Maxwell JC (1873) A treatise on electricity and magnetism, vol 1. Clarendon Press, Oxford
58. McCartney LN, Kelly A (2008) Maxwell’s far-ﬁeld methodology applied to the prediction of
properties of multi-phase isotropic particulate composites. Proc R Soc A 464:423–446
100.
196 V. I. Kushch
59. McPhedran RC, McKenzie DR (1978) The conductivity of lattices of spheres. 1. The simple
cubic lattice. Proc R Soc Lond A 359:45–63
60. McKenzie DR, McPhedran RC, Derrick GH (1978) The conductivity of lattices of spheres. II.
The body-centered and face-centered cubic lattices. Proc R Soc Lond A 362:211–232
61. Meisner MJ, Kouris DA (1995) Interaction of two elliptic inclusions. Int J Solids Struct 32:451–
466
62. Milne-Thomson LM (1960) Plane elastic systems. Springer, Berlin
63. Mogilevskaya SG, Kushch VI, Koroteeva O, Crouch SL (2011) Equivalent inhomogeneity
method for evaluating the effective conductivities of isotropic particulate composites. J Mech
Mater Struct (submitted)
64. Morse PM, Feshbach H (1953) Methods of theoretical physics. McGraw-Hill, New York
65. Movchan AB, Nicorovici NA, McPhedran RC (1997) Green’s tensors and lattice sums for
elastostatics and elastodynamics. Proc R Soc Lond A 453:643–662
66. Mura T (1982) Micromechanics of defects in solids. Martinus Nijhoff, Netherlands
67. MuskhelishviliNI(1953)Somebasicproblemsofthemathematicaltheoryofelasticity.Gronin-
gen, P. Noordhoff, Holland
68. Nemat-Nasser S, Iwakuma T, Hejazi M (1982) On composites with periodic structure. Mech
Mater 1:239–267
69. Perrins WT, McKenzie DR, McPhedran RC (1979) Transport properties of regular arrays of
cylinders. Proc R Soc Lond Ser A 369:207–225
70. Podil’chuk YuN (1984) The boundary value problems of statics of elastic solid. Naukova
Dumka, Kiev
71. Poladian L, McPhedran RC (1986) Effective transport properties of periodic composite mate-
rials. Proc R Soc Lond A 408:45–59
72. Rahman M, Michelitsch T (2007) A general procedure for solving boundary-value problems
of elastostatics for a spherical geometry based on Love’s approach. Quart J Mech Appl Math
60:139–160
73. Rayleigh L (1892) On the inﬂuence of obstacles arranged in rectangular order on the properties
of a medium. Phil Mag E 34:481–502
74. Russel WB, Acrivos A (1972) On the effective moduli of composite materials: slender rigid
inclusions at dilute concentrations. J Appl Math Phys (ZAMP) 23:434–464
75. Sangani AS, Acrivos A (1983) The effective conductivity of a periodic array of spheres. Proc
R Soc Lond A 386:263
76. Sangani AS, Lu W (1987) Elastic coefﬁcients of composites containing spherical inclusions in
a periodic array. J Mech Phys Solids 35:1–21
77. Sangani AS, Mo G (1996) An O(N) algorithm for stokes and Laplace interactions of particles.
Phys Fluids 8:1990–2009
78. Sangani AS, Mo G (1997) Elastic interactions in particulate composite with perfect as well as
imperfect interfaces. J Mech Phys Solids 45:2001–2031
79. Sangani AS, Yao C (1988) Bulk thermal conductivity of composites with spherical inclusions.
J Appl Phys 63:1334–1341
80. Sevostianov I, Yilmaz N, Kushch V, Levin V (2005) Effective elastic properties of matrix
composites with transversely-isotropic phases. Int J Solids Struct 42:455–476
81. Slobodyansky MG (1954) The general forms of solution of elasticity equations for single con-
nectedandmultiply-connecteddomainsexpressedthroughtheharmonicfunctions.Prikladnaya
matematika i mehanika 18:55–74
82. Suen WM, Wong SP, Young K (1979) The lattice model of heat conduction in a composite
material. J Phys D 12:1325–1338
83. Torquato S (2002) Random heterogeneous materials: microstructure and macroscopic proper-
ties. Springer, New York
84. Toya M (1974) A crack along interface of a circular inclusion embedded in an inﬁnite solid. J
Mech Phys Solids 22:325–348
85. Tsai SW (1988) Composites design, 4th edn. Think Composites, Dayton
101.
Multipole Expansion Method in Micromechanics of Composites 197
86. Yardley JG, McPhedran RC, Nicorovici NA, Botten LC (1999) Addition formulas and the
Rayleigh identity for arrays of elliptical cylinders. Phys Rev E 60:6068–6080
87. Yardley JG, Reuben AJ, McPhedran RC (2001) The transport properties of layers of elliptical
cylinreds. Proc R Soc Lond A 457:395–423
88. Zinchenko AZ (1994) An efﬁcient algorithm for calculating multiparticle interaction in a con-
centrated dispersion of spheres. J Comput Phys 111:120–135
89. Zinchenko AZ (1994) Algorithm for random close packing of spheres with periodic boundary
conditions. J Comput Phys 114:298–315
90. Zuzovski M, Brenner H (1977) Effective conductivities of composite materials composed of
cubic arrangements of spherical particles embedded in an isotropic matrix. Z Agnew Math
Phys (ZAMP) 28:979–992
Be the first to comment